Your SlideShare is downloading.
×

×

Saving this for later?
Get the SlideShare app to save on your phone or tablet. Read anywhere, anytime – even offline.

Text the download link to your phone

Standard text messaging rates apply

Like this document? Why not share!

- Advanced Mechanics of Materials by ... by Muhammad Abdullah... 900 views
- Solution manual mechanics of material by Marhaini Mazelan 81932 views
- Mechanical behavior of materials do... by Jeong-Gyu Lee 1137 views
- Introduction to-mechanics-of-materi... by Stephen Siwila 1809 views
- solution-manual-3rd-ed-metal-formi... by dean129 12852 views
- Mechanics of materials 5th edition ... by Rohith Reddy 10033 views
- Manufacturing Processes for Enginee... by Ayesha FaÐ¯ooq 14609 views
- Introduction to-mechanics-of-materi... by Stephen Siwila 1820 views
- Advances mechanics of_materials_6th... by Tarapong Pata 14951 views
- Mechanical Properties of Metals by guesteed04b 19521 views
- Advanced Mechanics of Materials, 6t... by LK Education 21088 views
- Mechanical engineering principles by goldenakos 36755 views

Like this? Share it with your network
Share

No Downloads

Total Views

13,458

On Slideshare

0

From Embeds

0

Number of Embeds

0

Shares

0

Downloads

2,598

Comments

0

Likes

7

No embeds

No notes for slide

- 1. This page intentionally left blank
- 2. MECHANICAL BEHAVIOR OF MATERIALSThe term mechanical behavior encompasses the response of materials to external forces.This text considers a wide range of topics, including mechanical testing to determinematerial properties, plasticity needed for FEM analyses of automobile crashes, meansof altering mechanical properties, and treatment of several modes of failure. This textﬁts courses on mechanical behavior of materials taught in departments of mechanicalengineering and materials science. It includes numerous examples and problems forstudent practice and emphasizes quantitative problem solving. End of chapter notes areincluded to increase students’ interest.W. F. Hosford is Professor Emeritus of Materials Science and Engineering at the Uni-versity of Michigan. He is the author of a number of books, including Metal Forming:Mechanics and Metallurgy, 2nd ed. (with R. M. Caddell), Mechanics of Crystals andTextured Polycrystals, and Mechanical Metallurgy.
- 3. Mechanical Behavior of Materials WILLIAM F. HOSFORD University of Michigan
- 4. Cambridge, New York, Melbourne, Madrid, Cape Town, Singapore, São PauloCambridge University PressThe Edinburgh Building, Cambridge , UKPublished in the United States of America by Cambridge University Press, New Yorkwww.cambridge.orgInformation on this title: www.cambridge.org/9780521846707© Cambridge University Press 2005This publication is in copyright. Subject to statutory exception and to the provision ofrelevant collective licensing agreements, no reproduction of any part may take placewithout the written permission of Cambridge University Press.First published in print format 2005- ---- eBook (NetLibrary)- --- eBook (NetLibrary)- ---- hardback- --- hardbackCambridge University Press has no responsibility for the persistence or accuracy of sfor external or third-party internet websites referred to in this publication, and does notguarantee that any content on such websites is, or will remain, accurate or appropriate.
- 5. ContentsPreface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . page xvNote to the Reader . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xix 1 Stress and Strain . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction 1 Stress 2 Sign Convention 3 Transformation of Axes 4 Principal Stresses 6 Mohr’s Stress Circles 6 Strains 9 Small Strains 11 Transformation of Axes 12 Mohr’s Strain Circles 14 Force and Moment Balances 15 Boundary Conditions 16 Note 17 Problems 18 2 Elasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21 Introduction 21 Isotropic Elasticity 21 Variation of Young’s Modulus 24 Isotropic Thermal Expansion 26 Anisotropic Elasticity 27 Orientation Dependence of Elastic Response 29 Orientation Dependence in Cubic Crystals 31 Orientation Dependence in Noncubic Crystals 32 v
- 6. vi CONTENTS Orientation Dependence in Materials Other Than Single Crystals 34 Anisotropic Thermal Expansion 34 Notes 35 References 36 Problems 36 3 Tensile Testing. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 39 Introduction 39 Tensile Specimens 39 Stress–Strain Curves 40 Ductility 43 True Stress and Strain 44 The Bridgman Correction 45 Temperature Rise 47 Sheet Anisotropy 47 Measurement of Force and Strain 48 Axial Alignment 49 Special Problems 49 Notes 50 References 51 Problems 51 4 Other Tests of Plastic Behavior . . . . . . . . . . . . . . . . . . . . . . . . . . 53 Introduction 53 Compression Test 53 Plane-Strain Compression 56 Plane-Strain Tension 57 Biaxial Tension (Hydraulic Bulge Test) 57 Torsion Test 59 Bend Tests 61 Hardness Tests 62 Mutual Indentation Hardness 66 Note 67 References 67 Problems 67 5 Strain-Hardening of Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 70 Introduction 70 Mathematical Approximations 70 Power-Law Approximation 72 Necking 73 Work per Volume 75 Localization of Strain at Defects 75 Notes 76 Problems 77
- 7. CONTENTS vii6 Plasticity Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 80 Introduction 80 Yield Criteria 80 Tresca Maximum Shear Stress Criterion 81 Von Mises Criterion 82 Flow Rules 84 Principle of Normality 85 Effective Stress and Effective Strain 86 Other Isotropic Yield Criteria 89 Anisotropic Plasticity 90 Effect of Strain-Hardening on the Yield Locus 93 Notes 93 References 94 Problems 947 Strain-Rate and Temperature Dependence of Flow Stress . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 99 Introduction 99 Strain-Rate Dependence of Flow Stress 99 Superplasticity 102 Combined Strain and Strain-Rate Effects 106 Strain-Rate Sensitivity of bcc Metals 107 Temperature Dependence 110 Combined Temperature and Strain-Rate Effects 111 Hot Working 115 Notes 116 References 116 Problems 1168 Slip . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 120 Introduction 120 Slip Systems 120 Schmid’s Law 121 Strains Produced by Slip 123 Strain-Hardening of fcc Single Crystals 125 Tensile Deformation of fcc Crystals 126 Slip in bcc Crystals 128 Slip in hcp Crystals 128 Lattice Rotation in Tension 129
- 8. viii CONTENTS Lattice Rotation in Compression 131 Texture Formation in Polycrystals 132 Approximate Calculation of R-Values 133 Notes 134 References 135 Problems 135 9 Dislocation Geometry and Energy . . . . . . . . . . . . . . . . . . . . . 139 Introduction 139 Theoretical Strength of Crystals 139 The Nature of Dislocations 141 Burgers Vectors 142 Energy of a Screw Dislocation 144 Reactions between Parallel Dislocations and Frank’s Rule 146 Stress Fields around Dislocations 147 Forces on Dislocations 149 Partial Dislocations in fcc Crystals 150 Stacking Faults 151 Notes 154 References 154 Problems 15610 Dislocation Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 158 Introduction 158 Frank–Read Sources 158 Dislocation Pile-Ups 161 Cross-Slip 161 Dislocation Intersections 163 Climb 166 Notes 166 References 167 Problems 16711 Mechanical Twinning and Martensitic Shear . . . . . . . . . . . 170 Introduction 171 Formal Notation 171 Twinning Shear 172 Twinning in fcc Metals 173 Twinning in bcc Metals 173 Twinning in hcp Metals 175 Shapes of Twins 178 Mechanism of Twinning 179 Martensite Transformation 182 Shape Memory and Superelasticity 183
- 9. CONTENTS ix Notes 184 References 185 Problems 18612 Hardening Mechanisms in Metals . . . . . . . . . . . . . . . . . . . . . . 188 Introduction 188 Deformation of Polycrystals 188 Texture Strengthening 190 Crystal Structure 191 Grain Size 193 Strain-Hardening 194 Solid-Solution Strengthening 195 Dispersion Strengthening 196 Yield Points and Strain-Aging 199 Dynamic Strain-Aging 201 Combined Effects 202 Notes 206 References 206 Problems 20613 Ductility and Fracture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210 Introduction 210 Ductile Fracture 212 Brittle Fracture 217 Impact Energy 220 Notes 224 References 224 Problems 22514 Fracture Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 227 Introduction 227 Theoretical Fracture Strength 227 Stress Concentration 229 Grifﬁth Theory 230 Orowan Theory 231 Fracture Modes 231 Irwin’s Fracture Analysis 231 Plastic Zone Size 233 Thin Sheets 235 Temperature and Loading Rate 236 Metallurgical Variables 237 Fracture Mechanics in Design 237 Compact Tensile Specimens 239 Strain-Energy Release 240 The J-integral 241
- 10. x CONTENTS Notes 242 References 243 Problems 243 Appendix I 245 Size and Shape of the Plastic Zone at a Crack Tip 24515 Viscoelasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 247 Introduction 247 Rheological Models 247 Series Combination of a Spring and Dashpot 248 Parallel Combination of a Spring and Dashpot 249 Combined Parallel–Series Model 250 More Complex Models 251 Damping 251 Natural Decay 253 Elastic Modulus – Relaxed Versus Unrelaxed 254 Thermoelastic Effect 255 Snoek Effect in bcc Metals 256 Other Damping Mechanisms 257 References 258 Notes 258 Problems 25916 Creep and Stress Rupture. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 262 Introduction 262 Creep Mechanisms 262 Temperature Dependence of Creep 266 Deformation Mechanism Maps 267 Cavitation 268 Rupture Versus Creep 269 Extrapolation Schemes 270 Alloys for High-Temperature Use 273 Notes 275 References 275 Problems 27617 Fatigue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 279 Introduction 279 Surface Observations 279 Nomenclature 281 S–N Curves 282
- 11. CONTENTS xi Effect of Mean Stress 283 The Palmgren–Miner Rule 285 Stress Concentration 286 Surfaces 288 Design Estimates 290 Metallurgical Variables 291 Strains to Failure 291 Crack Propagation 294 Cyclic Stress–Strain Behavior 296 Temperature and Cycling Rate Effects 297 Fatigue of Polymers 300 Fatigue Testing 302 Design Considerations 302 Summary 303 Notes 303 References 304 Problems 30418 Residual Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 308 Introduction 308 Small-Scale Stresses 308 Bauschinger Effect 311 Nonuniform Cooling 312 Nonuniform Material 313 Stresses from Welding 313 Stresses from Mechanical Working 314 Consequences of Residual Stresses 316 Measurement of Residual Stresses 317 Relief of Residual Stresses 319 Notes 321 References 321 Problems 32119 Ceramics and Glasses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 324 Introduction 324 Elastic Properties 324 Slip Systems 325 Hardness 326 Weibull Analysis 326 Testing 329 Porosity 329 High-Temperature Behavior 331 Fracture Toughness 331 Toughening of Ceramics 334
- 12. xii CONTENTS Fatigue 335 Silicate Glasses 335 Strength of Glasses 338 Thermally Induced Stresses 339 Delayed Fracture 340 Glassy Metals 341 Notes 342 References 343 Problems 34320 Polymers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 345 Introduction 345 Elastic Behavior 345 Rubber Elasticity 350 Damping 353 Yielding 353 Effect of Strain Rate 356 Effect of Pressure 356 Crazing 361 Yielding of Fibers in Compression 363 Fracture 364 Deformation Mechanism Maps 366 Shape-Memory Effect 367 References 368 Notes 368 Problems 37021 Composites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 372 Introduction 372 Fiber-Reinforced Composites 372 Elastic Properties of Fiber-Reinforced Composites 372 Strength of Fiber-Reinforced Composites 376 Volume Fraction of Fibers 377 Orientation Dependence of Strength 378 Fiber Length 379 Failures with Discontinuous Fibers 381 Failure under Compression 382 Typical Properties 383 Particulate Composites 384 Brick-Wall Model 385 Lamellar Composites 387 Notes 388 References 389 Problems 389
- 13. CONTENTS xiii22 Mechanical Working . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 392 Introduction 392 Bulk-Forming Energy Balance 392 Deformation Zone Geometry 396 Friction in Bulk Forming 399 Formability 400 Deep Drawing 401 Stamping 403 Notes 407 References 409 Problems 409Appendix A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 413Appendix B . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 418Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 421
- 14. PrefaceThe term “mechanical behavior” encompasses the response of materials to externalforces. This text considers a wide range of topics. These include mechanical testing todetermine material properties, plasticity for FEM analyses of automobile crashes, meansof altering mechanical properties, and treatment of several modes of failure. The two principal responses of materials to external forces are deformation and frac-ture. The deformation may be elastic, viscoelastic (time-dependent elastic deformation),plastic, or creep (time-dependent plastic deformation). Fracture may occur suddenly orafter repeated application of loads (fatigue). For some materials, failure is time-dependent. Both deformation and fracture are sensitive to defects, temperature, and rateof loading. The key to understanding these phenomena is a basic knowledge of the three-dimensional nature of stress and strain and common boundary conditions, which arecovered in the ﬁrst chapter. Chapter 2 covers elasticity, including thermal expansion.Chapters 3 and 4 treat mechanical testing. Chapter 5 is focused on mathematical approx-imations to stress–strain behavior of metals and how these approximations can be usedto understand the effect of defects on strain distribution in the presence of defects. Yieldcriteria and ﬂow rules are covered in Chapter 6. Their interplay is emphasized in prob-lem solving. Chapter 7 treats temperature and strain-rate effects and uses an Arrheniusapproach to relate them. Defect analysis is used to understand superplasticity as well asstrain distribution. Chapter 8 is devoted to the role of slip as a deformation mechanism. The tensornature of stresses and strains is used to generalize Schmid’s law. Lattice rotations causedby slip are covered. Chapters 9 and 10 treat dislocations: their geometry, movement, andinteractions. There is a treatment of stacking faults in fcc metals and how they affectstrain-hardening. Hardening by intersections of dislocations is emphasized. Chapter 11treats the various hardening mechanisms in metallic materials. Mechanical twinning iscovered in Chapter 12. Chapter 13 presents a phenomenological and qualitative treatment of ductility, andChapter 14 focuses on quantitative coverage of fracture mechanics. Viscoelasticity (time-dependent elasticity) is treated in Chapter 15. Mathematicalmodels are presented and used to explain stress and strain relaxation as well as damping xv
- 15. xvi PREFACEand rate dependence of the elastic modulus. Several mechanisms of damping are pre-sented. Chapter 16 is devoted to creep (time-dependent plasticity) and stress rupture. Thecoverage includes creep mechanisms and extrapolation techniques for predicting life. Failure by fatigue is the topic of Chapter 17. The chapter starts with a phenomenolog-ical treatment of the S–N curve and the effects of mean stress, variable stress amplitude,and surface condition. The important material aspects, Cofﬁn’s law, and the crack prop-agation rate are treated. Chapter 18 covers residual stresses and their origins, effects,measurement, and removal. Chapters 19, 20, and 21 cover ceramics, polymers, and composites. Separate chaptersare devoted to these materials because their mechanical behavior is very different fromthat of metals, which were emphasized in the earlier chapters. Because ceramics and glassare brittle and their properties are variable, Weibul analysis is presented here. Chapter 19also covers methods of improving toughness of ceramics and the role of thermally inducedstresses. The most important aspect of the mechanical behavior of polymers is their greattime dependence and the associated temperature dependence. The effects of pressureon yielding and the phenomenon of crazing are also unique. Rubber elasticity is verydifferent from Hookean elasticity. Composites may be divided into ﬁber, sheet, andparticulate composites. With ﬁber-reinforced composites, the orientation and length ofthe ﬁbers control properties. The volume fraction of the stronger, stiffer phase controlsthe overall properties of all composites. The ﬁnal chapter on metal forming analyzes bulk-forming and sheet-forming oper-ations. This text differs from other books on mechanical behavior in several aspects. Thetreatment of plasticity has a greater emphasis on the interrelationship of the ﬂow, effec-tive strain, and effective stress and their use in conjunction with yield criteria to solveproblems. The treatment of defects is new. Schmid’s law is generalized for complex stressstates. Its use with strains allows prediction of R-values for textures. Another feature is thetreatment of lattice rotations and how they lead to deformation textures. Most texts treatonly strain relaxation and neglect stress relaxation. The chapter on fracture mechanicsincludes Gurney’s approach. Most books omit any coverage of residual stresses. Muchof the analysis of particulate composites is new. Few books include anything on metalforming. Throughout this book, more emphasis is placed on quantitative problem-solvingthan in most other books. The notes at the ends of the chapters are included to increasereader interest in the subject. As a consequence of the increased coverage in these areas, the treatment of someother topics is not as extensive as in competing books. There is less coverage of fatiguefailure and fracture mechanics. This book may contain more material than can be covered in a single course. Depend-ing on the focus of the course, various chapters or portions of chapters may be omitted.It is hoped that this book will be of value to mechanical engineers as well as materialsengineers. If the book is used in a mechanical engineering course, the instructor maywish to skip some chapters. In particular, Chapters 8 through 11 may be omitted. If thebook is used in a materials science course, the instructor may wish to omit Chapters 10,18, and 22. Both may wish to skip Chapter 11 on twinning and memory metals. Even
- 16. PREFACE xviithough it was realized that most users may wish to skip this chapter, it was included forcompleteness and in the hope that it may prove useful as a reference. It is assumed that the students who use this book have had both an introductory mate-rials science course and a “strength of materials” course. From the strength of materialscourse, they can be expected to know basic concepts of stress and strain, how to resolvestresses from one axis system to another, and how to use Hooke’s laws in three dimensions.They should be familiar with force and moment balances. From the materials sciencecourse, they should have acquired the understanding that most materials are crystallineand that crystalline materials deform by slip as a result of the movement of dislocations.They should also be familiar with such concepts as substitutional and interstitial solidsolutions and diffusion. Appendices A (Miller Indices) and B (Stereographic Projection)are available for students not familiar with these topics. W. F. Hosford Ann Arbor, Michigan
- 17. Note to the ReaderEngineers who design products should understand how materials respond to appliedstresses and strains to avoid unexpected deﬂection, deformation, and failure. Understand-ing material behavior is also essential for shaping material, improving the mechanicalbehavior of materials for speciﬁc applications, and failure analysis. Some engineers have many misconceptions about the mechanical behavior of mate-rials. The following statements are typical:This spring isn’t stiff enough. We should use a harder steel.Perhaps a stronger steel would make a tougher pipeline. If something breaks, use a strongermaterial.This tungsten wire isn’t ductile enough. Let’s anneal it at a higher temperature.We are having too many fatigue failures. We’d get a longer life if we used a tougher grade of steel.I know that you are having trouble with the bar splitting when you roll it. Maybe you could roll itwithout having it split if you “babied” it by using a series of lighter reductions.If there is a strain in the x-direction, there must be a stress in the x-direction. Where there’s smoke,there’s ﬁre!Under rapid loading, a material that is very sensitive to the strain rate will have less ductility thana material that is insensitive to stain rate.Residual stresses in the glaze of pottery can be prevented by slow cooling after annealing.The fact that the stained glass windows in old European cathedrals are thicker at the bottom thanat the top is proof that glass creeps at room temperature.Since decreasing grain size increases strength, ﬁne-grained materials should creep more slowlythan coarse grain materials.A ductile, annealed sheet of aluminum should have a greater formability in can making than acold-worked sheet of aluminum.The presence of dislocations explains why the yield strengths of crystals are much lower thantheory predicts. Therefore, the strength should drop as the number of dislocations increases andmetals strain-harden as dislocations leave the surface, decreasing the number of dislocations leftin the crystal. xix
- 18. xx NOTE TO THE READERWe know that steel is brittle at low temperatures. Aluminum must be too.If the ductile–brittle transition temperature of a steel is −10◦ F, it won’t fail brittly above thattemperature.To increase the uniformity of deformation in the drawing of wire, we should use a large numberof very light passes rather than a few passes of heavy reduction.Since the reduction of area in a tension test is 55%, we cannot expect to roll the material to areduction greater than 55% without cracking.A cold-worked metal can be made almost isotropic by heating it so that it recrystallizes. All of these statements are incorrect. They are examples of incomplete understandingof the mechanical behavior of materials. It is to be hoped that this book will clear upthese misconceptions.
- 19. 1 Stress and StrainIntroductionThis book is concerned with the mechanical behavior of materials. The term mechanicalbehavior refers to the response of materials to forces. Under load, a material may eitherdeform or break. The factors that govern a material’s resistance to deformation are verydifferent from those governing its resistance to fracture. The word strength may refereither to the stress required to deform a material or to the stress required to cause fracture;therefore, care must be used with the term strength. When a material deforms under small stresses, the deformation may be elastic. Inthis case, when the stress is removed, the material will revert to its original shape. Mostof the elastic deformation will recover immediately. There may be, however, some time-dependent shape recovery. This time-dependent elastic behavior is called anelastic orviscoelastic. Larger stresses may cause plastic deformation. After a material undergoes plasticdeformation, it will not revert to its original shape when the stress is removed. Usually,high resistance to deformation is desirable, so that a part will maintain its shape in servicewhen stressed. On the other hand, it is desirable to have materials deform easily whenthey are being formed by rolling, extrusion, or other methods. Plastic deformation usuallyoccurs as soon as the stress is applied. At high temperatures, however, time-dependentplastic deformation called creep may occur. Fracture is the breaking of a material into two or more pieces. If fracture occurs beforemuch plastic deformation occurs, we say that the material is brittle. In contrast, if therehas been extensive plastic deformation preceding fracture, the material is consideredductile. Fracture usually occurs as soon as a critical stress has been reached; however,repeated applications of a somewhat lower stress may cause fracture. This is calledfatigue. The amount of deformation that a material undergoes is described by strain. Theforces acting on a body are described by stress. Although the reader should already befamiliar with these terms, they will be reviewed in this chapter. 1
- 20. 2 MECHANICAL BEHAVIOR OF MATERIALSStressStress, σ , is deﬁned as the intensity of force at a point: σ = ∂ F/∂ A as ∂ A → 0. (1.1a)If the state of stress is the same everywhere in a body, σ = F/A. (1.1b) A normal stress (compressive or tensile) is one in which the force is normal to thearea on which it acts. With a shear stress, the force is parallel to the area on which itacts. Two subscripts are required to deﬁne a stress. The ﬁrst subscript denotes the normalto the plane on which the force acts and the second subscript identiﬁes the direction ofthe force. * For example, a tensile stress in the x-direction is denoted by σx x , indicatingthat the force is in the x-direction and it acts on a plane normal to x. For a shear stress,σx y , a force in the y-direction acts on a plane normal to x. Because stresses involve both forces and areas, they are not vector quantities. Ninecomponents of stress are needed to describe a state of stressfully at a point, as shownin Figure 1.1. The stress component σ yy = Fy /A y describes the tensile stress in they-direction. The stress component σzy = Fy /A z is the shear stress caused by a shearforce in the y-direction acting on a plane normal to z. Repeated subscripts denote normal stresses (e.g., σ xx , σ yy , . . . ) whereas mixed sub-scripts denote shear stresses (e.g., σ xy , σ zx , . . . ). In tensor notation the state of stress isexpressed as σx x σ yx σzx σi j = σx y σ yy σzy , (1.2) σx z σ yz σzzwhere i and j are iterated over x, y, and z. Except where tensor notation is required, it isoften simpler to use a single subscript for a normal stress and to denote a shear stress byτ ; for example, σx ≡ σx x and τx y ≡ σx y . (1.3) A stress component expressed along one set of axes may be expressed along anotherset of axes. Consider the case in Figure 1.2. The body is subjected to a stress σ yy = Fy /Ay .It is possible to calculate the stress acting on a plane whose normal, y , is at an angle θto y. The normal force acting on the plane is Fy = Fy cos θ and the area normal to y isAy /cos θ, so σ y = σ y y = Fy /A y = (Fy cos θ)/(A y / cos θ) = σ y cos2 θ. (1.4a)* Use of the opposite convention should cause no confusion because σ ij = σ ji .
- 21. STRESS AND STRAIN 3 z y′ σzz y Fy σzy σzx σyz Ay′ Fy′ σxz σyy σxy σyx σxx y θ Fx′ x x x′Figure 1.1. The nine components of stress acting on Figure 1.2. Stresses acting on an area, A , under aan inﬁnitesimal element. The normal stress compo- normal force, Fy . The normal stress σ y y = F y /A y =nents are σ xx , σ yy , and σ zz . The shear stress compo- Fy cos θ /(Ay /cos θ) = σ yy cos2 θ. The shear stress τ y xnents are σ yz , σ zx , σ xy , σ zy , σ xz , and σ yx . = Fx /A y = Fy sin θ /(Ayx /cos θ) = σ yy cos θ sin θ.Similarly, the shear stress on this plane acting in the x -direction, τ y x (= σ y x ), is givenby τ y x = σ y x = Fx /A y = (Fy sin θ)/(A y / cos θ) = σ y cos θ sin θ. (1.4b)Note: The transformation requires the product of two cosine and/or sine terms.Sign convention. When we write σ ij = Fi /Aj , the term σ ij is positive if either i and j areboth positive or both negative. On the other hand, the stress component is negative for acombination of i and j in which one is positive and the other is negative. For example, inFigure 1.3 the terms σ xx are positive on both sides of the element, because both the forceand the normal to the area are negative on the left and positive on the right. The stressτ yx is negative because on the top surface the normal to the area, y, is positive and thex-direction force is negative, and on the bottom surface the x-direction force is positiveand y is negative. Similarly, τ xy is negative. Pairs of shear stress terms with reversed subscripts are always equal. A momentbalance requires that τ ij = τ ji . If they weren’t, equal, the element would undergo anFigure 1.3. The normal stress, σ xx , is τyx < 0positive because the direction of theforce, Fx , and the normal to the plane areeither both positive (right) or both nega- ytive (left). The shear stresses, τ xy and τ yx , σxx > 0are negative because the direction of theforce and the normal to the plane have τxy < 0opposite signs. x
- 22. 4 MECHANICAL BEHAVIOR OF MATERIALS τxy z z’τyx y’ τyx y A x’ τxy xFigure 1.4. An inﬁnitesimal element under shear Figure 1.5. Two orthogonal coordinate systems, x,stresses τ xy and τ yx . A moment balance about A re- y, and z and x , y , and z . The stress state may bequires that τ xy = τ yx . expressed in terms of either.inﬁnite rotational acceleration (Figure 1.4). For example, τ yx = τ xy . Therefore we canwrite in general that MA = τ yx − τ xy = 0, so σi j = σ ji , or τi j = τ ji . (1.5)This makes the stress tensor symmetric about the diagonal.Transformation of axes. Frequently we must change the axis system in which a stressstate is expressed. For example, we may want to ﬁnd the shear stress on a slip system fromthe external stresses acting on a crystal. Another example is ﬁnding the normal stressacross a glued joint in a tube subjected to tension and torsion. In general a stress stateexpressed along one set of orthogonal axes (e.g., m, n, and p) may be expressed along adifferent set of orthogonal axes (e.g., i, j, and k). The general form of the transformationis 3 3 σij = l im l jn σmn . (1.6) n=1 m=1The term lim is the cosine of the angle between the i and m axes, and l jn is the cosine ofthe angle between the j and n axes. The summations are over the three possible values ofm and n, namely m, n, and p. This is often written as σi j = l im l jn σmn (1.7)with the summation implied. The stresses in the x, y, z coordinate system in Figure 1.5may be transformed onto the x , y , z coordinate system by σx x = l x x l x x σx x + l x y l x x σ yx + l x z l x x σzx + l x x l x y σx y + l x y l x y σ yy + l x z l x y σzy + l x x l x z σx z + l x y l x z σ yz + l x z l x z σzz (1.8a)
- 23. STRESS AND STRAIN 5and σx y = l x x l y x σx x + l x y l y x σ yx + l x z l y x σzx + l x x l y y σx y + l x y l y y σ yy + l x z l y y σzy + l x x l y z σx z + l x y l y z σ yz + l x z l y z σzz . (1.8b) These equations may be simpliﬁed with the notation in Equation (1.3) using Equation(1.5) obtain σ x = l x x 2 σ x + l x y 2 σ y + l x z 2 σz + 2l x y l x z τ yz + 2l x z l x x τzx + 2l x x l x y τx y (1.9a)and τx z = l x x l y x σx x + l x y l y y σ yy + l x z l y z σzz + (l x y l y z + l x z l y y )τ yz + (l x z l y x + l x x l y z )τzx + (l x x l y y + l x y l y x )τx y . (1.9b)Now reconsider the transformation in Figure 1.2. Using Equations (1.9a) and (1.9b) withσ yy as the only ﬁnite term on the x, y, z axis system, σ y = l y y 2 σ yy = σ y cos2 θand τx y = l x y l y y σ yy = σ y cos θ sin θ, (1.10)in agreement with Equations (1.4a) and (1.4b). These equations can be used with Millerindices for planes and direction indices for crystals. The reader who is not familiar withthese is referred to Appendix A. Example problem 1.1: A cubic crystal is loaded with a tensile stress of 2.8 MPa applied along the [210] direction as shown in Figure 1.6. Find the shear stress on the ¯ (111) plane in the [101] direction. Figure 1.6. A crystal stressed in tension along [210] showing the (111) slip plane and the [101] slip di- rection.
- 24. 6 MECHANICAL BEHAVIOR OF MATERIALS SOLUTION: In a cubic crystal, the normal to a plane has the same indices as the plane, so the normal to (111) is [111]. Also, in a cubic crystal, the cosine of the angle between two directions is given by the dot product of unit vectors in those direc- tions. For example, the cosine of the angle between [u1 v1 w1 ] and [u2 v2 w2 ] is equal to (u1 u2 + v1 v2 + w1 w2 )/[(u1 2 + v1 2 + w1 2 )(u2 2 + v2 2 + w2 2 )]1/2 . Designating [210] as x, [101] as d, and [111] as n, τ nd = lnx ld x σx x = ¯ √ 2 2 √ {(2·1 + 1·1 + 0 · 1)/ [(2 +1 + 0)(12 +12 +12 )]} · {(2·1 + 1·0 + 0·−1)/ [(22 + √ 12 + 0)(12 +0+12 )]} · 2.8 MPa = 2.8(6/5) 6 MPa = 1.372 MPa.Principal stresses. It is always possible to ﬁnd a set of axes (1, 2, 3) along which theshear stress components vanish. In this case the normal stresses, σ 1 , σ 2 , and σ 3 , are calledprincipal stresses and the 1, 2, and 3 axes are the principal stress axes. The magnitudesof the principal stresses, σ p , are the three roots of σp 3 − I1 σp 2 − I2 σp − I3 = 0, (1.11)where I1 = σx x + σ yy + σzz , I2 = σ yz 2 + σzx 2 + σx y 2 − σ yy σzz − σzz σx x − σx x σ yy , (1.12)and I3 = σx x σ yy σzz + 2σ yz σzx σx y − σx x σ yz 2 − σ yy σzx 2 − σzz σx y 2 .The ﬁrst invariant I1 = −p/3, where p is the pressure. I1 , I2 , and I3 are independent of theorientation of the axes and are therefore called stress invariants. In terms of the principalstresses, the invariants are I1 = σ1 + σ2 + σ3 , I2 = −σ22 σ33 − σ33 σ11 − σ11 σ22 , (1.13)and I3 = σ11 σ22 σ33 . Example problem 1.2: Find the principal stresses in a body under the stress state σ x = 10, σ y = 8, σ z = −5, τ yz = τ zy = 5, τ zx = τ xz = −4, and τ xy = τ yx = −8, where all stresses are in MPa. SOLUTION: Using Equation (1.13), I1 = 10 + 8 − 5 = 13, I2 = 52 + (−4)2 + (−8)2 − 8(−5) − (−5)10 − 10·8 = 115, and I3 = 10·8(−5) + 2·5(−4)(−8) − 10·52 − 8(−4)2 − (−5)(−8)2 = −138. Solving Equation (1.11) gives σ p 3 − 13σ p 2 − 115σ p + 138 = 0, σ p = 1.079, 18.72, − 6.82.Mohr’s stress circles. In the special case where there are no shear stresses acting onone of the reference planes (e.g., τ zy = τ zx = 0), the normal to that plane, z, is a directionof principal stress and the other two principal stress directions lie in the plane. This
- 25. STRESS AND STRAIN 7 y σy z τxy y’ x’Figure 1.7. Stress state to which Mohr’scircle treatment applies. Two shearstresses, τ yz and τ zx , are zero. σy σx τxy τyx y σx x φ xis illustrated in Figure 1.7. For these conditions l x z = l y z = 0, τzy = τzx = 0, l x x =l y y = cos φ, and l x y = −l y x = sin φ. The variation of the shear stress component τx ycan be found by substituting these conditions into the stress transformation equation(1.8b). Substituting l x z = l y z = 0 gives τx y = cos φ sin φ(−σx x + σ yy ) + (cos2 φ − sin2 φ)τx y . (1.14a) Similar substitution into the expressions for σ x and σ y results in σx = cos2 φσx + sin2 φσ y + 2 cos φ sin φτx y (1.14b)and σ y = sin2 φσx + cos2 φσ y + 2 cos φ sin φτx y . (1.14c)These can be simpliﬁed by substituting the trigonometric identities sin2φ = 2sin φcos φand cos 2φ = cos2 φ − sin2 φ to obtain τx y = −[(σx − σ y )/2] sin 2φ + τx y cos 2φ, (1.15a) σx = (σx + σ y )/2 + [(σx − σ y )/2] cos 2φ + τx y sin 2φ, (1.15b)and σ y = (σx + σ y )/2 − [(σx − σ y )/2] cos 2φ + τx y sin 2φ. (1.15c)Setting τ x y = 0 in Equation (1.15a), φ becomes the angle θ between the principal stressaxes and the x and y axes. See Figure 1.8. τ x y = 0 = sin 2θ(σ x − σ y )/2 + cos 2θ τ xy or tan 2θ = τx y /[(σx − σ y )/2]. (1.16)The principal stresses σ 1 and σ 2 are the values of σ x and σ y for this value of φ, σ1,2 = (σx + σ y )/2 ± [(σx − σ y )/2] cos 2θ + τx y sin 2θor σ1,2 = (σx + σ y )/2 ± (1/2)[(σx − σ y )2 + 4τx y 2 ]1/2 . (1.17) A Mohr’s circle diagram is a graphical representation of Equations (1.16) and (1.17).It plots as a circle with radius (σ 1 − σ 2 )/2 centered at (σ1 + σ2 )/2 = (σx + σ y )/2 (1.17a)
- 26. 8 MECHANICAL BEHAVIOR OF MATERIALS τ σx y 2 2 )/ 1 σ 1 + τxy (σ θ x 2θ σ2 σ σ1 (σx-σy)/2 (σx- +σy)/2 a σy bFigure 1.8. Mohr’s circles for stresses showing the stresses in the x–y plane. Note: The 1-axis is rotatedclockwise from the x-axis in real space (a), whereas in the Mohr’s circle diagram (b) the 1-axis is rotatedcounterclockwise from the x-axis.as shown in Figure 1.8. The normal stress components, σ , are represented on the ordinateand the shear stress components, τ , on the abscissa. Consider the triangle in Figure 1.8b. Using the Pythagorean theorem, the hypotenuseis 1/2 (σ1 − σ2 )/2 = [(σx + σ y )/2]2 + τx y 2 (1.17b)and tan(2θ) = [τx y /[(σx + σ y )/2]. (1.17c) The full 3-dimensional stress state may be represented by three Mohr’s circles (Fig-ure 1.9). The three principal stresses, σ 1 , σ 2 , and σ 3 , are plotted on the horizontal axis.The circles connecting these represent the stresses in the 1–2, 2–3, and 1–3 planes. Thelargest shear stress may be (σ 1 − σ 2 )/2, (σ 2 − σ 3 )/2, or (σ 1 − σ 3 )/2. Figure 1.9. Three Mohr’s circles representing a stress state in three dimensions. The three circles represent the stress states in the 2–3, 3–1, and 1– 2 planes.
- 27. STRESS AND STRAIN 9 Example problem 1.3: A body is loaded under stresses σ x = 150 MPa, σ y = 60 MPa, τ xy = 20 MPa, and σ z = τ yz = τ zx = 0. Find the three principal stresses, sketch the 3-dimensional Mohr’s circle diagram for this stress state, and ﬁnd the largest shear stress in the body. SOLUTION: σ 1 , σ 2 = (σ x + σ y )/2 ± {[(σ x − σ y )/2]2 + τ xy 2 }1/2 = 154.2, 55.8 MPa, σ 3 = σ z = 0. Figure 1.10 is the Mohr’s circle diagram. Note that the largest shear stress, τ max = (σ 1 − σ 3 )/2 = 77.1 MPa, is not in the 1–2 plane. Figure 1.10. Mohr’s circles for Example 1.3.StrainsAn inﬁnitesimal normal strain is deﬁned by the change of length, L, of a line: dε = dL/L . (1.18)Integrating from the initial length, Lo , to the current length, L, ε= dL/L = ln(L/L o ). (1.19)This ﬁnite form is called true strain (or natural strain, logarithmic strain). Alternatively,engineering or nominal strain, e, is deﬁned as e= L/L o . (1.20)If the strains are small, then engineering and true strains are nearly equal. Expressingε = ln(L/Lo ) = ln(1 + e) as a series expansion, ε = e − e2 /2 + e3 /3!− · · ·, so as e →0, ε → e. This is illustrated in the following example.
- 28. 10 MECHANICAL BEHAVIOR OF MATERIALS Example problem 1.4: Calculate the ratio e/ε for several values of e. SOLUTION: e/ε = e/ln(1 + e). Evaluating: for e = 0.001, e/ε = 1.0005; for e = 0.01, e/ε = 1.005; for e = 0.02, e/ε = 1.010; for e = 0.05, e/ε = 1.025; for e = 0.10, e/ε = 1.049; for e = 0.20, e/ε = 1.097; for e = 0.50, e/ε = 1.233. Note that the difference between e and ε is less than 1% for e < 0.02. There are several reasons that true strains are more convenient than engineeringstrains.1. True strains for equivalent amounts of deformation in tension and compression are equal except for sign.2. True strains are additive. For a deformation consisting of several steps, the overall strain is the sum of the strains in each step.3. The volume change is related to the sum of the three normal strains. For constant volume, εx + ε y + εz = 0.These statements are not true for engineering strains, as illustrated in the followingexamples. Example problem 1.5: An element 1 cm long is extended to twice its initial length (2 cm) and then compressed to its initial length (1 cm). 1. Find true strains for the extension and compression. 2. Find engineering strains for the extension and compression. SOLUTION: 1. During the extension, ε = ln(L/L o ) = ln2 = 0.693, and during the compression, ε = ln(L/L o ) = ln(1/2) = −0.693. 2. During the extension, e = L/Lo = 1/1 = 1.0, and during the compression, e = L/L o = −1/2 = −0.5. Note that with engineering strains, the magnitude of strain to reverse the shape change is different. Example problem 1.6: A bar 10 cm long is elongated by (1) drawing it to 15 cm, and then (2) drawing it to 20 cm. 1. Calculate the engineering strains for the two steps and compare the sum of these with the engineering strain calculated for the overall deformation. 2. Repeat the calculation with true strains.
- 29. STRESS AND STRAIN 11 SOLUTION: 1. For step 1, e1 = 5/10 = 0.5; for step 2, e2 = 5/15 = 0.333. The sum of these is 0.833, which is less than the overall strain etot = 10/10 = 1.00. 2. For step 1, ε 1 = ln(15/10) = 0.4055; for step 2, ε 1 = ln(20/15) = 0.2877. The sum is 0.6931 and the overall strain is ε tot = ln(15/10) + ln(20/15) = ln(20/10) = 0.6931. Example problem 1.7: A block of initial dimensions Lxo , Lyo , Lzo is deformed so that the new dimensions are Lx , Ly , Lz . Express the volume strain, ln(V/Vo ), in terms of the three true strains, εx , εy , εz . SOLUTION: V/Vo = Lx Ly Lz /(Lxo Lyo Lzo ), so ln (V /Vo ) = ln (L x /L xo ) + ln (L y /L yo ) + ln (L z /L zo ) = εx + ε y + εz . Note that if there is no volume change (ln(V/Vo ) = 0), the sum of the normal strains εx + ε y + εz = 0.Small strains. As bodies deform, they often undergo translation and rotation as well asdeformation. Strain must be deﬁned in such a way as to exclude the effects of translationand rotation. Consider the 2-dimensional body in Figure 1.11. Normal strains are deﬁnedas the fractional extensions (tensile) or contractions (compressive) L/Lo , so εx x =(A D − AD)/AD =A D /AD − 1. For a small strain, this reduces to εx x = (∂u/∂ x)dx/dx = ∂u/∂ x. (1.21)Similarly, ε yy = (∂v/∂ y)/dy/dy = ∂v/∂ y. (1.22) Shear strains are similarly deﬁned in terms of the angles between AD and A D andbetween AB and A B , which are respectively (∂v/∂ x)dx/dx = ∂v/∂ x and (∂u/∂ y)dy/dy = ∂u/∂ y. y B’ C’ v +(∂v/∂y)dy B CFigure 1.11. Translation, rotation, and distortion of atwo-dimensional body. dy u A’ D’ u +(∂u/∂x)dx A V D dx x
- 30. 12 MECHANICAL BEHAVIOR OF MATERIALS a. b. c.Figure 1.12. Illustration of shear and rotation. With small deformations, (a) differs from (c) only by a rotation, (b).The total engineering shear strain, γ yx , is the sum of these angles, γ yx = ∂v/∂ x + ∂u/∂ y = γx y . (1.23)Figure 1.12 shows that this deﬁnition excludes the effects of rotation for small strains. For a 3-dimensional body with displacements w in the z-direction, ε yy = ∂v/∂ y, γ yz = γzy = ∂w/∂ y + ∂v/∂z,and γ yx = γx y = ∂v/∂ x + ∂u/∂ y. Small strains can be treated as tensors, εx x ε yx εzx εi j = εx y ε yy εzy , (1.24) εx z ε yz εzzwhere the mathematical shear strains, ε ij , are one-half of the engineering shear strains,γ ij : ε yz = εzy = (1/2)γ yz = (1/2)(∂v/∂z + ∂w/dy) εzx = εx z = (1/2)γzx = (1/2)(∂w/∂ x + ∂u/dz) (1.25) εx y = ε yx = (1/2)γx y = (1/2)(∂u/∂ y + ∂v/∂ x).Transformation of axes. Small strains may be transformed from one set of axesto another in a manner completely analogous to the transformation of stresses(Equation 1.9), εi j = l im l jn εmn , (1.26)where double summation is implied. For example, εx x = l x x l x x εx x + l x y l x x ε yx + l x z l x x εzx + l x x l x y εx y + l x y l x y ε yy + l x z l x y εzy + l x x l x z εx z + l x y l x z ε yz + l x z l x z εzz (1.27a)and εx y = l x x l y x εx x + l x y l y x ε yx + l x z l y x εzx + l x x l y y εx y + l x y l y y ε yy + l x z l y y εzy + l x x l y z εx z + l x y l y z ε yz + l x z l y z εzz . (1.27b)
- 31. STRESS AND STRAIN 13These can be written more simply in terms of the usual shear strains, ε x = l x x 2 ε x + l x y 2 ε y + l x z 2 εz + l x y l x z γ yz + l x z l x x γzx + l x x l x y γx y (1.28a)and γx y = 2(l x x l y x εx + l x y l y y ε y + l x z l y z εz ) + (l x y l y z + l x z l y y )γ yz + (l x z l y x + l x x l y z )γzx + (l x x l y y + l x y l y x )γx y . (1.28b) Large strains are not tensors and cannot be transformed from one axis system toanother by a tensor transformation. The reason is that the angles between material direc-tions are altered by deformation. With small strains, changes of angle are small and canbe neglected. The following example illustrates this point. Example problem 1.8: A 2-dimensional square body initially 1.000 cm by 1.000 cm was deformed into a rectangle 0.95 cm by 1.10 cm as shown in Figure 1.13. 1. Calculate the strain, ex , along the diagonal from its initial and ﬁnal dimensions. Then calculate the strains, ex and e y , along the edges and use the transformation equation ei j = l im l jn emn to ﬁnd the strain along the diagonal and compare with the two values of e x . 2. Repeat A for a 1.000 cm by 1.000 cm square deformed into a 0.50 cm by 2.0 cm rectangle. y x’ 1 or x 1 Figure 1.13. Small and large deformations of a body. SOLUTION: √ 1. The initial diagonal = 2 = 1.414214 and for the small deformation, the ﬁnal di- √ agonal becomes (.952 + 1.12 ) = 1.4534, so ex = (L − L o )/L o = L/L o − 1 = 1.4534/1.414214 − 1 = 0.0277. Taking the angle, θ, between the x and x (or y) axes as 45◦ , ex = l x x 2 εx + l x y 2 ε y = 0.1/2 − 0.05/2 = 0.025, which is very close to 0.0277. √ 2. For the large deformation, the diagonal becomes (22 + 0.52 ) = 2.062, so cal- culating the strain from this, ex = 2.062/1.414214 − 1 = 0.4577. The strains on the edges are ex = 1 and e y = −0.5, so ex = l x x 2 ex + l x y 2 e y = (1/2)(1) + (1/2)(−0.5) = 0.0250, which does not agree with ex = 0.4577, calculated from
- 32. 14 MECHANICAL BEHAVIOR OF MATERIALS γ/2 εx Figure 1.14. Mohr’s circle for strain. This is similar to Mohr’s stress circle except that the normal strain, ε ε2 γxy/2 (or e), is plotted on the horizontal axis (instead of σ ) ε1 ε and γ /2 is plotted vertically (instead of τ ). γxy/2 εy the specimen dimensions. With true strains the agreement is not much better. Di- rect calculation of ε x from the diagonal gives ε x = ln(2.062/1.414) = 0.377 and calculation from the strains along the sides gives ε x = (1/2)ln(2) + (1/2)ln (0.5) = 0. The reason is that with large strains, the angle θ changes with deformation.Mohr’s strain circles. Because small strains are tensor quantities, Mohr’s circle dia-grams apply if the strains ex , e y , and γx y are known along two axes and the third axis,z, is a principal strain axis (γ yz = γzx = 0). The strains may be either engineering, e,or true, ε, because they are equal when small. Care must be taken to remember that thetensor shear-strain terms are only one-half of the conventional shear strains. A plot ofγ /2 versus e (or ε) is a circle, as shown in Figure 1.14. The equations, analogous to thosefor stresses, are (e1 + e2 )/2 = (ex + e y )/2 (1.29) (e1 − e2 )/2 = {[(ex − e y )/2]2 + (γx y /2)}1/2 (1.30) 1/2 e1 , e2 = (ex + e y )/2 ± [(ex − e y )/2]2 + (γx y /2)2 (1.31) tan(2θ) = (γx y /2)/[(ex − e y )/2] = γx y /(ex − e y ). (1.32)As with Mohr’s stress circles, a 3-dimensional strain state can be represented by threeMohr’s circles. It is emphasized that the strain transformation equations, including theMohr’s circle equations, apply to small strains. Errors increase when the strains are largeenough to cause rotation of the axes. Example problem 1.9: Draw the 3-dimensional Mohr’s circle diagram for an x- direction tension test (assume ey = ez = −ex /3), plane strain (ey = 0) and an x-direction compression test (assume ey = ez = −ex /3). In each case determine γ max .
- 33. STRESS AND STRAIN 15 SOLUTION: The 3-dimensional Mohr’s circle diagrams are shown in Figure 1.15. γ/2 γ/2 γ/2 ey = ez ex e ez ey exe ex e ey = ez Figure 1.15. Three-dimensional Mohr’s strain circles for (A) tension, (B) plane strain, and (C) compression. In (A) and (C) the circles between ey and ez reduce to a point and the circles between ex and ey coincide with the circles between ex and ez .Force and moment balances. The solutions of many mechanics problems require forceand moment balances. The external forces acting on one half of the body must balancethose acting across the cut. Consider force balances to ﬁnd the stresses in the walls of acapped thin-wall tube loaded by internal pressure. Example problem 1.10: A capped thin-wall tube having a length L, a diameter D, and a wall thickness t is loaded by an internal pressure P. Find the stresses in the wall assuming that t is much smaller than D and that D is much less than L. SOLUTION: First make a cut perpendicular to the axis of the tube (Figure 1.16a) and consider the vertical (y-direction) forces. The force from the pressurization is the pressure, P, acting on the end area of the tube, PπD2 /4. The force in the wall is the stress, σ y , acting on the cross section of the wall, σ y πDt. Balancing the forces, Pπ D2 /4 = σ y πDt, and solving for σ y , σ y = P D/(4t). (1.33) P σy σy Figure 1.16. Cuts through a thin- wall tube loaded under internal σx P t pressure. t σx D D a b The hoop stress, σ x , can be found from a force balance across a vertical cut (Fig- ure 1.16b). The force acting to separate the tube is the pressure, P, acting on the internal area, DL, where L is the tube length. This is balanced by the hoop stress in
- 34. 16 MECHANICAL BEHAVIOR OF MATERIALS the two walls, σ x , acting on the cross-sectional area of the two walls, 2Lt. (The force in the capped ends is neglected because the tube is long and we are interested in the stress in regions remote from the ends.) Equating these two forces, PDL = σ x 2t, so that σx = P D/(2t) = 2σ y . (1.33) The stress in the radial direction though the wall thickness, σ z , is negligible relative to σ x and σ y if D t. On the inside surface σ z = −P and on the outside surface σ z = 0. The average, −P/2, is much less than PD/(2t), so for engineering purposes we can take σ z = 0. A moment balance may be made about any axis in a body under equilibrium. Themoment caused by external forces must equal the moment caused by internal stresses.An example is the torsion of a circular rod. Example problem 1.11: Relate the internal shear stress, τ xy , in a rod of radius R to the torque, T, acting on the rod. SOLUTION: Consider a differential element of dimensions (2πr)(dr) in a tubular element at a radius r from the axis and of thickness dr (Figure 1.17). The shear force acting on this element is the shear stress times the area, τ xy (2πr)(dr). The torque about the central axis caused by this element is the shear force times the distance from the axis r, dT = τx y (2πr )(r )dr, so that R T = 2π τ x yr 2 dr . (1.34) 0 dr Figure 1.17. A differential element of area 2π rdr in R r a rod loaded under torsion. The shear stress, τ xy , z τxy on this element causes a differential moment, 2π τ xy y r2 dr. x An explicit solution requires knowledge of how τ xy varies with r.Boundary conditions. It is important, in analyzing mechanical problems, to recognizesimple, often unstated, boundary conditions and use them to make simplifying assump-tions.1. Free surfaces: On a free surface the two shear stress components in the surface vanish; that is, if z is the normal to a free surface, τ yz = τ zx = 0. Unless there is a pressure acting on a free surface, the stress normal to it also vanishes; that is, σ zz = 0. Likewise there are no shear stresses, τ yz = τ zx , acting on surfaces that are assumed to be frictionless.
- 35. STRESS AND STRAIN 17 z B y A d d d xFigure 1.18. Grooved plate. The material outside the Figure 1.19. In the gauge section of a tensile bar, thegroove affects the x-direction ﬂow inside the groove effect of the ends almost disappears at a distance dso that εxA = εxB . from the shoulder.2. Constraints from neighboring regions: The deformation in a particular region is often controlled by the deformation in a neighboring region. Consider the deformation in a long narrow groove in a plate as shown in Figure 1.18. The long narrow groove (B) is in close contact with a thicker region (A). As the plate deforms, the defor- mation in the groove must be compatible with the deformation outside the groove. Its elongation or contraction must be the same as that in the material outside, so that ε xA = ε xB . The y- and z-direction strains in the two regions need not be the same.3. St. Venant’s principle states that the restraint from any end or edge effect will dis- appear within one characteristic distance. As an example, the enlarged end of a tensile bar (Figure 1.19) tends to suppress lateral contraction of the gauge section next to it. Here the characteristic distance is the diameter of the gauge section, so the constraint is almost gone at a distance from the enlarged end equal to the dia- meter. Another example of St. Venant’s principle is a thin, wide sheet bent to a constant radiusof curvature (Figure 1.20). The condition of plane strain (εy = 0) prevails over most of thematerial. This is because the top and bottom surfaces are so close that they restrain oneanother from contracting or expanding. Appreciable deviation from plane strain occursonly within a distance from the edges of the sheet equal to the sheet thickness. At theedge σ y = 0. zFigure 1.20. Bending of a thin sheet. Plane strain (ε y= 0) prevails except near the edges, where there is acondition of plane stress (σ y = 0). x yNOTEThe simpliﬁcation of the notation for tensor transformation, σi j = 3 n=1 m=1 l im l jn σmn , 3 to σi j =l im l jn σmn has been attributed to Albert Einstein.
- 36. 18 MECHANICAL BEHAVIOR OF MATERIALSPROBLEMS 1. Consider an aluminum single crystal under a stress state σ x = 250 psi, σ y = −50 psi, σ z = τ yz = τ zx = τ xy = 0, where x = [100], y = [010], and z = [001]. A. What is the resolved shear stress, τ nd , on the (111) plane in the [110] direction? that is, with n = [111], d = [110]? B. What is the resolved shear stress on the (111) plane in the [101] direction? 2. Consider the single crystal in problem 1. Now suppose that slip does occur on the (111) plane in the [101] direction and only on that slip system. Also assume that the resulting strains are small. Calculate the ratios of the resulting strains ε y /ε x and ε z /ε x . 3. A body is loaded under a stress state σ x = 400, σ y = 100, τ xy = 120, τ yz = τ zx = σ z = 0. A. Sketch the Mohr’s circle diagram. B. Calculate the principal stresses. C. What is the largest shear stress in the body? (Do not neglect the z direction.) 4. Three strain gauges have been pasted onto the surface of a piece of steel in the pattern shown in Figure 1.21. While the steel is under load, these gauges indicate the following strains parallel to their axes: Gauge A, 450 × 10−6 ; Gauge B, 300 × 10−6 ; Gauge C, −150 × 10−6 . A. Calculate the principal strains, ε 1 and ε2 . B. Find the angle between the 1 axis and the x-axis, where 1 is the axis of the largest principal strain. [Hint: Let the direction of gauge B be x , write the strain transformation equation expressing the strain ex in terms of the strains along the x and y axes, solve for gxy , and ﬁnally use the Mohr’s circle equat- ions.] 5. Consider a thin-wall tube that is 1 in. in diameter and has a 0.010-in. wall thickness. Let x, y, and z be the axial, tangential (hoop), and radial directions, respectively. A. The tube is subjected to an axial tensile force of 80 lbs. and a torque of 100 in.-lbs. i. Sketch the Mohr’s stress circle diagram showing stresses in the x–y plane. ii. What is the magnitude of the largest principal stress? iii. At what angles are the principal stress axes, 1 and 2, to the x and y directions? y C gauge B Figure 1.21. Arrangement of strain gauges. e ug 40° ga gauge A x
- 37. STRESS AND STRAIN 19y y 34° θ x x xFigure 1.22. Circle grids printed on a metal sheet. Figure 1.23. Glued rod. B. Now let the tube be capped and let it be subject to an internal pressure of 120 psi and a torque of 100 in.-lbs. i. Sketch the Mohr’s stress circle diagram showing stresses in the x–y plane. ii. What is the magnitude of the largest principal stress? iii. At what angles are the principal stress axes, 1 and 2, to the x and y directions? 6. A solid is deformed under plane-strain conditions (εz = 0). The strains in the x–y plane are ε x = 0.010, ε y = 0.005, and γ xy = 0.007. A. Sketch the Mohr’s strain circle diagram. B. Find the magnitude of ε 1 and ε2 . C. What is the angle between the 1 and x axes? D. What is the largest shear strain in the body? (Do not neglect the z direction.) 7. A grid of circles, each 10.00 mm in diameter, was etched on the surface of a sheet of steel as shown in Figure 1.22. When the sheet was deformed, the grid circles were distorted into ellipses. Measurement of one indicated that the major and minor diameters were 11.54 and 10.70 mm, respectively. A. What are the principal strains, ε 1 and ε 2 ? B. If the axis of the major diameter of the ellipse makes an angle of 34◦ to the x-direction, what is the shear strain, γ xy ? C. Draw the Mohr’s strain circle showing ε1 , ε2 , εx , and ε y . 8. Consider an aluminum single crystal under a stress state, σ x = + 75 psi, σ y = + 25 psi, σ z = τ yz = τ zx = τ xy = 0, where x = [100], y = [010], and z = [001]. What is the resolved shear stress, γ nd , on the (111) plane and in the [101] direction? 9. Consider the torsion of a rod that is 1 m long and 50 mm in diameter. A. If one end of the rod were twisted by 1.2◦ relative to the other end, what would be the largest principal strain on the surface? B. If the rod were extended by 1.2% and its diameter decreased by 0.4% at the same time that it was being twisted, what would be the largest principal strain?10. Two pieces of rod are glued together along a joint whose normal makes an angle, θ, with the rod axis, x, as shown in Figure 1.23. The joint will fail if the shear stress on the joint exceeds its shear strength, τ max . It will also fail if the normal stress across the joint exceeds its normal strength, σ max . The shear strength, τ max , is 80% of the normal strength, σ max . The rod will be loaded in uniaxial tension along its axis, and it is desired that the rod carry as high a tensile force, Fx as possible. The angle, θ, cannot exceed 65◦ .
- 38. 20 MECHANICAL BEHAVIOR OF MATERIALS tension Figure 1.24. Tube formed from a coiled and glued 0.030 in strip. 1.5 in 68° torque A. At what angle, θ, should the joint be made so that a maximum force can be carried? B. If θ max were limited to 45◦ , instead of 65◦ , how would your answer be altered? [Hint: plot σ x /σ max versus θ for both failure modes.]11. Consider a tube made by coiling and gluing a strip as shown in Figure 1.24. The diameter is 1.5 in., the length is 6 in., and the wall thickness is 0.030 in. If a tensile force of 80 lbs. and a torque of 30 in.-lbs. are applied in the direction shown, what is the stress normal to the glued joint? [Hint: Set up a coordinate system.]
- 39. 2 ElasticityIntroductionElastic deformation is reversible. When a body deforms elastically under a load, it willrevert to its original shape as soon as the load is removed. A rubber band is a familiarexample. Most materials, however, can undergo very much less elastic deformation thanrubber. In crystalline materials elastic strains are small, usually less than 1/2%. It issafe for most materials, other than rubber to assume that the amount of deformationis proportional to the stress. This assumption is the basis of the following treatment.Because elastic strains are small, it doesn’t matter whether the relations are expressed interms of engineering strains, e, or true strains, ε. The treatment in this chapter will start with the elastic behavior of isotropic materials,the temperature dependence of elasticity, and thermal expansion. Then anisotropic elasticbehavior and thermal expansion will be covered.Isotropic elasticityAn isotropic material is one that has the same properties in all directions. If uniaxialtension is applied in the x-direction, the tensile strain is ex = σ x /E, where E is Young’smodulus. Uniaxial tension also causes lateral strains, ey = ez = −υex , where υ is Poisson’sratio. Consider the strain, ex , produced by a general stress state, σ x , σ y , σ z . The stress σ xcauses a contribution ex = σ x /E. The stresses σ y , σ z cause Poisson contractions, ex =−υσ y /E and ex = −υσ z /E. Taking into account these Poisson contractions, the generalstatement of Hooke’s law is ex = (1/E)[σx − υ(σ y + σz )]. (2.1a)Shear strains are affected only by the corresponding shear stresses, so that γ yz = τ yz /G = 2e yz , (2.1b)where G is the shear modulus. Similar expressions apply for all directions, so that ex = (1/E)[σx − υ(σ y + σz )] γ yz = τ yz /G e y = (1/E)[σ y − υ(σz + σx )] γzx = τzx /G (2.2) ez = (1/E)[σz − υ(σx + σ y )] γx y = τx y /G. 21
- 40. 22 MECHANICAL BEHAVIOR OF MATERIALSEquations (2.1) and (2.2) hold whether or not x, y, and z are directions of principal stress. For an isotropic material, the shear modulus, G, is not independent of E and υ. Thiscan be demonstrated by considering a state of pure shear, τ xy , with σ x = σ y = σ z = τ yz =τ zx = 0. The Mohr’s circle diagram, Figure 2.1, shows that the principal stresses are σ 1 =τ xy , σ 2 = −τ xy , and σ 3 = 0. From Hooke’s law, e1 = (1/E)[σ 1 − υ(σ 2 + σ 3 )] = (1/E)[τ xy − υ(−τ xy + 0)] =[(1 + υ)/E]τ . The Mohr’s strain circle diagram (Figure 2.1) shows that γ xy /2 = e1 .Substituting for e1 , γ xy /2 = [(1 + υ)/E]τ xy . Now comparing with γ xy = τ xy /G, G = E/[2(1 + υ)]. (2.3)The bulk modulus, B, is deﬁned by the relation between the volume strain and the meanstress, V /V = (1/B)σm , (2.4)where σ m = (σ x + σ y + σ z )/3. The bulk modulus, like the shear modulus, is notindependent of E and υ. This can be demonstrated by considering the volume strainproduced by a state of hydrostatic stress, σ x = σ y = σ z = σ m . It was shown in ExampleProblem 1.7 that, for small deformations, the volume strain, V/V = ex + ey + ez .Substituting ex = (1/E)[σ x − υ(σ y + σ z )] = (1/E)[σ m − υ(σ m + σ m )] = [(1 − 2υ)/E]σ m .Then V/V = 3σ m (1 − 2υ)/E. Comparing with V/V = (1/B)σ m , B = E/[3(1 − 2υ)]. (2.5) For most materials, Poisson’s ratio is between 0.2 and 0.4. The value of υ cannotexceed 0.5 for an isotropic material; if it did, B would be negative, and that would implyan increase of pressure would cause an increase of volume. Any of the four elastic constants, E, υ, G, and B, can be expressed in terms of twoothers: E = 2G(1 + υ) = 3B(1 − 2υ) = 9BG/(G + 3B), (2.6a) υ = E/(2G) − 1 = 1/2 − E/6B) = 1/2 − (3/2)G/(3B + G), (2.6b) G = E/[2(1 + υ)] = 3E B/(9B − E) = (3/2)B(1 − 2υ)/(1 + υ), (2.6c) B = E/[3(1 − 2υ)] = E G/[3(3G − E)] = (2/3)G(1 + υ)/(1 − 2υ). (2.6d) Only three of the six normal stresses and strain components, ex , ey , ez , σ x , σ y , or σ z ,need to be known to ﬁnd the other three. This is illustrated in the following examples. y τ γ/2 τxy 1 τxy γxy/2 τxy σ e2 x σ2 σ1 e2 e1Figure 2.1. Mohr’s stress and strain circles for shear.
- 41. ELASTICITY 23 Example problem 2.1: A wide sheet (1 mm thick) of steel is bent elastically to a constant radius of curvature, ρ = 50 cm, measured from the axis of bending to the center of the sheet, as shown in Figure 2.2. Knowing that E = 208 GPa, and υ = 0.29 for steel, ﬁnd the stress in the surface. Assume that there is no net force in the plane of the sheet. Figure 2.2. Bent sheet. The strain ey and the stress σ z are zero. SOLUTION: Designate the directions as shown in Figure 2.2. Inspection shows that σ z = 0 because the stress normal to a free surface is zero. Also, ey = 0, because the sheet is wide relative to its thickness; ey must be the same on the top and bottom surfaces, and therefore equals zero. Finally, the strain ex at the outer surface can be found geometrically as ex = (t/2)/ρ = (1/2)/500 = 0.001. Now substituting into Hooke’s laws (Equation (2.2)), ey = 0 = (1/E)[σ y − υ(σ x − 0)], so σ y = υσ x . Substituting again, ex = t/(2ρ) = (1/E)[σ x − υ(σ y − 0)] = (1/E)(σ x − υ 2 σ x ) = σ x (1− υ 2 )/E; σ x = [t/(2ρ)]E/(1− υ 2 )] = (0.001)(208 × 109 )/(1 − 0.292 ) = 227 MPa; and σ y = υσx = 0.29 · 227 = 65.8 MPa. Example problem 2.2: A body is loaded elastically so that ey = 0, and σ z = 0. Both σ x and σ y are ﬁnite. Derive an expression for ez in terms of σ x , E, and υ only. SOLUTION: Substituting ey = 0 and σ z = 0 into Hooke’s law (Equation (2.2)), 0 = (1/E)[σ y − υ(0 + σ x )], so σ y = υσ x . Substituting into Hooke’s law again, ez = (1/E)[0 − υ(σx + υσx )] = −σx υ(1 + υ)/E. Example problem 2.3: Draw the 3-dimensional Mohr’s strain circle diagram for a body loaded elastically under balanced biaxial tension, σ 1 = σ 2 . Assume that υ = 0.25. What is the largest shear strain, γ ? SOLUTION: σ 1 = σ 2 and σ 3 = 0. From symmetry, e1 = e2 , so using Hooke’s laws, e1 = (1/E)(σ 1 − υσ 1 ) = 0.75σ 1 /E, e3 = (1/E)[0 − υ(σ 1 + σ 1 )] =− 0.5σ 1 . γ max = (e1 − e3 ) = 1.25σ 1 /E. In Figure 2.3, e1 , e2 , and e3 are plotted on the horizontal axis. The circle has a radius of 0.625σ 1 /E = (5/6) e1 with e2 = e1 and e3 = (−2/3)e1 . γ max = 1.67 1 .
- 42. 24 MECHANICAL BEHAVIOR OF MATERIALS γ/2 (γ/2)max = (5/6)e1 Figure 2.3. Mohr’s strain circles for an elastic body under biaxial tension. The (σ 1 − σ 2 ) circle reduces to a point and the (σ 1 − σ 3 ) and (σ 2 − σ 3 ) circles e2 = e1 e are superimposed as a single circle. . e3 =. -(2/3)e1Variation of Young’s modulus. The binding energy between two neighboring atoms orions can be represented by a potential well. Figure 2.4 is a schematic plot showing howthe binding energy varies with separation of atoms. At absolute zero, the equilibriumseparation corresponds to the lowest energy. The Young’s modulus and the melting pointare both related to the potential well; the modulus depends on the curvature at the bottomof the well and the melting point depends on the depth of the well. The curvature and thedepth tend to be related, so the elastic moduli of different crystals roughly correlate withtheir melting points (Figure 2.5). The modulus also correlates with the heat of fusion andthe latent heat of melting, which are related to the depth of the potential well. For a givenmetal, the elastic modulus decreases as the temperature is increased: see Figure 2.6. For crystalline materials the elastic modulus is generally regarded as being relativelyinsensitive to changes of microstructure. The Young’s moduli of body-centered cubic(bcc) and face-centered cubic (fcc) forms of iron differ by a relatively small amount.Heat treatments that have large effects on hardness and yield strength have little effect onthe elastic properties. Cold working and small alloy additions also have relatively smalleffects because only a small fraction of the near-neighbor bonds are affected by thesechanges.energy atomic separation Figure 2.4. Schematic plot of the variation of binding energy with atomic separation at absolute zero. equilibrium separation
- 43. ELASTICITY 25 600 Ir Re Youngs modulus, GPa 400 W Mo Be Rh Cr Co Ni 200 Fe Mn V Cu Zr Cd Au Al Ag Sn Mg 0 0 1000 2000 3000 4000 Melting temperature, KFigure 2.5. Correlation between elastic modulus at room temperature and melting point. Elements with highermelting points have higher elastic moduli. The elastic behavior of polymers is very different from that of metals. The elasticstrains are largely a result of the straightening of polymer chains by rotation of bondsrather than by bond stretching. Consequently the Young’s moduli of typical polymers areorders of magnitudes lower that those of metals and ceramics. Only in highly orientedpolymers is stretching of covalent bonds the primary source of elastic strains and theelastic moduli of highly oriented polymers comparable with those of metals and ceramics. 250Youngs Modulus GPa 200 iron 150 copper 100 aluminium 50 0 0 200 400 600 800 1000 1200 1400 Temperature, KFigure 2.6. Variation of Young’s moduli with temperature. Young’s moduli decrease with increasing temper-ature. However, the moduli at the melting point are less than ﬁve times those at 0◦ K. Data from W. Koster,Zeitschrift fur Metallkunde, Vol. 39, 1948. ¨
- 44. 26 MECHANICAL BEHAVIOR OF MATERIALSFor polymers the magnitude of elastic strain is often much greater than in metals andceramics. Hooke’s law does not describe the elasticity of rubber very well. This is treatedin Chapter 20.Isotropic thermal expansion. When the temperature of an isotropic material is changed,its fractional change in length is L/L = α T. (2.7)Such dimension changes can be considered strains, and Hooke’s law can be generalizedto include thermal strains, ex = (1/E)[σx − υ(σ y + σz )] + α T. (2.8)This generalization is useful for ﬁnding the stresses that arise when constrained bodiesare heated or cooled. Example problem 2.4: A glaze is applied on a ceramic body by heating it above 600◦ C, which allows it to ﬂow over the surface. On cooling the glaze becomes rigid at 500◦ C. See Figure 2.7. The coefﬁcients of thermal expansion of the glaze and the body are α g = 4.0 × 10−6 /◦ C and α b = 5.5 × 10−6 /◦ C. The elastic constants for the glaze are Eg = 70 GPa and υ g = 0.3. Calculate the stresses in the glaze when it has cooled to 20◦ C. Figure 2.7. Stresses in a glaze. SOLUTION: Let the direction normal to the surface be z, so that the x and y directions lie in the surface. The strains in the x and y directions must be the same in the glaze and body: exg = (1/E g )[σxg − υg (σ yg + σzg )] + αg T = (1/E b )[σxb − υb (σ yb + σzb )] + αb T. Take σzg = σzb = 0 (free surface) and σxg = σyg and σxb = σyb = 0 (symmetry). The stress in the ceramic body, σxb = σ yb , requires a balance of forces, tb σxb + tg σxg = 0 is negligible. Because the glaze is very thin, hence, (1/E g )[σxg (1 − υg )] + αg T = αb T, σxg = [E g /(1 − υg )](αb − αg ) T = ◦ [(70 × 109 Pa)/(1 − .3)]](4 − 5.5)(10−6 C)(−480 ◦ C) = −72 MPa (compression) on cooling.
- 45. ELASTICITY 27Table 2.1. Elastic constants and thermal expansion coefﬁcients for various materials Thermal expansion coefﬁcientMaterial E (GPa) Poisson’s ratio (× 10−6 /◦ C)aluminum 62. 0.24 23.6iron 208.2 0.291 11.8copper 128. 0.35 16.5magnesium 44. — 27.1nickel 207. 0.31 13.3MgO 205. — 9.Al3 O3 350. — 9.glass 70. — 9.polystyrene 2.8 — 63PVC 0.35 — 190.nylon 2.8 — 100. The elastic constants and thermal expansion coefﬁcients for various materials aregiven in Table 2.1. Bimetallic strips used for sensing temperature depend on the differences of the thermalexpansion of the two materials.Anisotropic elasticityAlthough it is frequently assumed that materials are isotropic (i.e., they have the sameproperties in all directions), they rarely are. In single crystals, elastic properties vary withcrystallographic direction. In polycrystals, anisotropy of elastic properties is caused bythe presence of preferred orientations or crystallographic textures. These arise becauseof preferred growth directions during solidiﬁcation and because of lattice rotation dur-ing deformation. Recrystallization may change the preferred orientations for grains orcrystallographic textures, but it does not eliminate them. Hooke’s law for anisotropic materials can be expressed in terms of compliances,sijmn , which relate the contributions of individual stress components to individual straincomponents. In the most general case of linear elasticity, each strain component is alinear function of every stress component. This relation may be written as: ei j = si jmn σmn , (2.9)where summation is implied. The individual compliances, sijmn , form a fourth-ordertensor. However, this relation is greatly simpliﬁed by taking advantage of the relationsσ ij = σ ji and γ ij = 2eij = 2eji and by adopting a new subscript convention for thecompliances: Two subscripts, i and j, are used to identify the location (row and column)of the compliance in the matrix, rather than the axes of strain and stress components.Because the subscripts identify the location of the compliances, the order of the stressand strain components in the matrix is critical. With this new convention Hooke’s law
- 46. 28 MECHANICAL BEHAVIOR OF MATERIALSbecomes e11 = s11 σ11 + s12 σ22 + s13 σ33 + s14 σ23 + s15 σ31 + s16 σ12 e22 = s21 σ11 + s22 σ22 + s23 σ33 + s24 σ23 + s25 σ31 + s26 σ12 e33 = s31 σ11 + s32 σ22 + s33 σ33 + s34 σ23 + s35 σ31 + s36 σ12 γ23 = s41 σ11 + s42 σ22 + s43 σ33 + s44 σ23 + s45 σ31 + s46 σ12 (2.10) γ31 = s51 σ11 + s52 σ22 + s53 σ33 + s54 σ23 + s55 σ31 + s56 σ12 γ12 = s61 σ11 + s62 σ22 + s63 σ33 + s64 σ23 + s65 σ31 + s66 σ12 .Note that the subscripts 1, 2, and 3 on the stress and strain terms refer to the crystallo-graphic axes of the crystal. It can be shown for all combinations of i and j that sij = sji .This simpliﬁes the matrix to e11 = s11 σ11 + s12 σ22 + s13 σ33 + s14 σ23 + s15 σ31 + s16 σ12 e22 = s12 σ11 + s22 σ22 + s23 σ33 + s24 σ23 + s25 σ31 + s26 σ12 e33 = s13 σ11 + s23 σ22 + s33 σ33 + s34 σ23 + s35 σ31 + s36 σ12 γ23 = s14 σ11 + s24 σ22 + s34 σ33 + s44 σ23 + s45 σ31 + s46 σ12 (2.11) γ31 = s15 σ11 + s25 σ22 + s35 σ33 + s45 σ23 + s55 σ31 + s56 σ12 γ12 = s16 σ11 + s26 σ22 + s36 σ33 + s46 σ23 + s56 σ31 + s66 σ12 .For the most general case there is a maximum of 21 independent elastic constants.Symmetry often causes many of these constants to be equal or to vanish when x, y, andz are parallel to the axes of symmetry. With orthotropic symmetry the 23, 31, and 12 planes are planes of mirror symmetry(making 1, 2, and 3 axes of twofold rotational symmetry). Paper, wood, and rolled sheetsof metal are a few examples of such materials. Hooke’s law simpliﬁes to e11 = s11 σ11 + s12 σ22 + s13 σ33 e22 = s12 σ11 + s22 σ22 + s23 σ33 e33 = s13 σ11 + s23 σ22 + s33 σ33 γ23 = s44 σ23 (2.12) γ31 = s55 σ31 γ12 = s66 σ12 .For cubic crystals, 1, 2, and 3 are the cubic <100> axes. Because of symmetry, s13 = s23 =s12 , s22 = s33 = s11 , and s66 = s55 = s44 , so the relations further simplify to e11 = s11 σ11 + s12 σ22 + s12 σ33 e22 = s12 σ11 + s11 σ22 + s12 σ33 e33 = s12 σ11 + s12 σ22 + s11 σ33 γ23 = s44 σ23 (2.13) γ31 = s44 σ31 γ12 = s44 σ12 .
- 47. ELASTICITY 29For hexagonal and cylindrical symmetry, z is taken as the hexagonal or cylindrical axis.The 1 and 2 axes are any axes normal to 3. In this case, s13 = s23 , s22 = s33 , and s66 =2(s11 − s12 ), which simpliﬁes Equation (2.10) to e11 = s11 σ11 + s12 σ22 + s13 σ33 e22 = s12 σ11 + s11 σ22 + s13 σ33 e33 = s13 σ11 + s13 σ22 + s33 σ33 γ23 = s44 σ23 (2.14) γ31 = s44 σ31 γ12 = 2(s11 − s12 )σ12 . The elastic compliances for several cubic crystals are listed in Table 2.2.Orientation dependence of elastic response. Equations (2.9)–(2.13) describe theelastic response along the symmetry axes. The elastic response along any other set ofaxes may be calculated by ﬁrst resolving the stress state onto the symmetry axes, thenusing the matrices of elastic constants to ﬁnd the strains along the symmetry axes, andﬁnally resolving these strains onto the axes of interest. Example problem 2.5: Derive expressions for the effective Young’s modulus and Pois- son’s ratio for a cubic crystal stressed along the [112] direction. SOLUTION: Let x = [112]. The axes y and z must be normal to x and each other; for example, y = [111] and z = [110]. The direction cosines between these axes and the cubic axes of the crystal can be found by dot products; √ example, l 1x = [100]·[112] = for (1·1 + 0·1 + 0·2)/(12 + 02 + 02 )(12 + 12 + 22 ) = 1/ 6. Forming a table of direction cosines: x = 112 y = 111 z = 110 √ √ √ 1 = 100 1/√6 1/√3 1/ √ 2 2 = 010 1/√6 1/ √ 3 −1/ 2 3 = 001 2/ 6 −1/ 3 0 For tension along [112], σ y = σ z = σ yz = σ zx = σ xy = 0, so the only ﬁnite stress on the x, y, z axis system is σ x . Transforming to the 1, 2, and 3 axes using Equation (1.8), σ1 = (1/6)σx σ23 = (1/3)σx σ2 = (1/6)σx σ31 = (1/3)σx σ3 = (2/3)σx σ12 = (1/6)σx . From Equation (2.13) for a cubic crystal, the resulting elastic strains are e1 /σx = (1/6)s11 + (1/6)s12 + (2/3)s12 = (1/6)s11 + (5/6)s12 ,
- 48. 30 MECHANICAL BEHAVIOR OF MATERIALSTable 2.2. Elastic compliances (TPa)−1 for various cubic crystalsMaterial s11 s12 s44Cr 3.10 −0.46 10.10Fe 7.56 −2.78 8.59Mo 2.90 −0.816 8.21Nb 6.50 −2.23 35.44Ta 6.89 −2.57 12.11W 2.45 −0.69 06.22Ag 22.26 −9.48 22.03Al 15.82 −5.73 35.34Cu 15.25 −6.39 13.23Ni 7.75 −2.98 8.05Pb 94.57 −43.56 67.11Pd 13.63 −5.95 13.94Pt 7.34 −3.08 13.07C 1.10 −1.51 1.92Ge 9.80 −2.68 15.00Si 7.67 −2.14 12.54MgO 4.05 −0.94 6.60MnO 7.19 −2.52 12.66LiF 11.65 −3.43 15.71KCl 26.00 −2.85 158.6NaCl 22.80 −4.66 78.62ZnS 18.77 −7.24 21.65InP 16.48 −5.94 21.74GaAs 11.72 −3.65 16.82Source: W. Boas and J. K. MacKenzie, Progress in Metal Physics, Vol. 2, Pergamon, 1950. e2 /σx = (1/6)s12 + (1/6)s11 + (2/3)s12 = (1/6)s11 + (5/6)s12 , e3 /σx = (1/6)s12 + (1/6)s12 + (2/3)s11 = (2/3)s11 + (1/3)s12 , γ23 /σx = γ31 /σx = (1/3)s44 , γ12 /σx = (1/6)s44 . Using Equation (1.27), transform these strains onto the x, y, and z axes, ex = (1/6)e1 + (1/6)e2 + (2/3)e3 + (1/3)γ23 + (1/3)γ31 + (1/6)γ12 = [1/6)s11 + (1/2)s12 + (1/4)s44 ]/σx , e y = (1/3)e1 + (1/3)e2 + (1/3)e3 − (1/3)γ23 − (1/3)γ31 + (1/3)γ12 = [(1/3)s11 + (2/3)s12 + (1/6)s44 ]/σx , ez = (1/2)e1 + (1/2)e2 − (1/2)γ23 = [(1/6)s11 + (5/6)s12 − (1/6)s44 ]/σx . Young’s modulus is E[112] = (ex /σ x )−1 = [(1/6)s11 + (1/2)s12 + (1/4)s44 ]−1 . There are two values of Poisson’s ratio: υ y = −ey /ex and υ z = −ez /ex . υ y = −e y /ex = −[(1/3)s11 + (2/3)s12 + (1/6)s44 ]/[(1/6)s11 + (1/2)s12 + (1/4)s44 ] = −(s11 + 8s12 + 2s44 )/(2s11 + 6s12 + 3s44 ), υz = −ez /ex = −[(1/6)s11 + (5/6)s12 − (1/6)s44 ]/[(1/6)s11 + (1/2) + (1/4)s44 ] = −(2s11 + 10s12 − 2s44 )/(2s11 + 6s12 + 3s44 ).
- 49. ELASTICITY 31 3 dFigure 2.8. Coordinate system for ﬁnding Ed . In this γﬁgure α, β, and γ are the direction cosines of theangles indicated. α β 2 1Orientation dependence in cubic crystals. A similar treatment can be used to ﬁndthe effective Young’s modulus, Ed , along any direction d. Consider a cubic crystal loadedunder a single tensile stress, σ d , applied along the d-direction. Let the direction cosinesof d with the 1, 2, and 3 axes be α, β, and γ as shown in Figure 2.8. The stresses alongthe cubic axes are then σ1 = α 2 σd σ23 = βγ σd σ2 = β σd σ31 = γ ασd 2 (2.15) σ3 = γ 2 σd σ12 = αβσd .From Equation (2.13) for cubic crystals, the corresponding strains are e1 /σd = s11 α 2 + s12 β 2 + s12 γ 2 , γ23 /σd = s44 βγ , e2 /σd = s12 α 2 + s11 β 2 + s12 γ 2 , γ31 /σd = s44 γ α, (2.16) e3 /σd = s12 α + s12 β + s11 γ , 2 2 2 γ12 /σd = s44 αβ.Resolving these components onto the d-axis using Equation (1.27a), ed /σd = α 2 e1 + β 2 e2 + γ 2 e3 + βγ ·γ23 + γ α·γ31 + αβ·γ12 , (2.17)and substituting Equation (2.14) into Equation (2.15), ed /σd = s11 (α 4 + β 4 + γ 4 ) + 2s12 (β 2 γ 2 + γ 2 α 2 + α 2 β 2 ) + s44 (β 2 γ 2 + γ 2 α 2 + α 2 β 2 ) = s11 (α 4 + β 4 + γ 4 ) + (2s12 + s44 )(β 2 γ 2 + γ 2 α 2 + α 2 β 2 ). (2.18)Substituting the identity, α 2 + β 2 + γ 2 = 1, in the form of (α 4 + β 4 + γ 4 ) = 1 − 2(β 2 γ 2 +γ 2 α 2 + α 2 β 2 ) into Equation (2.18), 1/E d = ed /σd = s11 + (−2s11 + 2s12 + s44 )(β 2 γ 2 + γ 2 α 2 + α 2 β 2 ). (2.19)If d is expressed by direction indices, [hkl ], α = h/ h 2 + k 2 + l 2 , β = k/ h 2 + k 2 + l 2 , γ = l/ h 2 + k 2 + l 2 .Then Equation (2.19) can be rewritten as 1/E d = s11 + (2s12 − 2s11 + s44 )(k 2l 2 + l 2 h 2 + h 2 k 2 )/(h 2 + k 2 + l 2 )2 . (2.20)
- 50. 32 MECHANICAL BEHAVIOR OF MATERIALSFor an isotropic material, Ed is independent of direction. Equations (2.19) and (2.20)indicate that this is possible only if (2s12 − 2s11 + s44 ) = 0. Therefore for isotropy s44 = 2(s11 − s12 ). (2.21) According to Equation (2.19), the extreme values of E in a cubic crystal occur for the[100] direction (α = β = γ = 0) and for the [111] direction (α = β = γ = 0 1/(α =β = γ = 1/ 3). Because 1/E[100] = s11 and 1/E[111] = (s11 + 2s12 + s44 )/3, the ratio isgiven by E [111] /E [100] = 3s11 /(s11 + 2s12 + s44 ). (2.22)This ratio represents the largest possible anisotropy in cubic crystals. Table 2.3 givesthe E[111] /E[100] ratios for several cubic crystals. For most, E111 > E100 , but there areexceptions. For Mo, Nb, Cr, and the alkali halides E100 > E111 . Tungsten is almostelastically isotropic. The orientation dependence in Equation (2.19) can be expressed as 1/E d = 1/E 100 + f [1/E 111 − 1/E 100 ], (2.23)where f = 3(β 2 γ 2 + γ 2 α 2 + α 2 β 2 ). The orientation dependence of Ed is plotted in Figure2.9 on the basic orientation triangle (see Appendix B for plotting of angles.)Orientation dependence in noncubic crystals. Similar expressions can be derived forother crystal classes. For hexagonal crystals, 1/E = (1 − γ 2 )s11 + γ 4 s33 + γ 2 (1 − γ 2 )(2s13 + s44 ), (2.24)Table 2.3. Values of E[111] /E[100] for several cubic crystalsMaterial E[111] /E[100]Cr 0.76Mo 0.92W 1.01Cu 2.91Si 1.44KCl 0.44ZnS 2.17Fe 2.14Nb 0.52Al 1.20Ni 2.36MgO 1.39NaCl 0.74GaAs 1.66Note: Values calculated from Table 2.2.
- 51. ELASTICITY 33 [111] 0.9 30 0.8 0.6 20 0.4 φ 0.2 10[100] [110] 0 15 30 45 θFigure 2.9. Contour plot of f in 1/Ed = 1/E100 + f [1/E111 −1/E100 ]. The extremes of E are found at the [100]and [111] orientations. From W. F. Hosford, The Mechanics of Crystals and Textured Polycrystals, copyright1993 by Oxford University Press. Inc. Used with permission of Oxford University Press, Inc.where γ is the cosine of the angle between the direction d and the c-axis (Figure 2.10).For orthorhombic crystals, s11 α 4 + s22 β 4 + s33 γ 4 + β 2 γ 2 (2s23 + s44 ) + γ 2 α 2 (2s31 + s55 ) + α 2 β 2 (2s12 + s66 ). (2.25) Example problem 2.6: Pressure, p, affects the c/a ratio of hexagonal crystals. Write an expression for d(c/a)/dp in terms of the elastic constants and c/a. Assume that σ 1 = σ 2 = σ 3 = −p. SOLUTION: d(c/a) = (adc − cda)/a2 = (c/a)(dc/c − da/a) = (c/a)(de3 − de1 ). Now substituting de1 = s11 dσ1 + s12 dσ2 + s13 dσ3 = −(s11 + s12 + s13 )d p and de3 = s13 dσ1 + s13 dσ2 + s33 dσ3 = −(2s13 + s33 )d p, d(c/a)/d p = −(c/a)(2s13 + s33 − s11 − s12 − s13 ) = −(c/a)(s13 + s33 − s11 − s12 ). c dFigure 2.10. Hexagonal cell showing the c-axis anda direction d. The dimensions of the cell are a and c. c γ a
- 52. 34 MECHANICAL BEHAVIOR OF MATERIALSOrientation dependence in materials other than single crystals. The basic formsof the elastic constant matrix can be used for materials that are not single crystals, butthat have similar symmetries of structure and properties. Such materials may be eithernatural or artiﬁcial composites. Examples include:1. Orthotropic (same as orthorhombic) symmetry (three axes of twofold symmetry): a. Rolled sheets or plates, both before and after recrystallization. The anisotropy is caused by crystallographic texture. The axes are the rolling, transverse, and thickness directions. b. Tubes and swaged wires or rods having cylindrical crystallographic textures. The axes are the radial, tangential (hoop), and axial directions. c. Wood. The axes are the radial, tangential, and axial directions.2. Tetragonal symmetry (one axis of four-fold symmetry, two axes of two-fold symmetry): a. Plywood with equal numbers of plies at 0◦ and 90◦ . The four-fold axis is normal to the sheet and the two two-fold axes are parallel to the wood grain in the two plies. The anisotropy is from oriented ﬁbers. b. Woven cloth, window screen, and composites reinforced with woven material if the cloth or screen has the same weft and warp (the two directions of thread in a woven cloth). The four-fold axis is normal to the cloth and the two two-fold axes are parallel to the threads of the weft and warp3. Axial symmetry (same as hexagonal symmetry): a. Drawn or extruded wire and rod. The anisotropy is caused by a ﬁber texture, all directions normal to the wire axis being equivalent. b. Electroplates and portions of ingots with columnar grains. All directions normal to the growth direction are equivalent. c. Uniaxially aligned composites. The axis of symmetry is parallel o the ﬁbers. In principle it should be possible to obtain the elastic moduli for a polycrystal froma weighted average of the elastic behavior of all orientations of crystals present in thepolycrystal. However, the appropriate way to average is not obvious.Anisotropic thermal expansion. As in the isotropic case, small-dimensional changescaused by temperature changes can be treated as strains, eij = α ij T, where α ij is the linearcoefﬁcient of thermal expansion and Hooke’s laws can be generalized to include theseterms. In the most general case, the thermal expansion coefﬁcients form a symmetrictensor, α11 α21 α31 α12 α22 α32 (2.26) α13 α23 α33
- 53. ELASTICITY 35Table 2.4. Coefﬁcients of thermal expansion for some noncubic crystals Temp. range α11 α22 α33Material Struct. (◦ C) (m/m)/K (m/m)/K (m/m)/Kzirconium hcp 300 to 900 5.7 α 22 = α 11 11.4zinc hcp 0 to 100 15.0 α 22 = α 11 61.5magnesium hcp 0 to 35 24.3 α 22 = α 11 27.1cadmium hcp at 0 19.1 α 22 = α 11 54.3titanium hcp 0 to 700 11.0 α 22 = α 11 12.8tin tetr. at 50 16.6 α 22 = α 11 32.9calcite hex. 0 to 85 −5.6 α 22 = α 11 25.1uranium ortho. at 75 20.3 −1.4 22.2where the subscripts on the a terms refer to the crystal axes, 1, 2, 3, and are the same ason the corresponding strain component. Using a shorter notation system, e1 = α1 T, e2 = α2 T, e3 = α3 T, (2.27)and γ23 = α4 T, γ31 = α5 T, γ12 = α6 T,where α1 = α11 , α2 = α22 , α3 = α33 , α4 = 2α23 , α5 = 2α31 , and α6 = 2α12 .There are simpliﬁcations for crystals of higher symmetry:1. Cubic: α 1 = α 2 = α 3 , α 4 = α 5 = α 6 = 0.2. Hexagonal and tetragonal: α 1 = α 2 = α 3 , α 4 = α 5 = α 6 = 0.3. Orthorhombic crystals: α 1 = α 2 = α 3 , α 4 = α 5 = α 6 = 0.The coefﬁcients of thermal expansion for some noncubic crystals are given in Table 2.4.NOTESRobert Hooke (1635–1703) was appointed curator of experiments of the Royal Society on therecommendation of Robert Boyle. In that post he devised apparatus to clarify points of discussionas well as to demonstrate his ideas. He noted that when he put weights on a string or a spring, itsdeﬂection was proportional to the weight. Hooke was a contemporary of Isaac Newton, whom heenvied. Several times he claimed to have discovered things attributed to Newton, but was neverable to substantiate these claims. Thomas Young (1773–1829) studied medicine, but because of his interest in science, he took apost as lecturer at the Royal Institution. In his lectures, he was the ﬁrst to deﬁne the concept of amodulus of elasticity, although he deﬁned it quite differently than we do today. He described themodulus of elasticity in terms of the deformation at the base of a column due to its own weight. Claude-Louis-Marre-Henri Navier (1785–1836) wrote a book in 1826 on the strength of mate-rials, in which he deﬁned the elastic modulus in terms of the load per unit cross-sectional areaand determined E for iron. Because his family was poor, S. D. Poisson (1781–1840) did not have a chance to learn to reador write until he was 15. After two years of visiting mathematics classes, he passed the exams foradmission to the Ecole Polytechnique with distinction. He realized that axial elongation, ε, mustbe accompanied by lateral contraction, which he took as (−1/4)ε, not realizing that the ratio ofcontractile strain to elongation strain is a property that varies from material to material.
- 54. 36 MECHANICAL BEHAVIOR OF MATERIALSREFERENCESH. B. Huntington, The Elastic Constants of Crystals, Academic Press, 1964.W. K¨ ster and H. Franz, Met. Rev., Vol. 6 (1961), pp. 1–55. oG. Simons and H. Wang, Single Crystal Elastic Constants and Calculated Properties – A Handbook, MIT Press, 1971.PROBLEMS 1. Reconsider Problem 4 in Chapter 1 and assume that E = 205 GPa and υ = 0.29. A. Calculate the principal stresses under load. B. Calculate the strain, ε z . 2. Consider a thin-walled tube, capped at each end and loaded under internal pres- sure. Calculate the ratio of the axial strain to the hoop strain, assuming that the deformation is elastic. Assume that E = 107 psi and υ = 1/3. Does the length of the tube increase, decrease, or remain constant? 3. A sheet of metal was deformed elastically under balanced biaxial tension (σ x = σ y , σ z = 0) A. Derive an expression for the ratio of elastic strains, ez /ex , in terms of the elastic constants. B. If E = 70 GPa and υ = 0.30, and ey is measured as 1.00 × 10−3 , what is the value of ez ? 4. A cylindrical plug of a gummite * is placed in a cylindrical hole in a rigid block of stifﬁte.* Then the plug is compressed axially (parallel to the axis of the hole). Assume that the plug exactly ﬁts the hole and that the stifﬁte does not deform at all. Assume elastic deformation and that Hooke’s law holds. Derive an expression for the ratio of the axial strain to the axial stress, ε a /σ a , in the gummite in terms of the Young’s modulus, E, and Poisson’s ratio, υ, of the gummite. 5. Strain gauges mounted on a free surface of a piece of steel (E = 205 GPa, υ = 0.29) indicate strains of ε x = −0.00042, ε y = 0.00071, and γ xy = 0.00037. A. Calculate the principal strains. B. Use Hooke’s laws to ﬁnd the principal stresses from the principal stresses. C. Calculate σ x , σ y , and τ xy directly from εx , εy , and γ xy . D. Calculate the principal stresses directly from σ x , σ y , and τ xy and compare your answers with the answers to B. 6. A steel block (E = 30 × 106 psi and υ= 0.29) is loaded under uniaxial compression along x.* “Gummite” and “stifﬁte” are ﬁctitious names.
- 55. ELASTICITY 37 PMMA glass Figure 2.11. Laminated sheets of PMMA PMMA z and glass. y x A. Draw the Mohr’s strain circle diagram. B. There is an axis, x , along which the strain εx = 0. Find the angle between x and x . 7. Poisson’s ratio for rubber is 1/2. What does this imply about the bulk modulus? 8. A sandwich is made of a plate of glass surrounded by two plates of polymethyl- methacrylate as shown in Figure 2.11. Assume that the composite is free of stresses at 40◦ C. What are the stresses when the sandwich is cooled to 20◦ C? The prop- erties of the glass and the polymethylmethacrylate are given below. The total thicknesses of the glass and the PMMA are equal. Assume each to be isotropic and assume that creep is negligible. Glass PMMA −1 −6 thermal expansion coefﬁcient (K ) 9. × 10 90. × 10−6 Young’s modulus (GPa) 69. 3.45 Poisson’s ratio 0.28 0.38 9. A bronze sleeve, 0.040 in. thick, was mounted on a 2.000-in. diameter steel shaft by heating it to 100◦ C, while the temperature of the shaft was maintained at 20◦ C Under these conditions, the sleeve just ﬁt on the shaft with zero clearance. Find the principal stresses in the sleeve after it cools to 20◦ C. Assume that friction between the shaft and the sleeve prevents any sliding at the interface during cooling, and assume that the shaft is so massive and stiff that strains in the shaft itself are negligible. For the bronze, E = 16 × 106 psi, υ = 0.30, and α = 18.4 × 10−6 (◦ C)−1 .10. Calculate Young’s modulus for an iron crystal when tension is applied along a <122> direction.11. Zinc has the following elastic constants: s11 = 0.84 × 10−11 Pa−1 ; s33 = 2.87 × 10−11 Pa−11 ; s12 = 0.11 × 10−11 Pa−1 ; s13 = −0.78 × 10−11 Pa−1 ; s44 = 2.64 × 10−11 Pa−11 ; s66 = 2(s11 − s12 ). Find the bulk modulus of zinc.12. Calculate the effective Young’s modulus for a cubic crystal loaded in the [110] direction in terms of the constants s11 , s12 , and s44 . Do this by assuming uniaxial tension along [110] and expressing σ 1 , σ 2 , . . .,τ 12 in terms of σ [110] . Then use the
- 56. 38 MECHANICAL BEHAVIOR OF MATERIALS matrix of elastic constants to ﬁnd e1 , e2 , . . .,γ 12 , and ﬁnally resolve these strains onto the [110] axis to ﬁnd e[110] .13. When a polycrystal is elastically strained in tension, it is reasonable to assume that the strains in all grains are the same. Using this assumption, calculate for iron the ratio of the stress in grains oriented with <111> parallel to the tensile axis to the average stress, σ 111 /σ av = E111 /Eav . Calculate σ 100 /σ av .14. Take the cardboard back of a pad of paper and cut it into a square. Then support the cardboard horizontally with blocks at each end and apply a weight in the middle. Measure the deﬂection. Next rotate the cardboard 90◦ and repeat the experiment using the same weight. By what factor do the two deﬂections differ? By what factor does the elastic modulus, E, vary with direction? Why was the cardboard used for the backing of the pad placed in the orientation that it was?
- 57. 3 Tensile TestingIntroductionTensile test data have many uses. Tensile properties are used in selecting materials forvarious applications. Material speciﬁcations often include minimum tensile propertiesto ensure quality. Tests must be made to ensure that materials meet these speciﬁcations.Tensile properties are also used in research and development to compare new materialsor processes. With plasticity theory, tensile stress–strain curves can be used to predict amaterial’s behavior under forms of loading other than uniaxial tension. Often the primary concern is strength. The level of stress that causes appreciableplastic deformation of a material is called its yield stress. The maximum tensile stressthat a material carries is called its tensile strength (or ultimate strength or ultimate tensilestrength). Both of these measures are used, with appropriate caution, in engineeringdesign. A material’s ductility is also of interest. Ductility is a measure of how muchthe material can deform before it fractures. Rarely, if ever, is the ductility incorporateddirectly into design. Rather it is included in speciﬁcations to ensure quality and toughness.Elastic properties may be of interest, but these are measured ultrasonically much moreaccurately that by tension testing.Tensile specimensFigure 3.1 shows a typical tensile specimen. It has enlarged ends or shoulders for gripping.The important part of the specimen is the gauge section. The cross-sectional area of thegauge section is less than that of the shoulders and grip region, so the deformation willoccur here. The gauge section should be long compared to the diameter (typically fourtimes). The transition between the gauge section and the shoulders should be at least asgreat as the diameter so that the larger ends do not constrain the deformation in the gaugesection. There are several ways of gripping specimens, as shown in Figure 3.2. The ends maybe screwed into threaded grips, pinned, or held between wedges. Specimens with buttends use special grips. The gripping system should ensure that the maximum load can be 39
- 58. 40 MECHANICAL BEHAVIOR OF MATERIALS shoulder diameter, d gauge length x≥dFigure 3.1. Typical tensile specimen with a reduced gauge section and larger shoulders. a b c d e split collar serratedthreaded wedgesgrip serrated wedges pinFigure 3.2. Systems for gripping tensile specimens. For round specimens these include threaded grips (a),serrated wedges (b), and split collars for butt-end specimens (c). Sheet specimens may be gripped by pins(d) or by serrated wedges (e). From W. F. Hosford in Tensile Testing, ASM Int. 1992.applied without slippage or appreciable deformation in the grip region. Bending shouldbe minimized.Stress–strain curves. A tension test involves mounting a specimen in a machine, ex-tending it, and recording how the tensile force changes as the specimen is elongated.Figure 3.3 is a typical engineering stress–strain curve for a ductile material. For small strains the deformation is elastic and reverses if the load is removed. Athigher stresses plastic deformation occurs. This is not recovered when the load is removed.Bending a wire or paper clip with the ﬁngers (Figure 3.4) illustrates the difference. Ifthe wire is bent a small amount it will snap back when released. However, if the bend ismore severe, it will only partly recover, leaving a permanent bend. The onset of plastic
- 59. TENSILE TESTING 41 40,000 Engineering Stress (psi) 30,000Figure 3.3. Typical engineering stress– 20,000strain curve for a ductile material. 10,000 0 0.0 0.1 0.2 0.3 0.4 0.5 Engineering Straindeformation is usually associated with the ﬁrst deviation of the stress–strain curve fromlinearity * . It is tempting to deﬁne an elastic limit as the stress that causes the ﬁrst plastic defor-mation and to deﬁne a proportional limit as the ﬁrst departure from linearity. However,neither deﬁnition is very useful because they both depend on accuracy of measurement.The more accurate the strain measurement is, the lower is the stress at which plasticdeformation and nonlinearity can be detected. To avoid this problem, the onset of plasticity is usually described by an offset yieldstrength that can be measured with more reproducibility. It is found by constructing astraight line parallel to the initial linear portion of the stress–strain curve, but offset fromit by e = 0.002 (0.2%.) The yield strength is taken as the stress level at which this straightline intersects the stress–strain curve (Figure 3.5). The rationale is that if the materialhad been loaded to this stress and then unloaded, the unloading path would have beenalong this offset line, resulting in a plastic strain of e = 0.002 (0.2%). The advantageFigure 3.4. Using the ﬁngers to sense the elastic andplastic responses of a wire. With a small force (top)all bending is elastic and disappears when the forceis released. With a greater force (below), the elasticpart of the bending is recoverable but the plastic partis not. From W. F. Hosford, ibid.* For some materials, there may be nonlinear elastic deformation.
- 60. 42 MECHANICAL BEHAVIOR OF MATERIALS 200 150 Engineering Stress, MPa 0.2% offset yield strength 100 Figure 3.5. The low-strain region of the stress–strain curve for a ductile material. From W. F. Hosford, ibid. 50 0.002 0.2% 0 0 0.01 0.02 Engineering Strainof this way of deﬁning yielding is that it is easily reproduced. Occasionally other offsetstrains are used and or yielding is deﬁned in terms of the stress necessary to achievea speciﬁed total strain (e.g., 0.5%) instead of a speciﬁed plastic strain. In all cases thecriterion should be made clear to the user of the data. Yield points: The stress–strain curves of some materials (e.g., low carbon steelsand linear polymers) have an initial maximum followed by a lower stress, as shown inFigure 3.6. After the initial maximum, at any given instant all of the deformation occurswithin a relatively small region of the specimen. For steels this deforming region is calleda L¨ der’s band. Continued elongation occurs by propagation of the L¨ der’s band along u uthe gauge section, rather than by continued deformation within it. Only after the band upper yield strength 30Engineering stress, 1000 psi Engineering stress, psi 2000 lower yield strength 20 1000 10 0 0 0 2 4 6 0 0.01 0.02 0.03 Engineering strain Engineering strainFigure 3.6. Inhomogeneous yielding of low carbon steel (left) and a linear polymer (right). After the initialstress maximum, the deformation in both materials occurs within a narrow band that propagates the lengthof the gauge section before the stress rises again.
- 61. TENSILE TESTING 43 engineering stressFigure 3.7. After a maximum on the stress–straincurve, deformation localizes to form a neck. engineering strainhas traversed the entire gauge section does the stress rise again. In the case of linear poly-mers, the yield strength is usually deﬁned as the initial maximum stress. For steels, thesubsequent lower yield strength is used to describe yielding. The initial maximum stressis too sensitive to specimen alignment to be useful. Even so, the lower yield strength issensitive to the strain rate. ASTM standards should be followed. The stress level duringL¨ der’s band propagation ﬂuctuates. Some laboratories report the minimum level as the uyield strength and other use the average level. As long as the engineering stress–strain curve rises, the deformation will occur uni-formly along the length. For a ductile material the stress will reach a maximum wellbefore fracture. When the maximum is reached, the deformation localizes, forming aneck, as shown in Figure 3.7. The tensile strength (or ultimate strength) is deﬁned as the highest value of theengineering stress (Figure 3.8). For ductile materials, the tensile strength corresponds tothe point at which necking starts. Less ductile materials fracture before they neck. In thiscase, the fracture stress is the tensile strength. Very brittle materials (e.g., glass) fracturebefore they yield. Such materials have tensile strengths, but no yield stresses.Ductility. Two common parameters are used to describe the ductility of a material. Thepercent elongation is simply deﬁned as %El = (L f − L o )/L o × 100%, (3.1)where Lo is the initial gauge length and Lf is the length of the gauge section at fracture.Measurements may be made on the broken pieces or under load. For most materials, theEngineering stress Engineering stress Engineering stress Tensile strength Tensile strength Tensile strength Engineering strain Engineering strain Engineering strainFigure 3.8. The tensile strength is the maximum engineering stress, regardless of whether the specimennecks or fractures before necking. From W. F. Hosford, ibid.
- 62. 44 MECHANICAL BEHAVIOR OF MATERIALSelastic elongation is so small compared to the plastic elongation that it can be neglected.When this is not so, as with brittle materials or with rubber-like materials, it should bemade clear in reporting whether the percent elongation includes the elastic portion. The other common measure of ductility is the percent reduction of area at fracture,deﬁned as %RA = (Ao − Af )/Ao × 100%, (3.2)where Ao is the initial cross-sectional area and Af is the cross-sectional area of the fracture.If the failure occurs before the necking, the %El can be calculated from the %RA byassuming constant volume. In this case %El = %RA/(100 − %RA) × 100%. (3.3)The %El and %RA are no longer directly related after a neck has formed. Percent elongation, as a measure of ductility, has the disadvantage that it combines theuniform elongation that occurs before necking and the localized elongation that occursduring necking. The uniform elongation depends on the plastic behavior rather than thefracture behavior. The necking elongation is sensitive to the specimen shape. If the gaugesection is very long compared to the diameter, the contribution of necking to the totalelongation is very small. On the other hand, if the gauge section is very short, the neckingelongation accounts for most of the elongation. For round bars, this problem has beenremedied by standardizing the ratio of the gauge length to the diameter at 4:1. However,there is no simple relation between the percent elongation of such standardized roundbars and the percent elongation measured on sheet specimens or wires. Percent reduction of area, as a measure of ductility, does not depend on the ratio ofthe gauge length to the diameter. However, for very ductile materials, it is difﬁcult tomeasure the ﬁnal cross-sectional area, especially with sheet specimens.True stress and strain. If the tensile tests are used to predict how the material willbehave under other forms of loading, true stress–true strain curves are useful. The truestress is deﬁned as σ = F/A, (3.4)where A is the instantaneous cross-sectional area corresponding to the force F. Beforenecking begins, the true strain is given by ε = ln(L/L o ). (3.5)The engineering stress is deﬁned as the force divided by the original area, s = F/Ao , andthe engineering strain is deﬁned as the change in length divided by the original length,e = L/Lo . As long as the deformation is uniform along the gauge length, the true stressand true strain can be calculated from the engineering quantities. With constant volume,LA = Lo Ao , so that Ao /A = L/L o , (3.6)
- 63. TENSILE TESTING 45 1000Figure 3.9. Comparison of engineering σ−ε 800and true stress–strain curves. Before ε = n(1+e)necking, a point on the true stress–straincurve (σ –ε) can be constructed from a 600 σ = s(1+e) stresspoint on the engineering stress–strain s −ecurve (s–e) with Equations (3.7) and (3.8). 400After necking, the cross-sectional area atthe neck must be measured to ﬁnd the 200true stress and strain. 0 0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 strainand thus Ao /A = 1 + e. Rewriting Equation (3.4) as σ = (F/Ao )(Ao /A) and substitutingAo /A = 1 + e and s = F/Ao , σ = s(1 + e). (3.7)Substitution of L/Lo = 1 + e into Equation (3.5) gives ε = ln(1 + e). (3.8) These expressions are valid only if the deformation is uniformly distributed along thegauge section. After necking starts, Equation (3.4) is still valid for true stress, but thecross-sectional area at the base of the neck must be measured independently. Equation(3.5) could still be used if L and Lo were known for a gauge section centered on themiddle of the neck and so short that the variations of area along its length were negligible.Equation (3.6) would be valid over such a gauge section, so the true strain can be calculatedas ε = ln(Ao /A), (3.9)where A is the area at the base of the neck. Figure 3.9 shows the comparison of theengineering and true stress–strain curves for the same material. Example problem 3.1: In a tensile test, a material fractured before necking. The true stress and strain at fracture were 630 MPa and 0.18 respectively. What is the tensile strength of the material? SOLUTION: The engineering strain at fracture was e = exp(0.18) − 1 = 0.197. Because s = σ /(1 + e), the tensile strength = 630/1.197 = 526 MPa.The Bridgman correction. The state of stress at the center of a neck is not uniaxialtension. As material in the center of the neck is being stretched in the axial direction, itmust contract laterally. This contraction is resisted by the adjacent regions immediatelyabove and below that have larger cross sections and are therefore not deforming. The net
- 64. 46 MECHANICAL BEHAVIOR OF MATERIALS 1.5 σz 1.25 σz(av) 1 σzσ/σ R 0.75 r σy σx 0.5 σx = σy a 0.25 0 -1 0 1 r/aFigure 3.10. The stress distribution across a neck (left) and the corresponding geometry of the neck (right).Both axial and lateral tensile stresses are at a maximum at the center of the neck.effect is that the center of a neck is under triaxial tension. Figure 3.10 shows the stressdistribution calculated by Bridgman. Only the part of the axial stress that exceeds the lateral stress is effective in causingyielding. Bridgman showed that the effective part of the stress, σ , is σ /σ = 1/[(1 + 2R/a) ln(1 + a/2R)], (3.10)where σ is the measured stress, F/A, a = D/2 is the radius of the specimen at the baseof the neck, and R is the radius of curvature of the neck proﬁle. Figure 3.11 is a plot of the Bridgman correction factor, σ /σ , as a function of a/Raccording to Equation (3.10). The radius of curvature, R, can be measured by sliding acalibrated cone along the neck until it becomes tangent at the base of the neck. 1.00 Bridgman Correction 0.95 a 0.90 Rσ/σ-- 0.85 0.80 0.75 0.0 0.5 1.0 1.5 a/RFigure 3.11. The Bridgman correction factor as a function of the neck shape. The plot gives the ratio of theeffective stress to the axial true stress for measured values of a/R.
- 65. TENSILE TESTING 47Temperature rise. Most of the mechanical energy expended by the tensile machine isliberated as heat in the tensile specimen. If the testing is rapid, little of the heat is lostto the surroundings and the temperature rise can be surprisingly high. With very slowtesting most of the heat is dissipated to the surroundings, so the temperature rise is muchless. Example problem 3.2: Calculate the temperature rise in a tension test of a low-carbon steel after a tensile elongation of 22%. Assume that 95% of the energy goes to heat and remains in the specimen. Also assume that Figure 3.3 represents the stress–strain curve of the material. For steel, the heat capacity is 447 J/kg K and the density is 7.88 Mg/m3 . SOLUTION: The heat released equals 0.95 s de. From Figure 3.3, s de = sav e = about 34 × 0.22 ksi = 51.6 MPa = 61.6 MJ/m3 . T = Q/C where Q = 0.95(61.6 × 106 J/m3 ) and C is heat capacity per volume = (7.8 × 103 kg/m3 )(447 J/kg/K). Substituting, T = 0.95(61.6 × 106 J/m3 )/[(7.8 × 103 kg/m3 )(447 J/kg/K)] = 17◦ C. This is a moderate temperature rise. For high–strength materials the rise can be much higher.Sheet anisotropy. The angular variation of yield strength in many sheet materials is notlarge. However, such a lack of variation does not indicate that the material is isotropic.The parameter that is commonly used to characterize the anisotropy is the strain ratioor R-value∗ (Figure 3.12). This is deﬁned as the ratio, R, of the contractile strain in thewidth direction to that in the thickness direction during a tension test, R = ε w /ε t . (3.11)In an isotropic material, the width and thickness strains, ε w and εt , are equal, so the valueof R for an isotropic material is 1; however, R is usually either greater or less than 1 in realsheet materials. Direct measurement of the thickness strain in thin sheets is inaccurate. rolling directionFigure 3.12. Tensile specimen cut from a sheet (left).The R-value is the ratio of the lateral strains, ε w /ε t , εw θ εtduring the extension (right).∗ Some authors use the symbol r instead of R.
- 66. 48 MECHANICAL BEHAVIOR OF MATERIALSInstead, εt is usually deduced from the width and length strains assuming constancy ofvolume, εt = −ε w − ε l : R = −ε w /(εw + εl ). (3.12) To avoid constraint from the shoulders, strains should be measured well away fromthe ends of the gauge section. Some workers suggest that the strains be measured whenthe total elongation is 15%, if this is less than the necking strain. The change of R duringa tensile test is usually quite small and the lateral strains at 15% elongation are greatenough to be measured with accuracy. Example problem 3.3: Consider the accuracy of R measurement for a material having an R of about 1.00. Assume the width is about 0.5 in and can be measured to an accuracy of ±0.001 in., which corresponds to an uncertainty of strain of ±0.001/0.5 = ±0.002. The errors in measuring the length strain are much smaller. Estimate the error in ﬁnding R if the total strain were 5%. How would this be reduced if the total strain were 15%? SOLUTION: At an elongation of 5%, the lateral strain would be about 0.025, so an error of ±0.002/0.025 = 8%. If the R-value were 1, this would cause an error in R of approximately 0.08 × 0.5/(1 − 0.5) or 8%. At 15% elongation, the percent error should be about one-third of this or roughly ±3%.The value of R usually depends on the direction of testing. An average R-value is con-ventionally taken as R = (R0 + R90 + 2R45 )/4. (3.13)The angular variation of R is characterized by R, deﬁned as R = (R0 + R90 − 2R45 )/2. (3.14)Both of these are important in analyzing what happens during sheet metal forming.Measurement of force and strain. In most tensile testing machines, the force is appliedthrough load cells. The load cell is built so that it will deform elastically under the appliedloads. The amount of elastic deformation is sensed and converted to an electrical signal,which in turn may be recorded electronically or used to drive a recording pen. Several methods may be used to measure strain. With ductile polymers and metals,the deformation is often so great that it may be calculated from the crosshead movement.In this case no direct measurements on the specimen are required. With screw-drivenmachines, the crosshead movement can be deduced from time. If it is assumed that all thecrosshead displacement corresponds to specimen elongation, the engineering strain issimply the crosshead displacement divided by the gauge length. This procedure ignoresthe fact that some of the crosshead movement corresponds to elastic distortion of themachine and the gripping system as well as some plastic deformation in the shouldersof the specimen. The machine displacements can be found as a function of the load by
- 67. TENSILE TESTING 49Figure 3.13. Nonaxiality can result from off-centerloading (a). With the bending caused by off-centerloading, strain measurements on the outside ofthe bend will be higher than the centerline strain.Straightening of an initially bent specimen (b) willcause measurements of strain on the outside of thebend to be lower than the strain at the centerline.From W. F. Hosford, ibid.running a calibration experiment with a known specimen. Subtracting these machinegrip displacements from the crosshead displacement will increase the accuracy of themethod. For small strains, much greater accuracy can be achieved with an extensometer at-tached to the specimen. An extensometer is a device speciﬁcally designed to measuresmall displacements by using resistance strain gauges, differential capacitances, or differ-ential inductances. The change in resistance, capacitance, or inductance is converted toan electrical signal, which in turn controls a pen or paper drive or is stored in a computerﬁle.Axial alignment. For measurement of strains in the elastic region, substantial errorsmay result from the use of a single extensometer unless the specimen is very straightand axially aligned. Nonaxial alignment and specimen curvature have analogous effectsduring loading, causing a bending or unbending of the specimen as sketched in Fig-ure 3.13. The extensometer will respond to the bending as well as the axial elongation. Asimple way of compensating for bending and misalignment is to mount two extensometerson opposite sides of the specimen. The averaged response will not be affected by thebending. Axiality of loading is of particular importance during the testing of brittle materials.In bending, the load on one side of the specimen is higher than that on the opposite side,but the average stress deduced from the load will be less than the stress on the moreheavily stressed side. Thus, the recorded tensile strength will be lower than the actualstress at the location where the fracture initiates. With low carbon steels, nonaxial loadingmay mask the upper yield point. With ductile materials, nonaxiality is not a problem afterthe initial yielding because the specimens straighten during the ﬁrst plastic deformation.Special problemsIn testing of wire or rope, there is no simple way to use a reduced gauge section. Insteadthe wire or rope is wound around a drum so that friction provides the gripping. Whenspecimens are tested at high or low temperatures, the entire gauge section should be atthe test temperature. For low-temperature testing, the specimen can be immersed in a
- 68. 50 MECHANICAL BEHAVIOR OF MATERIALS Figure 3.14. Leonardo’s sketch of a system for ten- sile testing of wire. The load was applied by pouring sand into a basket suspended from the wire.constant-temperature liquid bath. For testing at elevated temperatures, the specimen isusually surrounded by a controlled furnace.NOTESLeonardo da Vinci (1452–1519) described a tensile test of a wire. Fine sand was fedthrough a small hole into a basket attached to the lower end of the wire until the wirebroke. Figure 3.14 shows his sketch of the apparatus. Galileo Galilei (1564–1642) stated that the strength of a bar in tension was propor-tional to its cross-sectional area and independent of its length. Petrus von Musschenbr¨ k o(1692–1761) devised the tensile testing machine and grip system illustrated in Fig-ure 3.15. Percy W. Bridgman (1882–1961) was born in Cambridge, Massachusetts, and attendedHarvard, where he graduated in 1904 and received his Ph.D. in 1908. He discovered thehigh-pressure forms of ice and is reputed to have discovered “dry ice” and he wrote aclassic book, Physics of High Pressures, in 1931. In 1946 he was awarded the Nobelprize in physics for his work at high pressure. Another book, Studies in Large PlasticFlow and Fracture (1952), summarizes his work in the mechanics of solids. The yield point effect in linear polymers may be experienced by pulling the pieceof plastic sheet that holds a six-pack of carbonated beverage cans together. When onepulls hard enough the plastic will yield and the force will drop. A small thinned region E A E C F C Figure 3.15. Musschenbrok’s design ¨ D G D (1729) for a tensile testing machine that K K used a lever to increase the applied force. His system for gripping the specimen is shown at the right. E E D GB D K K C C
- 69. TENSILE TESTING 51develops. As the force is continued, this region will grow. The yield point effect in lowcarbon steel may be experienced by bending a low carbon steel wire. (Florist’s wire workswell.) First heat the wire in a ﬂame to anneal it. Then bend a six-inch length by holding itonly at the ends. Instead of bending uniformly, the deformation localizes to form severalsharp kinks. Why? Bend an annealed copper wire for comparison.REFERENCESTensile Testing, ASM International, 1992.Percy Bridgman, Studies in Large Plastic Flow and Fracture, McGraw–Hill, 1952.PROBLEMS 1. The results of a tensile test on a steel test bar are given below. The initial gauge length was 25.0 mm and the initial diameter was 5.00 mm. The diameter at the fracture was 2.6 mm. The engineering strain and engineering stress in MPa are as follows; Strain Stress Strain Stress Strain Stress 0.0 0.0 0.06 319.8 0.32 388.4 0.0002 42.0 0.08 337.9 0.34 388.0. 0.0004 83.0 0.10 351.1 0.38 386.5 0.0006 125.0 0.15 371.7 0.40 384.5 0.0015 155.0 0.20 382.2 0.42 382.5 0.005 185.0 0.22 384.7 0.44 378.0 0.02 249.7 0.24 386.4 0.46 362.0 0.03 274.9 0.26 387.6 0.47 250 0.04 293.5 0.28 388.3 0.05 308.0 0.30 388.5 A. Plot the engineering stress–strain curve. B. Determine i. Young’s modulus, ii. the 0.2% offset yield strength, iii. the tensile strength, iv. the percent elongation, and v. the percent reduction of area. 2. Construct the true stress–true strain curve for the material in Problem 1. Note that necking starts at maximum load, so the construction should be stopped at this point. 3. Determine the engineering strains, e, and the true strains, ε, for each of the following: A. Extension from L = 1.0 to L = 1.1 B. Compression from h = 1 to h = 0.9 C. Extension from L = 1 to L = 2 D. Compression from h = 1 to h = 1/2.
- 70. 52 MECHANICAL BEHAVIOR OF MATERIALS 4. The ASM Metals Handbook (Vol. 1, eighth ed., p. 1008) gives the percent elon- gation in a 2-in. gauge section for annealed electrolytic tough-pitch copper as A. 55% for a 0.505-in.-diameter bar B. 45% for a 0.030-in.-thick sheet, and C. 38.5% for a 0.010-in.-diameter wire. Suggest a reason for the differences. 5. The tensile strength of iron–carbon alloys increases as the percent carbon increases up to about 1.5 to 2%. Above this the tensile strength drops rapidly with increased percent carbon. Speculate about the nature of this abrupt change. 6. The area under an engineering stress–strain curve up to fracture is the en- ergy/volume. The area under a true stress–strain curve up to fracture is also the energy/volume. If the specimen necks, these two areas are not equal. What is the difference? Explain. 7. Suppose it is impossible to use an extensometer on the gauge section of a test specimen. Instead a butt-end specimen (Figure 3.2c) is used and the strain is computed from the cross-head movement. There are two possible sources of error in this procedure. One is that the gripping system may deform elastically and the other is that the butt end may be drawn partly through the collar. How would each of these errors affect the calculated true stress and true strain? 8. Equation (3.10) relates the average axial stress in the neck, σ , to the effective stress, σ . The variation of the local stresses with distance, r, from the center is given by σ Z = σ [1 + ln(1 + a/2R − r 2 /2a R)] with σ x = σ y = σ z − σ . Derive an expression for the level of hydrostatic stress, σ H = (σ x + σ y + σ z )/3, at the center in terms of a, R, and σ . 9. The tensile strengths of brazed joints between two pieces of steel are often con- siderably higher than the tensile strength of the braze material itself. Furthermore, the strengths of thin joints are higher than those of thick joints. Explain.10. Two strain gauges were mounted on opposite sides of a tensile specimen. Strains measured as the bar was pulled in tension were used to compute Young’s modulus. Readings from one gauge gave a modulus much higher than those from the other gauge. What was the probable cause of this discrepancy?
- 71. 4 Other Tests of Plastic BehaviorIntroductionNecking limits uniform elongation in tension, making it difﬁcult to study plastic stress–strain relationships at high strains. Much higher strains can be reached in compression,torsion, and bulge tests. The results from these tests can be used, together with the theoryof plasticity (Chapter 6), to predict stress–strain behavior under other forms of loading.Bend tests are used to avoid the problem of gripping brittle material without breakingit. Hardness tests eliminate the considerable time and effort required to machine tensilespecimens. Also, hardness tests are simple to perform and are not destructive.Compression testMuch higher strains are achievable in compression tests than in tensile tests. However,two problems limit the usefulness of compression tests: friction and buckling. Frictionon the ends of the specimen tends to suppress the lateral spreading of material near theends (Figure 4.1). A cone-shaped region of dead metal (nondeforming material) canform at each end, with the result that the specimen becomes barrel shaped. Friction canbe reduced by lubrication and the effect of friction can be lessened by increasing theheight-to-diameter ratio, h/d, of the specimen. If the coefﬁcient of friction, µ, between the specimen and the platens is constant, theaverage pressure to cause deformation is Pav = Y (1 + (µd/ h)/3 + (µd/ h)2 /12 + · · ·), (4.1)where Y is the true ﬂow stress of the material. If, on the other hand, there is a constantshear stress at the interface, such as would be obtained by inserting a thin ﬁlm of a softmaterial (e.g., lead, polyethylene, or Teﬂon), the average pressure is Pav = Y + (1/3)k (d/ h), (4.2)where k is the shear strength of the soft material. However, these equations usually donot accurately describe the effect of friction because neither the coefﬁcient of frictionnor the interface shear stress is constant. Friction is usually highest at the edges, where 53
- 72. 54 MECHANICAL BEHAVIOR OF MATERIALS dead metal dead metal Figure 4.2. Photograph of the end of a compression specimen. The darker central region was the origi- nal end. The lighter region outside was originally partFigure 4.1. Unless the ends of a compression spec- of the cylindrical wall that folded up with the severeimen are well lubricated, there will be a conical re- barreling. From G. W. Pearsall and W. A. Backofen,gion of undeforming material metal at each end of Journal of Engineering for Industry, Trans. ASME Vol.the specimen. As a consequence the midsection will 85B (1963); pp. 68–76.bulge out or barrel.liquid lubricants are lost and thin ﬁlms may be cut during the test by sharp edges ofthe specimens. Severe barreling caused by friction may cause the sidewalls to fold upand become part of the ends as shown in Figure 4.2. Periodic unloading to replace orrelubricate the ﬁlm will help reduce these effects. Although increasing h/d reduces the effect of friction, the specimen will buckle if itis too long and slender. Buckling is likely if the height-to-diameter ratio is greater thanabout 3. If the test is so well lubricated that the ends of the specimen can slide relative tothe platens, buckling can occur for h/d ≥ 1.5 (Figure 4.3). One way to overcome the effects of friction is to test specimens with different diam-eter/height ratios. The strains at several levels of stress are plotted against d/h. By theextrapolating the stresses to d/h = 0, the stress levels can be found for an inﬁnitely longspecimen, in which the friction effects would be negligible (Figure 4.4). During compression the cross-sectional area that carries the load increases. Therefore,in contrast to the tension test, the absolute value of engineering stress is greater than the Figure 4.3. Problems with compression testing: (a) friction at the ends pre- vents spreading, which results in barreling; (b) buckling of poorly lubricated specimens can occur if the height-to-diameter ratio, h/d, exceeds about 3; (c) without any fric- tion at the ends buckling can occur if h/d is greater than about 1.5.
- 73. OTHER TESTS OF PLASTIC BEHAVIOR 55 σ1Figure 4.4. Extrapolation scheme for eliminating fric- straintional effects in compression testing. Strains at differ- σ2ent levels of stress (σ 1 , σ 2 , σ 3 ) are plotted for speci-mens of differing heights. The strain for “frictionless” σ3conditions is obtained by extrapolating d/h to 0. σ1 > σ2 > σ3 0 0.5 1.0 2.0 d/htrue stress (Figure 4.5). The area increase, together with work hardening, can lead to veryhigh forces during compression tests, unless the specimens are very small. The shape of the engineering stress–strain curve in compression can be predictedfrom the true stress–strain curve in tension, assuming that absolute values of true stressin tension and compression are the same at the same absolute strain values. Equations(3.7) and (3.8) apply, but it must be remembered that both the stress and strain are negativein compression, ecomp = exp(ε) − 1 (4.3) 400 300 engineering stress-strain stress (MPa) s and σ s vs. eFigure 4.5. Stress–strain relations incompression for a ductile material. Eachpoint σ , ε on the true stress–true strain 200curve corresponds to a point s, e on the trueengineering stress–strain curve. The ar- stress-strainrows connect these points. σ−ε 100 0 0 0.1 0.2 0.3 0.4 0.5 strain, e and ε
- 74. 56 MECHANICAL BEHAVIOR OF MATERIALSand scomp = σ/(1 + e). (4.4) Example problem 4.1: In a tensile test, the engineering stress s = 100 MPa at an engineering strain of e = 0.20. Find the corresponding values of σ and ε. At what engineering stress and strain in compression would the values of |σ | and |ε| equal those values of σ and ε? SOLUTION: In the tensile test, σ = s(1 + e) = 100(1.2) = 120 MPa, ε = ln(1 + e) = ln(1.2) = 0.182. At a true strain of −0.182 in compression, the engineering strain would be ecomp = exp(−0.182) − 1 = −0.1667 and the engineering stress would be scomp = σ /(1 + e) = −120 MPa/(1 − .1667) = −144 MPa. Failures of brittle materials occur by shear fractures on planes at 45◦ to the compressionaxis. In materials of high ductility, cracks may occur on the barreled surface, either at45◦ to the compression axis or perpendicular to the hoop direction. In the latter case,secondary tensile stresses are responsible. The frictional constraint on the ends causesthe sidewalls to bow outward. Because of this barreling, the axial compressive stressin the bowed walls is lower than in the center. Therefore a hoop-direction tension mustdevelop to aid in the circumferential expansion.Plane-strain compressionThere are two simple ways of performing plane-strain compression tests. Small samplescan be compressed in a channel that prevents spreading (Figure 4.6a). In this case, thereis friction on the sidewalls of the channel as well as on the platens, so the effect offriction is even greater than in uniaxial compression. An alternative way of producingplane-strain compression is to use a specimen that is very wide relative to the breadth ofthe indenter (Figure 4.6b). This eliminates the sidewall friction, but the deformation atz w y z t x b x ya. b.Figure 4.6. Plane-strain compression tests: (a) compression in a channel with the side walls preventingspreading; (b) plane-strain compression of a wide sheet with a narrow indenter. Lateral constraint forcing ε y =0 is provided by the adjacent material that is not under the indenter.
- 75. OTHER TESTS OF PLASTIC BEHAVIOR 57 a b cFigure 4.7. Several ways of making plane-strain tension tests on sheet specimens. All have a gauge sectionthat is very short relative to its width: (a) enlarged grips produced by welding to additional material; (b) reducedgauge section cut into edge; (c) very short gauge section achieved by friction on the cylindrical grips.and near the edges deviates from plane strain. This departure from plane strain extendsinward for a distance approximately equal to the indenter width. To minimize this effectit is recommended that the ratio of the specimen width to the indenter width, w/b, beabout 8. It is also recommended that the ratio of indenter width to sheet thickness, b/t,be about 2. Increasing b/t increases the effect of friction. Both of these tests simulatethe plastic conditions that prevail during ﬂat rolling of sheet and plate. They ﬁnd theirgreatest usefulness in exploring the plastic anisotropy of materials.Plane-strain tensionPlane-strain can be achieved in tension with specimens having gauge sections that arevery much wider than they are long. Figure 4.7 shows several possible specimens andspecimen-gripping arrangements. Such tests avoid all the frictional complications ofplane-strain compression. However, the regions near the edges lack the constraint nec-essary to impose plane strain. At the very edge, the stress-preventing contraction dis-appears, so the stress state is uniaxial tension. Corrections must be made for departurefrom plane-strain ﬂow near the edges.Biaxial tension (hydraulic bulge test)Much higher strains can be reached in bulge tests than in uniaxial tension tests. This allowsevaluation of the stress–strain relationships at high strains. A setup for bulge testing issketched in Figure 4.8. A sheet specimen is placed over a circular hole, clamped, andbulged outward by oil pressure acting on one side. Consider a force balance on a smallcircular element of radius ρ near the pole when θ is small (Figure 4.9). Using thesmall-angle approximation, the radius of this element is ρ θ , where ρ is the radius ofcurvature. The stress, σ , on this circular region acts on an area 2π ρ θt and creates a tFigure 4.8. Schematic of a hydraulic bulge test ofa sheet specimen. Hydraulic pressure causes biaxial P Pstretching of the clamped sheet. ρ
- 76. 58 MECHANICAL BEHAVIOR OF MATERIALS Figure 4.9. Force balance on a small circular region near a dome. The force acting upward is the pres- sure times the circular area. The total tangential force equals the thickness times the tangential stress. The downward force is the vertical component of this.tangential force equal to 2π σ ρ θt. The vertical component of the tangential force is2π σ ρ θt times θ, or 2π σ ρ( θ)2 t. This is balanced by the pressure, P, acting on anarea π (ρ θ ) 2 and creating an upward force of Pπ(ρ θ )2 . Equating the vertical forces, σ = Pρ/(2t). (4.5)To ﬁnd the stress, the pressure, the radius of curvature, and the radial strain must bemeasured simultaneously. The thickness, t, is then deduced from the original thickness,to , and the radial strain, ε r ; t = to exp(−2εr ). (4.6) Example problem 4.2: Assume that in a hydraulic bulge test, the bulged surface is a portion of a sphere and that at every point on the thickness of the bulged surface the thickness is the same. (Note that this is not strictly true). Express the radius of curvature, ρ, in terms of the die radius, r, and the bulged height, h. Also express the thickness strain at the dome in terms of r and h. See Figure 4.10. Figure 4.10. Geometry of a bulged surface. SOLUTION: Using the Pythagorean theorem, (ρ − h)2 + r 2 = ρ 2 , so 2ρh = h 2 + r 2 or ρ = (r + h 2 )/(2h). 2 The area of the curved surface of a spherical segment is A = 2πrh. The original area of the circle was Ao = πr 2 , so the average thickness strain is ε t ≈ ln[(2πrh)/(πr 2 )] = ln(2h/r)].
- 77. OTHER TESTS OF PLASTIC BEHAVIOR 59Figure 4.11. Equivalence of biaxial tension and through-thickness compression. Hydrostatic compression superimposed on the state of biaxial tension at the dome ofa bulge is equivalent to a state of through-thickness compression as shown schematicallyin Figure 4.11. The hydrostatic part of the stress state has no effect on plastic ﬂow.Therefore the plastic stress-strain behavior of biaxial tension (in the plane of the sheet)and through-thickness compression are equivalent.Torsion testVery high strains can be reached in torsion. The specimen shape remains constant, so thereis no necking instability or barreling. There is no friction on the gauge section. Thereforetorsion testing can be used to study plastic stress–strain relations to high strains. In atorsion test, each element of the material deforms in pure shear as shown in Figure 4.12.The shear strain, γ , in an element is given by γ = r θ/L , (4.7)where r is the radial position of the element, θ is the twist angle, and L is the specimenlength. The shear stress, τ , cannot be measured directly or even determined unequivocallyfrom the torque. This is because the shear stress, τ , depends on γ , which varies withradial position. Therefore τ depends on r. Consider an annular element of radius r andwidth dr having an area 2πrdr. The contribution of this element to the total torque, T, isthe product of the shear force on it, τ · 2π rdr, and the lever arm, r, R dT = 2π τr 2 dr and T = 2π τ yz r 2 dr . (4.8) 0 R r θ R γyz = rθ/L τ r dr z dT = rτyz2πrdr L y xFigure 4.12. Schematic of torsion test.
- 78. 60 MECHANICAL BEHAVIOR OF MATERIALSEquation (4.8) cannot be integrated directly because τ depends on r. Integration requiressubstitution of the stress–strain (τ –γ ) relation. Handbook equations for torque are usuallybased on assuming elasticity. In this case τ = Gγ = Gr θ/L. Substituting this and Equation(4.7) into Equation (4.8), R T = 2π(θ/L)G r 3 dr = (π/2)(θ/L)G R 4 . (4.9) 0Substituting GR θ/L = τ s into Equation 4.9, T = (π/2)R3 τ s . Now, solving for τ s , τs = 2T /(π R 3 ). (4.10) If the bar is not elastic, Hooke’s law cannot be assumed. The other extreme is whenthe entire bar is plastic and the material does not work-harden. In this case τ is a constant. Example problem 4.3: Consider a torsion test in which the twist is great enough so that the entire cross section is plastic. Assume that the shear yield stress, τ , is a constant. Express the torque, T, in terms of the bar radius, R, and τ . SOLUTION: The shear force on a differential annular element at a radius r is τ · 2πrdr. This causes a differential torque of dT = r(τ · 2πrdr). Integrating, R T = 2π τ r 2 dr = (2/3)π R 3 τ. (4.11) 0 If the torsion test is being used to determine the stress–strain relationship, the formof the stress–strain relationship cannot be assumed, so one does not know how the stressvaries with the radial position. One way around this problem might be to test a thin-walledtube in which the variation of stress and strain across the wall would be small enough sothat the variation of τ with r could be neglected. In this case the integral (Equation (4.8))could be approximated as T = 2π r 2 r τ, (4.12)where r is the wall thickness. However, thin-walled tubes tend to buckle and collapsewhen subjected to torsion. The buckling problem can be circumvented by making separatetorsion tests on two bars of slightly different diameter. The difference between the twocurves is the torque–twist curve for a cylinder whose wall thickness is half of the diameterdifference.
- 79. OTHER TESTS OF PLASTIC BEHAVIOR 61 The advantage of torsion tests is that very high strains can be reached, even at elevatedtemperatures. Because of this, torsion tests have been used to simulate the deformationin metal during hot rolling, so that the effects of simultaneous hot deformation andrecrystallization can be studied. It should be realized that in a torsion test, the materialrotates relative to the principal stress axes. Because of this, the strain path in the materialis constantly changing.Bend testsBend tests are used chieﬂy for materials that are very brittle and difﬁcult to machineinto tensile bars. In bending, as in torsion, the stress and strain vary with location. Theengineering strain, e, varies linearly with distance, z, from the neutral plane, e = z/ρ, (4.13)where ρ is the radius of curvature at the neutral plane as shown in Figure 4.13. Considerbending a plate of width w. The bending moment, dM, caused by the stress on a differentialelement at z is the force σ wdz times the lever arm, z: dM = σ wzdz. The total bendingmoment is twice the integral of dM from the neutral plane to the outside surface: t/2 M =2 σ wzdz. (4.14) 0To integrate, σ must be expressed in terms of z. If the entire section is elastic, and w t,σ = eE (or if w t, σ = eE/(1−v 2 )). Substituting for e, σ = (z/ρ)E. Integrating, t/2 M = 2w (E/ρ) z 2 dz, (4.15) 0 M = 2w (E/ρ)(t/2)3 /3 = w (E/ρ)t 3 /12. w t Y dz neutral planeFigure 4.13. Bending moment caused by a differ- zential element of width w and thickness dz at adistance z from the neutral plane. ρ
- 80. 62 MECHANICAL BEHAVIOR OF MATERIALSThe surface stress σs = E(t/2)/ρ. Substituting ρ = wEt 3 /(12M ) from Equation (4.15), σs = 6M/(w t2 ). (4.16)In three-point bending, M = FL/4, and in four-point bending, M = FL/2, as shownin Figure 4.14. The relation between the moment and the stress is different if plasticdeformation occurs. Example problem 4.4: Consider a four-point bend test on a ﬂat sheet of width w of a material for which the stress to cause plastic deformation is a constant, Y. Assume also that the bend is sharp enough so that the entire thickness is plastic. Derive an expression that can be used to determine Y from the force F. SOLUTION: The differential force on an element of thickness dz at a distance z from the center is Y(wdz). This force causes a differential moment dM = wYzdz. The net moment is twice the integral of dM from the center to the surface (z = t/2). Thus M = 2wY(t/2)2 /2 = wt 2 Y /4. Substituting M = FL/2 (Equation (4.16) for four-point bending), Y = 2FL/wt 2 . Measurements of fracture strengths of brittle materials are usually characterized by alarge amount of scatter because of pre existing ﬂaws, so many duplicate tests are usuallyrequired. The fracture stress is taken as the value of the surface stress, σ s , at fracture.This assumes that no plastic deformation has occurred. See Chapters 14 and 19.Hardness testsHardness tests are very simple to perform and they can be performed on production partsas quality control checks without destroying the parts. They depend on measuring theamount of deformation caused when a hard indenter is pressed into a surface with a ﬁxed F/2 F F/2 L LFigure 4.14. Three-point bending test (left) and four-point bending test (right). Note that L is deﬁned differentlyfor each test.
- 81. OTHER TESTS OF PLASTIC BEHAVIOR 63force. The disadvantage is that although the hardness of a material depends on the plasticproperties, the stress–strain relation cannot be obtained. Figure 4.15 shows the indentersused for various tests. The Rockwell tests involve measuring the depth of indentation.There are several different Rockwell scales, each of which uses a different shape and sizeof indenter and a different load. Conversion from one scale to another is approximateand empirical. Brinell hardness is determined by pressing a ball, 1 cm in diameter, into a surfaceunder a ﬁxed load (500 or 3000 kg). The diameter of the impression is measured with aneyepiece and converted to hardness. The scale is such that the Brinell hardness number,HB , is given by HB = F/As (4.17)where F is the force expressed in kg and As is the spherical surface area of the impressionin mm2 . This area can be calculated from As = π D[D − (D 2 − d 2 )1/2 ]/2, (4.18)where D is the ball diameter and d is the diameter of the impression, but it is morecommonly found from tables. Brinell data can be used to determine the Meyer hardness, HM , which is deﬁned asthe force divided by the projected area of the indentation, π d 2 /4. The Meyer hardnesshas greater fundamental signiﬁcance because it is relatively insensitive to load. Vickersand Knoop hardnesses are also deﬁned as the indentation load divided by the projectedarea. They are very nearly equal for the same material. Indentations under different loads Shape of Indentation Side Top Formula for Test Indenter View View Load Hardness Number 10-mm sphere D 2PBrinell of steel or p BHN = tungsten carbide πD(D − √D 2 − d 2) d d 136° Diamond d1 d1Vickers p VHN = 1.72 P/d12 pyramid t bKnoop Diamond p KHN = 14.2 P/l 2microhardness pyramid l/b = 7.11 l b/t = 4.00Rockwell A 60 kg RA = Diamond 20° C 150 kg RC = 100 − 500t cone D 100 kg RD = t 1 in.- B 16 100 kg RB = F diameter 60 kg RF = G steel sphere 150 kg RG = 130 − 500t 1 t 8 in.- 8 E diameter 100 kg RE = steel sphereFigure 4.15. Various hardness tests. From H. W. Hayden, William G. Moffat, and John Wulff, Structure andProperties of Materials, Vol. III, Mechanical Behavior, Wiley, 1965.
- 82. 64 MECHANICAL BEHAVIOR OF MATERIALS 1000 100 Rockwell B Knoop 800 80 Brinell Hardness (Rockwell A, B, & C) Rockwell AHardness (Knoop, Brinell) Rockwell C 60 600 400 40 200 20 Rockwell C 0 0 0 200 400 600 800 1000 Vickers Hardness No.Figure 4.16. Approximate relations between several hardness scales. For Brinell (3000 kg) and Knoop readleft. For Rockwell A, B, and C scales read right. Data from Metals Handbook, Vol. 8, ninth ed., AmericanSociety for Metals, 1985.are geometrically similar unless the indentation is so shallow that the indenter tip radiusis not negligible compared to the indentation size. For this reason, the hardness does notdepend on the load. For Brinell, Knoop, and Vickers hardness, a rule of thumb is that thehardness is about three times the yield strength when expressed in the same units. (Notethat hardness is conventionally expressed in kg/mm2 and strength in MPa. To convertkg/mm2 to MPa, multiply by 9.807. Figure 4.16 shows approximate conversions betweenseveral hardness scales. The Brinell, Meyers, Vickers, and Knoop hardness numbers are deﬁned as the force onthe indenter divided by area. (This is the projected area except in the case of the Brinellnumber.) The hardness number is related to the yield strength measured at the straincharacteristic of the indentation. For a non-work-hardening material under plane-strainindentation, theoretical analysis predicts that √ H = (2/ 3)(1 + π/2)Y = 2.97Y ≈ 3Y. (4.19) There are several approximate relations between the different scales, B ≈ 0.95V, (4.20) K ≈ 1.05V, (4.21) √ RC ≈ 100 − 1480/ B, (4.22)
- 83. OTHER TESTS OF PLASTIC BEHAVIOR 65 90 Brinell Hardness NumberBrinell Hardness Number 70 80 60 70 a. c. 50 60 0 1 2 0 1 2 Distance from Indentation Center to Edge Distance to Prior Indentation/Indentation (x/d) Diameter Brinnell Hardness Number 90 80 b. 70 0 0.5 1 1.5 Thickness/Indentation diameterFigure 4.17. Variation of hardness readings (a) with distance from the center of the edge, (b) with distancefrom the center of the prior indentation, (c) with specimen thickness. In all cases the distances are given inmultiples of the indention diameter.and RB ≈ 134 − 6700/B, (4.23)where B, V, K, RC , and RB are the Brinell, Vickers, Knoop, Rockwell C, and RockwellB hardness numbers. Another useful approximation for steels is that the tensile strength(expressed in psi) is about 500 times the Brinell hardness number (expressed in kg/mm2 )Possible errors in making hardness tests include:1. Making an indentation too close to an edge of the material. If the plastic zone around an indenter extends to an edge, the reading will be too low.2. Making an indentation too close to a prior indentation. If the plastic zone around an indenter overlaps that of a prior indentation, the strain hardening during the prior test will cause the new reading to be too high.3. Making too large an indentation on a thin specimen. If the plastic zone penetrates to the bottom surface, the reading will be in error. The effects of these on brass are illustrated in Figure 4.17. With Rockwell tests, it is important that the bottom of the specimen be ﬂat andsupported on a rigid anvil. This is necessary because the dial reading, which indicatesthe hardness by measuring the depth of penetration, is inﬂuenced by bending or settlingof the specimen, with the result of recording too low a hardness.
- 84. 66 MECHANICAL BEHAVIOR OF MATERIALS 10000 diamond corundum topazVickers hardness quartz 1000 orthoclase apatite fluorite Figure 4.18. Relation between Knoop and Mohs calcite hardness scales. 100 gypsum talc 10 0 1 2 3 4 5 6 7 8 9 10 11 Mohs hardness number Among the other hardness tests is the Shore seleroscope test, which measures therebound of a ball dropped from a ﬁxed height onto the surface to be measured. Thisworks on the principle that the energy absorbed when the ball hits the surface is ameasure of hardness. With hard materials, little energy is absorbed, so the rebounds arehigh. Mineralogists frequently classify minerals by the Moh’s scratch hardness. The systemis based on ranking minerals on a scale of 1 to 10. The scale is such that a mineral higheron the scale will scratch a mineral lower on the scale. The scale is arbitrary and notwell suited to metals, because most metals tend to fall in the range between 4 and 8.Actual values vary somewhat with how the test is made (e.g., the angle of inclination ofthe scratching edge.) Figure 4.18 gives the approximate relationship between Moh’s andVickers hardnesses.Mutual indentation hardnessHardness tests are normally made with indenters that do not deform. However, it ispossible to measure hardness when the indenters do deform. This is useful at very hightemperatures where it is impossible to ﬁnd a suitable material for the indenter. Deﬁningthe hardness as the indentation force/area of indentation, the hardness, H, of a materialis proportional to its yield strength, H = cY, (4.24)where c depends mainly on the geometry of the test. For example, in a Brinell testwhere the indenting ball is very much harder than the test material, c ≈ 2.8. For mutualindentation of cross wedges, c ≈ 3.4 (Figure 4.19), and for crossed cylinders, c ≈ 2.4. Theconstant c has been determined for other geometries and for cases where the indentershave different hardnesses. The forces in automobile accidents have been estimated byexamining the depths of mutual indentations.
- 85. OTHER TESTS OF PLASTIC BEHAVIOR 67Figure 4.19. Mutual indentation of two wedges. Thehardness is the force/area.NOTEAn apparatus suggested by Galileo for bending tests is illustrated in Figure 4.20. Figure 4.20. Galileo’s sketch of a bending test. D A B C EREFERENCESMetals Handbook, ninth ed., Vol. 8, Mechanical Testing, ASM, 1985.D. K. Felbeck and A. G. Atkins, Strength and Fracture of Engineering Solids, Prentice– Hall, 1984.PROBLEMS 1. The engineering stress–strain curve from a tension test on a low carbon steel is plotted in Figure 4.21. From this, construct the engineering stress–strain curve in compression, neglecting friction. 2. Discuss how friction and inhomogeneous deformation affect the results from A. The two types of plane-strain compression tests illustrated in Figure 4.6. B. The plane-strain tension tests illustrated in Figure 4.7.
- 86. 68 MECHANICAL BEHAVIOR OF MATERIALS 500 400 Engineering Stress, MPa 300 200 100 0 0 0.1 0.2 0.3 0.4 0.5 0.6 Engineering Strain Figure 4.21. Engineering stress–strain curve for a low carbon steel. 3. Sketch the 3-dimensional Mohr’s stress and strain diagrams for a plane-strain compression test. 4. Draw a Mohr’s circle diagram for the surface stresses in a torsion test, showing all three principal stresses. At what angle to the axis of the bar are the tensile stresses the greatest? 5. For a torsion test, derive equations relating the angle, ψ, between the axis of the largest principal stress and the axial direction and the angle, ψ , between the axis of the largest principal strain and the axial direction in terms of L, r, and the twist angle, θ. Note that for ﬁnite strains, these two angles are not the same. 6. Derive an expression relating the torque, T, in a tension test to the shear stress at the surface, τ s , in terms of the bar diameter, D, assuming that the bar is A. Entirely elastic, so that τ varies linearly with the shear strain, γ . B. Entirely plastic and does not work-harden, so that the shear stress, τ , is constant. 7. The principal strains in a circular bulge test are the thickness strain, ε t , the cir- cumferential (hoop) strain, εc , and the radial strain, ε r . Describe how the ratio εc /εr varies over the surface of the bulge. Assume that the sheet is locked at the opening. 8. Derive an expression for the fracture stress, Sf , in bending as a function of Ff , L, w, and t for three-point bending of a specimen having a rectangular cross section, where Ff is the force at fracture, L is the distance between supports, w is the specimen width, and t is the specimen thickness. Assuming the deformation is elastic, the deﬂection y in bending is given by y = αFL3 /(EI), where α is a constant and E is Young’s modulus. How would you expect the value of α to depend the ratio of t/w?
- 87. OTHER TESTS OF PLASTIC BEHAVIOR 69 9. Equation 4.16 gives the stresses at the surface of bend specimens. The derivation of this equation is based on the assumption of elastic behavior. If there is plastic deformation during the bend test, will the stress predicted by this equation be (a) too low, (b) too high, (c) either too high or too low depending on where the plastic deformation occurs, or (d) correct?10. By convention, Brinell, Meyer, Vickers, and Knoop hardness numbers are stresses expressed in units of kg/mm2 , which is not an SI unit. To what stress, in MPa, does a Vickers hardness of 100 correspond?11. In making Rockwell hardness tests, it is important that bottom of the specimen be ﬂat so that the load doesn’t cause any bending of the specimen. On the other hand, this is not important in making Vickers or Brinell hardness tests. Explain.
- 88. 5 Strain-Hardening of MetalsIntroductionWith elastic deformation, the strains are proportional to the stress, so every level ofstress causes some elastic deformation. On the other hand, a deﬁnite level of stress mustbe applied before any plastic deformation occurs. As the stress is further increased, theamount of deformation increases, but not linearly. After plastic deformation starts, thetotal strain is the sum of the elastic strain (which still obeys Hooke’s law) and the plasticstrain. Because the elastic part of the strain is usually much less than the plastic part, itwill be neglected in this chapter and the symbol ε will signify the true plastic strain. The terms strain-hardening and work-hardening are used interchangeably to describethe increase of the stress level necessary to continue plastic deformation. The term ﬂowstress is used to describe the stress necessary to continue deformation at any stageof plastic strain. Mathematical descriptions of true stress–strain curves are needed inengineering analyses that involve plastic deformation, such as prediction of energy ab-sorption in automobile crashes, design of dies for consist stamping parts, and analysis ofthe stresses around cracks. Various approximations are possible. Which approximationis best depends on the material, the nature of the problem, and the need for accuracy.This chapter will consider several approximations and their applications.Mathematical approximationsThe simplest model is one with no work-hardening. The ﬂow stress, σ , is independentof strain, so σ = Y, (5.1)where Y is the tensile yield strength (see Figure 5.1a). For linear work-hardening (Fig-ure 5.1b), σ = Y + Aε. (5.2) It is more common for materials to work-harden with a hardening rate that decreaseswith strain. For many metals a log–log plot of true stress versus true strain is nearly linear.70
- 89. STRAIN-HARDENING OF METALS 71σ σ σ σ σ Y Y σ0 ε ε ε ε ε ε0 σ=Y σ =Y + Aε σ = Kεn σ = K(ε + ε0)n σ = σ0[1 − exp(−Aε)] a b c d eFigure 5.1. Mathematical approximations of the true stress–strain curve.In this case, a power law, σ = K εn , (5.3)is a reasonable approximation (Figure 5.1c). A better ﬁt is often obtained with σ = K (ε + εo )n . (5.4)(See Figure 5.1d.) This expression is useful where the material has undergone a prestrainof εo . Still another model is a saturation model suggested by Voce (Figure 5.1e), σ = σ o [1 − exp(−Aε)]. (5.5)Equation (5.5) predicts that the ﬂow stress approaches an asymptote, σ o , at high strains.This model seems to be reasonable for a number of aluminum alloys. Example problem 5.1: Two points on a true stress–strain curve are σ = 222 MPa at ε = 0.05 and σ = 303 MPa at ε = 0.15. 1. Find the values of K and n in Equation (5.3) that best ﬁt the data. Then using these values of K and n, predict the true stress at a strain of ε = 0.30. 2. Find the values of σ o and A in Equation (5.5) that best ﬁt the data. Then using these values of K and n, predict the true stress at a strain of ε = 0.30. SOLUTION 1. Apply the power law at two levels of stress, σ 2 and σ 1 . Then take the ratios σ 2 /σ 1 = (ε 2 /ε 1 )n , and ﬁnally take the natural logs of both sides, n = ln (σ 2 /σ 1 )/ln(ε 2 /ε1 ) = ln(303/222)/ln(0.15/0.05) = 0.283. K = σ /ε n = 303/ 0.150.283 = 518.5 MPa. At ε = 0.30, σ = 518.4(0.30)0.283 = 368.8 MPa. 2. Apply the saturation model at two levels of stress, σ 2 and σ 1 , σ 1 = σ o [1 − exp (−Aε1 )] and σ 2 = σ o [1 − exp(Aε2 )]. Then take the ratios σ 2 /σ 1 = [1 − exp (−Aε2 )]/[1 − exp(−Aε 1 )]. Substituting σ 2 /σ 1 = 303/222 = 1.365, ε 1 = 0.05, and ε 2 = 0.15 and solving by trial and error, A = 25.2. σ 0 = 303[1 − exp(−25.2 × 0.15)] = 296 MPa. At ε = 0.30, σ = 310[1 − exp(−25.2 × 0.30)] = 309.8 MPa.
- 90. 72 MECHANICAL BEHAVIOR OF MATERIALSTable 5.1. Typical values of n and K Strength Strain-hardeningMaterial coefﬁcient, K (MPa) exponent, nlow-carbon steels 525 to 575 0.20 to 0.23HSLA steels 650 to 900 0.15 to 0.18austenitic stainless 400 to 500 0.40 to 0.55copper 420 to 480 0.35 to 0.5070/30 brass 525 to 750 0.45 to 0.60aluminum alloys 400 to 550 0.20 to 0.30Note: From various sources including W. F. Hosford and R. M. Caddell, Metal Forming:Mechanics and Metallurgy, Prentice–Hall, 1983.Power-law approximationThe most commonly used expression is the simple power law (Equation (5.3)). Typicalvalues of the exponent n are in the range from 0.1 to 0.6. Table 5.1 lists K and n forvarious materials. As a rule, high-strength materials have lower n-values than low-strengthmaterials. Figure 5.2 shows that the exponent, n, is a measure of the persistence ofFigure 5.2. True stress–strain curves for σ = K εn with several values of n. To make the effect of n on theshape of the curves apparent, the value of K for each curve has been adjusted so that it passes throughσ = 1 at ε = 0.3.
- 91. STRAIN-HARDENING OF METALS 73hardening. If n is low, the work-hardening rate is initially high, but the rate decreasesrapidly with strain. On the other hand, with a high n, the initial work hardening is lessrapid but continues to high strains. If σ = K εn , ln σ = ln K + n ln ε, so the true stress–strain relation plots as a straight line on log–log coordinates as shown in Figure 5.3. Theexponent, n, is the slope of the line. The preexponential, K, can be found by extrapolatingto ε = 1.0. K is the value of σ at this point. The level of n is particularly signiﬁcant instretch forming because it indicates the ability of a metal to distribute the strain over awide region. Often a log–log plot of the true stress–strain curve deviates from linearityat low or high strains. In such cases it is still convenient to use Equation (5.3) over thestrain range of concern. The value of n is then taken as the slope of the linear portion ofthe curve: n = d(ln σ )/d(ln ε) = (ε/σ )dσ /dε. (5.6)Necking. As a tensile specimen is extended, the level of true stress, σ , rises but thecross-sectional area carrying the load decreases. The maximum load-carrying capacityis reached when dF = 0. The force equals the true stress times the actual area, F = σ A.Differentiating gives A dσ + σ dA = 0. (5.7)Since the volume, AL, is constant, dA/A = −dL/L = −dε. Rearranging terms, dσ =−σ dA/A = σ dε, or dσ /dε = σ . (5.8)Equation (5.8) simply states that the maximum load is reached when the rate of workhardening is numerically equal to the stress level. As long as dσ /dε > σ , deformation will occur uniformly along the test bar. However,once the maximum load is reached (dσ /dε = σ ), the deformation will localize. Anyregion that deforms even slightly more than the others will have a lower load-carrying 1000 KTrue Stress 100 0.01 0.1 1 True StrainFigure 5.3. A plot of the true stress–strain curve on logarithmic scales. Because σ = K ε n , ln σ = ln K + n ln ε.The straight line indicates that σ = K ε n holds. The slope is equal to n and K equals the intercept at ε = 1.
- 92. 74 MECHANICAL BEHAVIOR OF MATERIALSFigure 5.4. The condition for necking in a tensiontest is met when the true stress, σ , equals the slope,dσ /dε, of the true stress–strain curve.capacity and the load will drop to that level. Other regions will cease to deform, sodeformation will localize into a neck. Figure 5.4 is a graphical illustration. If a mathematical expression is assumed for the stress–strain relationship, the limit ofuniform elongation can be found analytically. For example, with power-law hardening,Equation (5.3), σ = K ε n , and dσ /dε = n K εn−1 . Substituting into Equation (5.8) givesK εn = n K εn−1 , which simpliﬁes to ε = n, (5.9)so the strain at the start of necking equals n. Uniform elongation in a tension test oc-curs before necking. Therefore so materials with a high n value have large uniformelongations. Since the ultimate tensile strength is simply the engineering stress at maximum load,the power-law hardening rule can be used to predict it. First ﬁnd the true stress at maximumload by substituting the strain, n, into Equation (5.3): σ max load = K n n . (5.10)Then substitute s = σ /(1 + e) = σ exp(−ε) = σ exp(−n) into Equation (5.10); the ten-sile strength is expressed as smax = K n n exp(−n) = K (n/e)n , (5.11)where e is the base of natural logarithms. Similarly the uniform elongation and tensile strength may be found for other approx-imations to the true stress–strain curve.
- 93. STRAIN-HARDENING OF METALS 75 Example problem 5.2: A material has a true stress–strain curve that can be approxi- mated by σ = Y + Aε. Express the uniform elongation, e, in terms of the constants, A and Y . SOLUTION: The maximum load is reached when dσ /dε = σ . Equating dσ /dε = A, and σ = Y + Aε, the maximum load is reached when A = Y + Aε or ε = 1 − Y /A. The engineering strain e = exp(ε) − 1 = exp(1 − Y /A) − 1.Work per volume. The area under the true stress–strain curve is the work per volume, w,expended in the deformation of a material. That is, w = σ dε. With power-law hardening w = K ε n + 1 /(n + 1). (5.12)This is sometimes called the tensile toughness.Localization of strain at defects. If the stresses that cause deformation in a body arenot uniform, the deformation will be greatest where the stress is highest, and least wherethe stress is lowest. The differences between the strains in the different regions dependon the value of n. If n is high, the difference will be less than if n is low. For example,consider a tensile bar in which the cross-sectional area of one region is a little less thanthat in the rest of the bar (Figure 5.5). Let these areas be Aao and Abo . The tensile force, F, is the same in both regions, Fa = Fb , so σ a Aa = σ b Ab . (5.13)Because ε = ln(L/L o ) and (L/L o ) = (Ao /A), the instantaneous area, A, may be expre-ssed as A = Ao exp(−ε), so Aa = Aao exp(−ε a ), and Ab = Abo exp(−ε b ). Assumingpower-law hardening (Equation (5.3)), σ a = K ε a n , and σ b = K ε b n . Substituting intoEquation (5.13), K ε a Aao exp(−ε a ) = K ε b Abo exp(−ε b ). n n (5.14)Now simplify by substituting f = Abo /Aao : εa exp(−ε a ) = fε b exp(−ε b ). n n (5.15) Equation (5.15) can be numerically evaluated to ﬁnd εa as a function of εb . Fig-ure 5.6 shows that with low values of n, the region with the larger cross section deformsvery little. On the other hand, if n is high, there is appreciable deformation in the thickerregion, so more overall stretching will have occurred when the thinner region fails. Thisleads to greater formability. Figure 5.5. Stepped tensile specimen. The initial a b c cross-sectional area of region b is f times the cross-sectional area A.
- 94. 76 MECHANICAL BEHAVIOR OF MATERIALSFigure 5.6. The relative strains in two regions of a tensile bar having different initial cross-sectional areas. Example problem 5.3: To ensure that the neck in a tensile bar would occur at the middle of the gauge section, the machinist made the bar with a 0.500-in. diameter in the middle of the gauge section and machined the rest of it to a diameter of 0.505 in. After testing it was found that the diameter away from the neck was 0.470 in. Assume that the stress–strain relation follows the power law, Equation (5.3). What was the value of n? SOLUTION: Let the regions with the larger and smaller diameters be designated a and b. When the maximum load is reached, the strain in b is εb = n and the strain in region a is εa = ln(Ao /A) = ln(do /d)2 = 2 ln(0.505/0.470) = 0.1437. f = (0.500/0.505)2 = 0.9803. Substituting ε b = n, ε a = 0.1437, and f = 0.98 into Equa- tion (5.15), 0.1437n exp(−0.1437) = 0.9803n n exp(−n). Solving by trial and error, n = 0.238. Note that there would have been a large error if the effect of the different initial cross sections had been ignored and n had been taken as 2 ln(0.505/0.470) = 0.1437.NOTESProfessor Zdzislaw Marciniak of the Technical University of Warsaw was the ﬁrst to analyze theeffect of a small defect or inhomogeneity on the localization of plastic ﬂow * . His analysis of necking* Z. Marciniak and K. Kuczynski, Int. J. Mech. Sci., Vol. 9 (1967): p. 609.
- 95. STRAIN-HARDENING OF METALS 77forms the basis for understanding superplastic elongations (Chapter 7) and for calculating theforming limit diagrams (Chapter 22). He has been Acting Rector, Senior Professor, and Director ofthe Institute of Metal Forming at the Technical University of Warsaw and has published a numberof books in Polish on metal forming and many papers in the international literature. One can experience work hardening by holding the ends of a wire in one’s ﬁngers and bendingit, straightening it, and bending it again. The second time the bend will occur in a different spotthan the ﬁrst bend. Why?PROBLEMS 1. What are the values of K and n in Figure 5.3? 2. The following true stress–true strain data were obtained from a tension test. Strain Stress (MPa) Strain Stress (MPa) 0.00 0.00 0.10 250.7 0.01 188.8 0.15 270.6 0.02 199.9 0.20 286.5 0.05 223.5 A. Plot true stress versus true strain on a logarithmic plot B. What does your plot suggest about n in Equation (5.3)? C. What does your plot suggest about a better approximation? 3. The true stress–strain curve of a material obeys the power-hardening law with n = 0.18. A piece of this material was given a tensile strain of ε = 0.03 before being sent to a laboratory for tension testing. The laboratory workers were unaware of the prestrain and tried to ﬁt their data to Equation (5.3). A. What value of n would they report if they determined n from the elongation at maximum load? B. What value of n would they report if they determined n from the loads at ε = 0.05 and 0.15? 4. In a tension test, the following values of engineering stress and strain were found: s = 133.3 MPa at e = 0.05, s = 155.2 MPa at e = 0.10, and s = 166.3 MPa at e = 0.15. A. Determine whether the data ﬁt Equation (5.3). B. Predict the strain at necking. 5. Two points on a stress–strain curve for a material are σ = 278 MPa at ε = 0.08 and σ = 322 MPa at ε = 0.16. A. Find K and n in the power-law approximation and predict σ at ε = 0.20. B. For the approximation σ = K (ε o + ε)n (Equation (5.4)) with ε o = 0.01, ﬁnd K and n and predict σ at ε = 0.20.
- 96. 78 MECHANICAL BEHAVIOR OF MATERIALS 6. The tensile stress–strain curve of a certain material is best represented by a satu- ration model, σ = σ o [1 − exp(−Aε)]. A. Derive an expression for the true strain at maximum load in terms of the constants A and σ o . B. In a tension test, the maximum load occurred at an engineering strain of e = 21% and the tensile strength was 350 MPa. Determine the values of the constants A and σ o for the material. [Remember that the tensile strength is the maximum engineering stress.] 7. A material has a stress–strain relation that can be approximated by σ = 150 + 185ε. For such a material A. What percent uniform elongation should be expected in a tension test? B. What is the material’s tensile strength? 8. A. Derive expressions for the true strain at the onset of necking if the stress–strain curve is given by σ = K (ε o + ε)n (Equation (5.4)). B. Write an expression for the tensile strength. 9. Consider a tensile specimen made from a material that obeys the power hardening law with K = 400 MPa and n = 0.20. Assume K is not sensitive to strain rate. One part of the gauge section has an initial cross-sectional area that is 0.99 times that of the rest of the gauge section. What will be the true strain in the larger area after the smaller area necks and reduces to 50% of its original area?10. Consider a tensile bar that was machined so that most of the gauge section was 1.00 cm in diameter. One short region in the gauge section has a diameter 1/2% less (0.995 cm). Assume the stress–strain curve of the material is described by the power law with K = 330 MPa and n = 0.23 and the ﬂow stress is not sensitive to strain rate. The bar was pulled in tension well beyond maximum load and it necked in the reduced section. A. Calculate the diameter away from the reduced section. B. Suppose that an investigator had not known that the bar initially had a reduced section and had assumed that the bar had a uniform initial diameter of 1.00 cm. Suppose that she measured the diameter away from the neck and had used that to calculate n. What value of n would she have calculated?11. A tensile bar was machined so that most of the gauge section had a diameter of 0.500 cm. One small part of the gauge section had a diameter 1% smaller (0.495 cm). Assume power-law hardening with n = 0.17. The bar was pulled until necking occurred. A. Calculate the uniform elongation (%) away from the neck. B. Compare this with the uniform elongation that would have been found if there had been no initial reduced section.
- 97. STRAIN-HARDENING OF METALS 7912. Repeated cycles of freezing of water and thawing of ice will cause copper pipes to burst. Water expands about 8.3% when it freezes. A. Consider a copper tube as a capped cylinder that cannot lengthen or shorten. If it were ﬁlled with water, what would be the circumferential strain in the wall when the water froze? B. How many cycles of freezing/thawing would it take to cause the tube walls to neck? Assume the tube is ﬁlled after each thawing. Assume n = 0.55.
- 98. 6 Plasticity TheoryIntroductionPlasticity theory deals with yielding of materials under complex stress states. It allowsone to decide whether or not a material will yield under a stress state and to determine theshape change that will occur if it does yield. It also allows tensile test data to be used topredict the work-hardening during deformation under such complex stress states. Theserelations are a vital part of computer codes for predicting crashworthiness of automobilesand codes for designing forming dies.Yield criteriaThe concern here is to describe mathematically the conditions for yielding under complexstresses. A yield criterion is a mathematical expression of the stress states that will causeyielding or plastic ﬂow. The most general form of a yield criterion is f (σx , σ y , σz , τ yz , τzx , τx y ) = C, (6.1)where C is a material constant. For an isotropic material this can be expressed in termsof principal stresses, f (σ1 , σ2 , σ3 ) = C. (6.2) The yielding of most solids is independent of the sign of the stress state. Reversing thesigns of all the stresses has no effect on whether a material yields. This is consistent withthe observation that for most materials, the yield strengths in tension and compressionare equal. * Also, with most solid materials, it is reasonable to assume that yielding isindependent of the level of mean normal stress, σm = (σ1 + σ2 + σ3 )/3. (6.3)* This may not be true when the loading path is changed during deformation. Directional differences in yielding behavior after prior straining are called a Bauschinger effect. This subject is treated in Chapter 18. It is also not true if mechanical twinning is an important deformation mechanism. (See Chapter 11.) The compressive yield strengths of polymers are generally higher than the tensile yield strengths. (See Chapter 20.)80
- 99. PLASTICITY THEORY 81It will be shown later that this is equivalent to assuming that plastic deformation causesno volume change. This assumption of constancy of volume is certainly reasonablefor crystalline materials that deform by slip and twinning because these mechanismsinvolve only shear. With slip and twinning only the shear stresses are important. Withthis simpliﬁcation, the yield criteria must be of the form f [(σ2 − σ3 ), (σ3 − σ1 ), (σ1 − σ2 )] = C. (6.4)In terms of the Mohr’s stress circle diagrams, only the sizes of the circles (not their posi-tions) are of importance in determining whether yielding will occur. In three-dimensionalstress space (σ 1 vs. σ 2 vs. σ 3 ) the locus can be represented by a cylinder parallel to theline σ 1 = σ 2 = σ 3 , as shown in Figure 6.1.Tresca maximum shear stress criterion. The simplest yield criterion is one ﬁrst pro-posed by Tresca. It states that yielding will occur when the largest shear stress reaches acritical value. The largest shear stress is τ max = (σ max − σ min )/2, so the Tresca criterioncan be expressed as σmax − σmin = C. (6.5)If the convention is maintained that σ 1 ≥ σ 2 ≥ σ 3 , this can be written as σ1 − σ3 = C. (6.6)The constant C can be found by considering uniaxial tension. In a tension test, σ 2 = σ 3 =0 and at yielding σ 1 = Y, where Y is the yield strength. Substituting into Equation (6.6),C = Y. Therefore the Tresca criterion may be expressed as σ1 − σ3 = Y. (6.7)For pure shear, σ 1 = −σ 3 = k, where k is the shear yield strength. Substituting in Equation(6.7), k = Y/2, so σ1 − σ3 = 2k = C. (6.8) σ3 σ1 = σ2 = σ3Figure 6.1. A yield locus is the surface of a body inthree-dimensional stress space. Stress states on thelocus will cause yielding. Those inside the locus willnot cause yielding. σ2 σ1
- 100. 82 MECHANICAL BEHAVIOR OF MATERIALS Example problem 6.1: Consider an isotropic material, loaded so that the principal stresses coincide with the x, y, and z axes of the material. Assume that the Tresca yield criterion applies. Make a plot of the combinations of σ y versus σ x that will cause yielding with σ z = 0. SOLUTION: Divide the σ y versus σ x stress space into six sectors as shown in Figure 6.2. The following conditions are appropriate: 1. σ x > σ y > σ z = 0, so σ 1 = σ x , σ 3 = σ z = 0, so σ x = Y 2. σ y > σ x > σ z = 0, so σ 1 = σ y , σ 3 = σ z = 0, so σ y = Y 3. σ y > σ z = 0 > σ x , so σ 1 = σ y , σ 3 = σ x , so σ y − σ x = Y 4. σ z = 0 > σ y > σ x , so σ 1 = 0, σ 3 = σ x , so − σ x = Y 5. σ z = 0 > σ x > σ y , so σ 1 = 0, σ 3 = σ y , so − σ y = Y 6. σ x > σ z = 0 > σ y , so σ 1 = σ x , σ 3 = σ y , so σ x − σ y = Y These are plotted in Figure 6.2. Figure 6.2. Plot of the yield locus for the Tresca criterion for σz = 0. The Tresca criterion predicts that the intermediate principal stress has no ef- fect on yielding. For example, in sector I, the value of σy has no effect on the value of σx re- quired for yielding. Only if σy is negative or if it is higher than σx does it have an inﬂuence. In these cases, it is no longer the intermediate principal stress. It seems reasonable to incorporate the effect of the intermediate principal stress intothe yield criterion. One might try this by assuming that yielding depends on the averageof the diameters of the three Mohr’s circles, [(σ 1 − σ 2 ) + (σ 2 − σ 3 ) + (σ 1 − σ 3 )]/3,but the intermediate stress term, σ 2 , drops out of the average: [(σ 1 − σ 2 ) + (σ 2 − σ 3 )+ (σ 1 − σ 3 )]/3 = (2/3)(σ 1 − σ 3 ). Therefore an average diameter criterion reduces tothe Tresca criterion.Von Mises criterion. The effect of the intermediate principal stress can be included byassuming that yielding depends on the root-mean-square diameter of the three Mohr’s ∗circles . This is the von Mises criterion, which can be expressed as 1/2 (σ2 − σ3 )2 + (σ3 − σ1 )2 + (σ1 − σ2 )2 3 = C. (6.9)∗ This is equivalent to assuming that yielding occurs when the elastic distortional strain energy reaches a critical value.
- 101. PLASTICITY THEORY 83Note that each term is squared, so the convention σ 1 ≥ σ 2 ≥ σ 3 is not necessary. Again thematerial constant, C, can be evaluated by considering a uniaxial tension test. At yielding,σ 1 = Y and σ 2 = σ 3 = 0. Substituting, [02 + (−Y)2 + Y2 ]/3 = C2 , or C = (2/3)1/3 Y, sothe equation is usually written as (σ 2 − σ 3 )2 + (σ 3 − σ 1 )2 + (σ 1 − σ 2 )2 = 2Y 2 . (6.10) For a state of pure shear, σ 1 = −σ 3 = k and σ 2 = 0. Substituting in Equation 6.10,(−k)2 + [(−k) − k]2 + k2 = 2Y2 , so √ k = Y / 3. (6.11)Equation (6.10) can be simpliﬁed if one of the principal stresses is zero (plane-stressconditions). Substituting σ 3 = 0, σ 1 2 + σ 2 2 − σ 1 σ 2 = Y2 , which is an ellipse. Withfurther substitution of α = σ 2 /σ 1 , σ 1 = Y /(1 − α + α 2 )1/2 . (6.12) Example problem 6.2: Consider an isotropic material loaded so that the principal stresses coincide with the x, y, and z axes. Assuming the von Mises yield criterion applies, make a plot of σ y versus σ x yield locus with σ z = 0. SOLUTION: Let σ x = σ 1 , σ y = σ 2 , and σ z = 0. Now α = σ 2 /σ 1 . Figure 6.3 results from substituting several values of α into Equation (6.12), solving for σ x /Y and σ y /Y = ασ x /Y, and then plotting. Figure 6.3. The Mises criterion with σ z = 0 plots as an ellipse. Example problem 6.3: For plane stress (σ 3 = 0), what is the largest possible ratio of σ 1 /Y at yielding and at what stress ratio, α, does this occur?
- 102. 84 MECHANICAL BEHAVIOR OF MATERIALS SOLUTION: Inspecting Equation (6.12), it is clear that the maximum ratio of σ 1 /Y corresponds to the minimum value 1 − α + α 2 . Differentiating and setting to zero, d(1 − α + α 2 )/dα = −1 + 2α; α = −1/2. Substituting into equation 6.12, σ 1 /Y = √ [1 − 1/2 + (1/2)2 ]−1/2 = (4/3) = 1.155. The von Mises yield criterion can also be expressed in terms of stresses that are notprincipal stresses. In this case it is necessary to include shear terms, (σ y − σ z )2 + (σ z − σ x )2 + (σ x − σ y )2 + 6 τ yz 2 + τ zx 2 + τ x y 2 = 2Y 2 , (6.13)where x, y, and z are not principal stress axes.Flow rules. When a material yields, the ratio of the resulting strains depends on thestress state that causes yielding. The general relations between plastic strains and thestress states are called the ﬂow rules. They may be expressed as dεi j = dλ(∂ f /∂σ i j ), (6.14)where f is the yield function corresponding to the yield criterion of concern and dλ is a ∗constant that depends on the shape of the stress–strain curve . For the von Mises criterion,we can write f = [(σ 2 − σ 3 )2 + (σ 3 − σ 1 )2 + (σ 1 − σ 2 )2 ]/4. In this case Equation (6.14)results in dε1 = dλ[2(σ 1 − σ 2 ) − 2(σ 3 − σ 1 )]/4 = dλ · [σ 1 − (σ 2 + σ 3 )/2] dε2 = dλ[σ 2 − (σ 3 + σ 1 )/2] dε3 = dλ[σ 3 − (σ 1 + σ 2 )/2].† (6.15)These are known as the Levy–Mises equations. Even though dλ is not usually known,these equations are useful for ﬁnding the ratio of strains that result from a known stressstate or the ratio of stresses that correspond to a known strain state. Example problem 6.4: Find the ratio of the principal strains that result from yielding if the principal stresses are σ y = σ x /4, σ z = 0. Assume the von Mises criterion. SOLUTION: According to Equation (6.15), dε 1 : dε2 : dε3 = [σ 1 − (σ 2 + σ 3 )/2] : [σ 2 − (σ 3 + σ 1 )/2] : [σ 3 − (σ 1 + σ 2 )/2] = (7/8)σ 1 : (−1/4)σ 1 : (−5/8)σ 1 = 7 : −2 : −5.∗ The constant, dλ, can be expressed as dλ = dε/dσ , which is the inverse slope of the effective stress–strain curve at the point where the strains are being evaluated.† Equations (6.15) parallel the Hooke’s law equations (Equation (2.2)), where dλ = dε/dσ replaces 1/ E and 1/2 replaces Poisson’s ratio, v. For this reason it is sometimes said that the “plastic Poisson’s ratio” is 1/2.
- 103. PLASTICITY THEORY 85 The ﬂow rules for the Tresca criterion can be found by applying Equation (6.14) withf = σ 1 − σ 3 . Then dε1 = dλ, dε2 = 0, and dε 3 = −dλ, or dε1 : dε2 : dε3 = 1 : 0 : −1. (6.16) Example problem 6.5: Find the ratio of the principal strains that result from yielding if the principal stresses are σ y = σ x /4, σ z = 0, assuming the Tresca criterion. SOLUTION: Here dε1 = dεx , dε2 = dε y , and dε3 = dεz , so dεx : dε y : dε z = 1 : 0 : −1. Example problem 6.6: Circles were printed on the surface of a part before it was deformed. Examination after deformation revealed that the principal strains in the sheet are ε 1 = 0.18 and ε2 = 0.078. Assume that the tools did not touch the surface of concern and that the ratio of stresses remained constant during the deformation. Using the von Mises criterion, ﬁnd the ratio of the principal stresses. SOLUTION: First, realize that with a constant ratio of stresses, dε 2 : dε 1 = ε 2 : ε1 . Also, if the tools did not touch the surface, it can be assumed that σ 3 = 0. Then according to Equation (6.15), ε2 /ε 1 = dε2 /dε1 = (σ 2 − σ 1 /2)/(σ 1 − σ 2 /2). Substituting, α = σ 2 /σ 1 , and ρ = ε 2 /ε 1 , (α −1/2)/(1 − α/2) = ρ. Solving for α, α = (ρ + 1/2)/(ρ/2 + 1). (6.16) Now substituting ρ = 0.078/0.18 = 0.4333, α = 0.7671. Example problem 6.7: Draw the three-dimensional Mohr’s circle diagrams for the stresses and plastic strains in a body loaded under plane-strain tension, ε y = 0, with σ z = 0. Assume the von Mises yield criterion. SOLUTION: From the ﬂow rules, εy = 0 = λ[σ y − (1/2)(σ x + σ z )] with εy = 0 and σ z = 0, σ y = 1/2(σ x ). The Mohr’s stress circles are determined by the principal stresses, σ x , σ y = 1/2(σ x ), and σ z = 0. For plastic ﬂow, εx + εy + εz = 0, so with ε y = 0, εz = −ε x . The Mohr’s strain circles (Figure 6.4) are determined by the principal strains, ε x , εy = 0, and εz = −ε x . γ/2 τ Figure 6.4. Mohr’s strain and stress circles for plane strain. εz εy εx ε σz σy σx σPrinciple of normality . The ﬂow rules may be represented by the principle of normality.According to this principle, if a normal to the yield locus is constructed at the point ofyielding, the strains that result from yielding are in the same ratio as the stress componentsof the normal. This is illustrated in Figure 6.5. A corollary is that for a σ 1 versus σ 2 yield
- 104. 86 MECHANICAL BEHAVIOR OF MATERIALS σy σz = 0 dε dεy dεx σxFigure 6.5. The ratios of the strains resulting from Figure 6.6. The ratio of strains resulting from yieldingyielding are in the same proportion as the compo- along several loading paths. At A, ε y = ε x ; at B, ε ynents of a vector normal to the yield surface at the = 0; at C (uniaxial tension) ε y = −1/2ε x ; and at D,point of yielding. ε y = −ε x .locus with σ 3 = 0, dε1 /dε2 = −∂σ 2 /∂σ 1 , (6.17)where ∂σ 2 /∂σ 1 is the slope of the yield locus at the point of yielding. It should be notedthat Equations (6.14) and (6.17) are general and can be used with other yield criteria,including ones formulated to account for anisotropy and for pressure-dependent yielding. Figure 6.6 shows how different shape changes result from different loading paths.The components of the normal at A are dσ y /dσ x = 1, so εy = εx . At B the normal has aslope of dσ y = 0, so εy = 0. For uniaxial tension at C, the slope of the normal is dσ y /dσ x = −1/2, which corresponds to ε y = (−1/2)ε x . At D, dσ y /dσ x = −1, so ε y = −ε x . Figure 6.7 is a representation of the normality principle applied to the Tresca criterion.All stress states along a straight edge cause the same ratio of plastic strains. The shapechanges corresponding to the corners are ambiguous because it is ambiguous which stresscomponent is σ max and which stress component is σ min . For example, with yielding underbiaxial tension, σ x = σ y , 0 ≤ ε y /ε x ≤ ∞.Effective stress and effective strain. The concepts of effective stress and effectivestrain are necessary for analyzing the strain hardening that occurs on loading paths otherthan uniaxial tension. Effective stress, σ , and effective strain, ε, are deﬁned so that1. σ and ε reduce to σ x and εx in an x-direction tension test.2. The incremental work per volume done in deforming a material plastically is dw = σ dε.3. Furthermore it is usually assumed that the σ versus ε curve describes the strain ∗ hardening for loading under a constant stress ratio, α, regardless of α. The effective stress, σ , is a function of the applied stresses that determine whetheryielding occurs. When σ reaches the current ﬂow stress, plastic deformation will occur.∗ At large strains, the σ versus ε curves do depend on the loading path because of orientation changes within the material. These orientation changes (texture development) depend on the loading path. However, the dependence of strain hardening on the loading path is signiﬁcant only at large strains.
- 105. PLASTICITY THEORY 87 σy εx = 0Figure 6.7. The normality principle applied to theTresca yield criterion. All stress states on the same εy = 0side of the locus cause the same shape change. Theshape changes at the corners are ambiguous. Biaxial σxtension can produce any shape change from ε y = 0to ε x = 0. εy = -εxFor the von Mises criterion, √ 1/2 σ = (1/ 2) (σ 2 − σ 3 )2 + (σ 3 − σ 1 )2 + (σ 1 − σ 2 )2 , (6.18)and for the Tresca criterion, σ = (σ 1 − σ 3 ). (6.19)Note that in a tension test, the effective stress reduces to the tensile stress, so both criteriapredict yielding when σ equals the current ﬂow stress. The effective strain, ε, is a mathematical function of the strain components, deﬁnedin such a way that ε reduces to the tensile strain in a tension test and that the plastic workper volume is dw = σ dε = σ 1 dε1 + σ 2 dε2 + σ 3 dε3 . (6.20)For the von Mises criterion, dε can be expressed as √ 1/2 dε = ( 2/3) (dε 2 − dε3 )2 + (dε 3 − dε1 )2 + (dε 1 − dε2 )2 (6.21)or as 1/2 dε = (2/3)1/3 dε1 2 + dε2 2 + dε3 2 , (6.22)which is completely equivalent. Example problem 6.8: Show that dε in Equations (6.21) and (6.22) reduces to dε 1 in a 1-direction tension test. SOLUTION: In a 1-direction tension test dε 2 = dε3 = −(1/2)dε 1 . Substituting into Equation (6.21), √ 1/2 dε = ( 2/3) (0)2 + [−(1/2)dε 1 − dε 1 ]2 + [dε1 − (−1/2)dε1 ]2 √ 1/2 = ( 2/3) (9/4)dε 1 2 + (9/4)dε 1 2 = dε1 . Substituting dε2 = dε3 = −(1/2)dε 1 into Equation (6.22), √ 1/2 dε = (2/3) dε 1 2 + (−1/2dε1 )2 + (−1/2dε1 )2 √ 1/2 = (2/3) dε1 2 + dε1 2 /4 + dε1 2 /4 = dε 1 .
- 106. 88 MECHANICAL BEHAVIOR OF MATERIALS If the straining is proportional (constant ratios of dε 1 : dε 2 : dε 3 ), the total effectivestrain can be expressed as 1/2 ε = (2/3) ε 1 2 + ε2 2 + ε3 2 . (6.23)If the straining is not proportional, ε must be found by integrating dε along the strainpath. The effective strain (and stress) may also be expressed in terms of nonprincipal strains(and stresses). For the von Mises criterion, 1/2 ε = (2/3) ε x 2 + ε y 2 + ε z 2 + (1/3) γ yz 2 + γ zx 2 + γ x y 2 (6.24)and √ σ = (1/ 2) (σ y − σ z )2 + (σ z − σ x )2 + (σ x − σ y )2 1/2 + 6 τ yz 2 + τ zx 2 + τ x y 2 . (6.25) For the Tresca criterion, the effective strain is the absolutely largest principal strain, dε = |dεi |max . (6.26) Although the Tresca effective strain is not widely used, it is of value because it is soextremely simple to ﬁnd. Furthermore, it is worth noting that the value of the von Miseseffective strain can never differ greatly from it. Always |dεi |max ≤ dεMises ≤ 1.15|dεi |max . (6.27)Equation (6.27) provides a simple check when the von Mises effective strain is calculated.If one calculates a value for dεMises that does not fall within the limits of Equation (6.27),a mistake has been made. As a material deforms plastically, the level of stress necessary to continue deformationincreases. It is postulated that the strain-hardening depends only on ε. In that case, thereis a unique relation, σ = f (ε). (6.28)Because, for a tension test, ε is the tensile strain and σ is the tensile stress, the σ − εcurve in a tension test is the σ − ε curve. Therefore the stress–strain curve in a tensiontest can be used to predict the stress–strain behavior under other forms of loading. Example problem 6.9: The strains measured on the surface of a piece of sheet metal after deformation are ε1 = 0.182, ε 2 = −0.035. The stress–strain curve in tension can be approximated by σ = 30 + 40ε. Assume the von Mises criterion and assume that the loading was such that the ratio of ε2 /ε 1 was constant. Calculate the levels of σ 1 and σ 2 reached before unloading. SOLUTION: First, ﬁnd the effective strain. With constant volume, ε 3 = − ε1 − ε2 = − 0.182 + 0.035 = −0.147. The Mises effective strain, ε = [(2/3)(ε 1 2 + ε2 2 + ε3 2 )]1/2 = [(2/3)(0.1822 + 0.0352 + 0.1472 )]1/2 = 0.193. [Note that this is larger than 0.182 and smaller than 1.15 × 0.182.] Since the tensile stress–strain curve is
- 107. PLASTICITY THEORY 89Figure 6.8. Yield loci for (σ 2 − σ 3 ) a + (σ 3 − σ 1 ) a +(σ 1 − σ 2 ) a = 2 Y a with several values of a. Note thatthe von Mises criterion corresponds to a = 2 and theTresca criterion to a = 1. the effective stress–effective strain relation, σ = 30 + 40ε = 30 + 40 × 0.193 = 37.7. At the surface, √ z = 0, so the effective stress func- σ tion can be written as σ /σ 1 = (1/ 2)[α 2 + 1 + (1 − α)2 ]1/2 = (1 − α + α 2 )1/2 . From the ﬂow rules with σ z = 0, ρ = dε 2 /dε 1 = (α − 1/2)/(1 − α/2). Solv- ing for α, α = (ρ + 1/2)/(1 + ρ/2). Substituting ρ = −0.035/0.182 = −0.192, α = (−0.192 + 1/2)/(1 − 0.192/2) = + 0.341, σ /σ 1 = [1 − α + α 2 ]1/2 = [1 − √ 0.341 + 0.3412 ]1/2 = 0.881. σ 1 = 0.881 σ = 37.7/0.881 = 42.8 and σ 2 = ασ 1 = 0.341 × 42.8 = 14.6.Other isotropic yield criteria. Von Mises and Tresca are not the only possible isotropic ∗criteria. Experimental data tend to lie between the two and can be represented by |σ 2 − σ 3 |a + |σ 3 − σ 1 |a + |σ 1 − σ 2 |a = 2Y a . (6.29)This criterion reduces to von Mises for a = 2 and a = 4, and to Tresca for a = 1 and a → ∞.For values of the exponent greater than 4, this criterion predicts yield loci between Trescaand von Mises, as shown in Figure 6.8. If the exponent, a, is an even integer, this criterioncan be written without the absolute magnitude signs as (σ 2 − σ 3 )a + (σ 3 − σ 1 )a + (σ 1 − σ 2 )a = 2Y a . (6.30)Theoretical calculations based on {111}<110> slip suggest an exponent of a = 8 for fccmetals. Similar calculations suggest that a = 6 for bcc. These values ﬁt experimentaldata as well.∗ W. F. Hosford, J. Appl. Mech. (Trans. ASME Ser E.) vol. 39E (1972): pp. 607–9.
- 108. 90 MECHANICAL BEHAVIOR OF MATERIALS Example problem 6.10: Derive the ﬂow rules for the high-exponent yield criterion, Equation (6.29). SOLUTION: When the yield function is expressed as f = (σ y − σ z )a + (σ z − σ x )a + (σ x − σ y )a , the ﬂow rules can be found from dε ij = dλ(df/dσ ij ): dε x = dλ[a(σ x − σ z )a−1 + a(σ x − σ y )a−1 ], dε y = dλ[a(σ y − σ x )a−1 + a(σ y σ z )a 1 ], and dε z = dλ[a(σ z − σ x )a−1 + a(σ z − σ y )a−1 ]. These can be expressed as dεx : dεy : dεz = [(σ x − σ z )a−1 + (σ x − σ y )a−1 ] : [(σ y − σ x )a−1 + (σ y − σ z )a−1 ] : [(σ z − σ x )a−1 + (σ z − σ y )a−1 ]. (6.31)Anisotropic plasticityAlthough it is frequently assumed that materials are isotropic (have the same propertiesin all directions), they rarely are. There are two main causes of anisotropy. One cause ispreferred orientations of grains or crystallographic texture. The second is mechanicalﬁbering, which is the elongation and alignment of microstructural features such as in-clusions and grain boundaries. Anisotropy of plastic behavior is almost entirely causedby preferred orientations. ∗ The ﬁrst complete quantitative treatment of plastic anisotropy was in 1948 by Hill,who proposed an anisotropic yield criterion to accommodate such materials. It is ageneralization of the von Mises criterion, F(σ y − σ z )2 + G(σ z − σ x )2 + H (σ x − σ y )2 + 2Lτ yz 2 + 2Mτ zx 2 + 2N τ x y 2 = 1, (6.32)where the axes x, y, and z are the symmetry axes of the material (for example the rolling,transverse, and through-thickness directions of a rolled sheet). If the loading is such that the directions of principal stress coincide with the symmetryaxes and if there is planar isotropy (properties do not vary with direction in the x–y plane),Equation (6.32) can be simpliﬁed to (σ y − σ z )2 + (σ z − σ x )2 + R(σ x − σ y )2 = (R + 1)X 2 , (6.33)where X is the yield strength in uniaxial tension. For plane stress (σ z = 0), Equation (6.33) plots as an ellipse, as shown in Figure 6.9.The higher the value of R, the more the ellipse extends into the ﬁrst quadrant. Thus thestrength under biaxial tension increases with R as suggested earlier. The corresponding ﬂow rules are obtained by applying the general equation, dε ij =dλ(∂f/∂σ ij ) (Equation (6.14)), where now f(σ ij ) is given by Equation (6.33): dεx : dεy : dεz = [(R + 1)σ x − Rσ y − σ z ] : [(R + 1)σ y − Rσ x − σ z ] : [2σ z − σ y − σ x ]. (6.34)∗ R. Hill, Proc. Roy. Soc, vol. 193A (1948): pp. 281–97.
- 109. PLASTICITY THEORY 91 2 R=5 plane strain εy=0 R=3 1.5Figure 6.9. Plane stress (σ z = 0) yield lo- R=2 σycus predicted by the Hill 1948 yield crite-rion for planar isotropy (Equation (6.33)) R=1 R=.5with several values of R. The dashed R=0 1line is the locus of stress states that pro-duce plane strain (ε y = 0). Note that thestrength under biaxial tension increaseswith R. A high R indicates a resistance to 0.5thinning in a tension test, which is con-sistent with high strength under biaxialtension where thinning must occur. FromW. F. Hosford, The Mechanics of Crystalsand Textured Polycrystals, copyright 1993 0 σxby Oxford University Press. Used by per- 0 0.5 1 1.5 2mission of Oxford University Press Inc. −0.5 −1This means that ρ = ε y /ε x for σ z = 0 and α = σ y /σ x for σ z = 0 are related by ρ = [(R + 1)α − R]/[(R + 1) − Rα] (6.35)and α = [(R + 1)ρ + R]/[(R + 1) + Rρ]. (6.36)Note that if R = 1, these reduce to Equation (6.15); the effective stress is 1/2 σ = (σ y − σ z )2 + (σ z − σ x )2 + R(σ x − σ y )2 /(R + 1) . (6.37)For σ z = 0, σ /σ x = {[α 2 + 1 + R(1 − α)2 ]/(R + 1)}1/2 . (6.38)The effective strain function is given as ε/ε x = (σ 1 /σ )(1 + αρ). (6.39) The Hill criterion often overestimates the effect of the R-value on the ﬂow stress. Amodiﬁcation of Equation (6.33), referred to as the high-exponent criterion, was suggested ∗to overcome this difﬁculty, (σ y − σ z )a + (σ z − σ x )a + R(σ x − σ y )a = (R + 1)X a , (6.40)∗ W. F. Hosford, 7th North Amer. Metalworking Conference., SME, Dearborn, MI, 1979, pp. 191−7 and R. W. Logan and W. F. Hosford, Int. J. Mech. Sci., Vol. 22 (1980): pp. 419−30.
- 110. 92 MECHANICAL BEHAVIOR OF MATERIALS σy/Y σy/Y a=6 a=2 a=6 1 1 a=2 Tresco R=0.5 R=2 Tresco 0 0 1 σx/Y 1 σx/Y 6 6 2 2−1 −1Figure 6.10. Yield loci predicted by the high-exponent criterion for planar isotropy. The loci for the 1948 Hillcriterion correspond to a = 2. Note that with a high exponent, there is much less effect of R on strength underbiaxial tension. From W. F. Hosford, ibid.where a is an even exponent much higher than 2. Calculations based on crystallographicslip have suggested that a = 6 is appropriate for bcc metals and a = 8 for fcc metals.Figure 6.10 compares the yield loci predicted by this criterion and the Hill criterion forseveral levels of R. With this criterion, the ﬂow rules are dε x : dε y : dε z = [R(σ x − σ y )a−1 + (σ x − σ z )a−1 ] : [(σ y − σ z )a−1 + R(σ y − σ x )a−1 ] : [(σ z − σ x )a−1 + (σ z − σ y )a−1 ]. (6.41) The effective stress function corresponding to Equation (6.28) is σ = [(σ y − σ z )a + (σ z − σ x )a + R(σ x − σ y )a ]/(R + 1)}1/a . (6.42)The effective strain function is ε = (σ x /σ )(1 + αρ), (6.43)where α = (σ y − σ z )/(σ x − σ y ) and ρ = ε y /ε x . Although the nonlinear ﬂow rules for the high-exponent criterion (Equation (6.41))cannot be explicitly solved for the stresses, iterative solutions with calculators or personalcomputers are simple. The nonquadratic yield criterion and accompanying ﬂow rules(Equations (6.40) and (6.41)) have been shown to gived better ﬁt to experimental datathan the quadratic form (Equations (6.33) and (6.34)).
- 111. PLASTICITY THEORY 93 σy σy σx σx kinematic hardening isotropic hardening a bFigure 6.11. The effect of strain-hardening on the yield locus. The isotropic model (a) predicts an expansionof the locus. The kinematic hardening model predicts a translation of the locus in the direction of the loadingpath. Example problem 6.11: A steel sheet, which has an R-value of 1.75 in all directions in the sheet, was stretched in biaxial tension with σ z = 0. Strain measurements in- dicate that throughout the deformation εy = 0. Find the stress ratio, α = σ y /σ x , that prevailed according to the Hill yield criterion (Equation (6.33)) and according to the nonquadratic yield criterion (Equation (6.40)) with a = 8. SOLUTION: For the Hill criterion Equation (6.36) gives α = [(R + 1)(ρ) + R]/[R + 1 + Rρ]. With ρ = 0, α = R/(R + 1) = 1.75/2.75 = 0.636. For the nonquadratic criterion, the ﬂow rules (Equation (6.41)) with σ z = 0 and ρ = 0 can be expressed as 0 = dε y /dεx = [α a−1 + R(α − 1)a−1 ]/[R(1 − α)a−1 + 1] = [α 7 − 1.75(1 − α)7 ]/[1.75(1 − α)7 + 1]. Trial and error solution gives α = 0.520.Effect of strain-hardening on the yield locusAccording to the isotropic hardening model, the effect of strain-hardening is simply toexpand the yield locus without changing its shape. The stresses for yielding are increasedby the same factor along all loading paths. This is the basic assumption that σ = f (ε)(Equation (6.28)). The isotropic hardening model can be applied to anisotropic materials.It does not imply that the material is isotropic. An alternative model is kinematic hardening. According to this model, plastic defor-mation simply shifts the yield locus in the direction of the loading path without changingits shape or size. If the shift is large enough, unloading may actually cause plastic de-formation. The kinematic model is probably better for describing small strains after achange in load path. However, the isotropic model is better for describing behavior duringlarge strains after a change of strain path. Figure 6.11 illustrates both models.NOTESOtto Z. Mohr (1835–1918) worked as a civil engineer, designing bridges. At 32, he was appointeda professor of engineering mechanics at Stuttgart Polytecknium. Among other contributions, he
- 112. 94 MECHANICAL BEHAVIOR OF MATERIALSdevised the graphical method of analyzing the stress at a point. He then extended Coulomb’s ideathat failure is caused by shear stresses into a failure criterion based on maximum shear stress,or diameter of the largest circle. For cast iron, he proposed that the different fracture stresses intension, shear, and compression could be combined into a single diagram, in which the tangentsform an envelope of safe stress combinations. This is essentially the Tresca yield criterion. It maybe noted that early workers used the term “failure criteria,” which failed to distinguish betweenfracture and yielding.Lame assumed a maximum stress theory of failure. However, later a maximum strain theory, of ´which Poncelet and Saint-Venant were proponents, became generally accepted. They proposedthat failure would occur when a critical strain was reached, regardless of the stress state.In letters to William Thomson, James Clerk Maxwell (1831–1879) proposed that “strain energy ofdistortion” was critical, but he never published this idea and it was forgotten. M. T. Huber, in 1904,ﬁrst formulated the expression for “distortional strain energy,”U = [1/(12G)][(σ 2 − σ 3 )2 + (σ 3 −σ 1 )2 + (σ 1 − σ 2 )2 ], where U = σ yp 2 /(6G). The same idea was independently developed by vonMises (Gottinger. Nachr. (1913): p. 582), for whom the criterion is generally called. It is also referred ¨to by the names of several people who independently proposed it: Huber and Hencky, as well asMaxwell. It is also known as the “maximum distortional energy” theory and the “octahedral shearstress” theory. The ﬁrst name reﬂects that the elastic energy in an isotropic material, associatedwith shear (in contrast to dilatation) is proportional to the left-hand side of Equation (6.10). Thesecond name reﬂects that the shear terms, (σ 2 − σ 3 ), (σ 3 − σ 1 ), and (σ 1 − σ 2 ), can be representedas the edges of an octahedron in principal stress space.In 1868, Tresca presented two notes to the French Academy. From these, Saint-Venant establishedthe ﬁrst theory of plasticity based on the assumptions that1. plastic deformation does not change the volume of a material,2. directions of principal stresses and principal strains coincide, and3. the maximum shear stress at a point is a constant.The Tresca criterion is also called the Guest or the maximum shear stress criterion.REFERENCESR. Hill, The Mathematical Theory of Plasticity, Oxford Univ. Press, 1950.W. A. Backofen, Deformation Processing, Addison–Wesley, 1972.W. F. Hosford and R. M. Caddell, Metal Forming: Mechanics and Metallurgy, second ed., Prentice–Hall, 1993.PROBLEMS 1. For the Mises yield criterion with σ z = 0, calculate the values of σ x /Y at yielding if A. α = 1/2 B. α = 1 C. α = −1 D. α = 0 where α = σ y /σ x .
- 113. PLASTICITY THEORY 95 σxFigure 6.12. Plane-strain tensile specimen. Lateral grip sectioncontraction of material in the groove is constrainedby material outside the groove. y gauge section z 2. For each of the values of α in problem 1, calculate the ratio ρ = dε y dε x . 3. Repeat problems 1 and 2 assuming the Tresca criterion instead of the Mises criterion. 4. Repeat problems 1 and 2 assuming the following yield criterion: (σ 2 − σ 3 )a + (σ 3 − σ 1 )a + (σ 1 − σ 2 )a = 2Y a , where a = 8. 5. Consider a plane-strain tension test in which the tensile stress is applied along the x-direction as shown in Figure 6.12. The strain, ε y , is zero along the trans- verse direction and the stress in the z-direction vanishes. Assuming the von Mises criterion, write expressions for A. σ as a function of σ x , and B. dε as a function of dε x . C. Using the results of parts A and B, write an expression for the incremental work per volume, dw, in terms of σ x and dε x . D. Derive an expression for σ x as a function of εx in such a test, assuming that the strain hardening can be expressed by σ = K ε n . 6. A 1.00-cm-diameter circle was printed onto the surface of a sheet of steel before forming. After forming, the circle was found to be an ellipse with major and minor diameters of 1.18 cm and 1.03 cm, respectively. Assume that both sets of measurements were made when the sheet was unloaded, that during forming the stress perpendicular to the sheet surface was zero, and that the ratio, α, of the stresses in the plane of the sheet remained constant during forming. The tensile stress–strain curve for this steel is shown in Figure 6.13. Assume the von Mises yield criterion. A. What were the principal strains, ε 1 , ε 2 , and ε 3 ? B. What was the effective strain, ε? C. What was the effective stress, σ ? D. Calculate the ratio ρ = ε 2 /ε 1 and use this to ﬁnd the ratio α = σ 2 /σ 1 . (Take σ 1 and σ 2 respectively as the larger and smaller of the principal stresses in the plane of the sheet.) E. What was the level of σ 1 ?
- 114. 96 MECHANICAL BEHAVIOR OF MATERIALS 500 400 True stress, MPa 300 Figure 6.13. True tensile stress- strain curve for the steel in Problem 200 6. 100 0 0 0.1 0.2 0.3 0.4 true strain 7. Measurements on the surface of a deformed sheet after unloading indicate that e1 = 0.154 and e2 = 0.070. Assume that the von Mises criterion is appropriate and that the loading was proportional (i.e., the ratio α = σ y /σ x remained constant during loading). It has been found that the tensile stress–strain relationship for this alloy can be approximated by σ = 150 + 185ε, where σ is the true stress in MPa and ε is the true strain (see Figure 6.14). A. What was the effective strain? B. What was the effective stress? C. What was the value of the largest principal stress? 8. The following yield criterion has been proposed for an isotropic material: “Yield- ing will occur when the sum of the diameters of the largest and second largest Mohr’s circles reaches a critical value.” Deﬁning σ 1 ≥ σ 2 ≥ σ 3 , this can be expressed mathematically this can be expressed as follows: (σ 1 − σ 2 ) ≥ (σ 2 − σ 3 ), (σ 1 − σ 2 ) + (σ 1 − σ 3 ) = C or 2σ 1 − σ 2 − σ 3 = C, (1) but if (σ 2 − σ 3 ) ≥ (σ 1 − σ 2 ), (σ 1 − σ 3 ) + (σ 2 − σ 3 ) = C or σ 1 + σ 2 − 2σ 3 = C. (2) Evaluate C in terms of the yield strength, Y, in uniaxial tension or the yield strength, − Y, in compression. Plot the yield locus as σ x versus σ y for σ z = 0, σ Figure 6.14. True tensile stress–strain curve for the σ = (150 + 185ε)MPa steel in Problem 7. ε
- 115. PLASTICITY THEORY 97 where σ x , σ y , and σ z are principal stresses. [Hint: For each region in σ x versus σ y stress space, determine whether (1) or (2) applies.] 9. Consider a long thin-wall tube, capped at both ends. It is made from a steel with a yield strength of 40,000 psi. Its length is 60 in., its diameter is 2.0 in., and the wall thickness is 0.015 in. The tube is loaded under an internal pressure P, and a torque of 1500 in.-lbs. is applied. A. What internal pressure can it withstand without yielding, according to Tresca? B. What internal pressure can it withstand without yielding, according to von Mises?10. In ﬂat rolling of a sheet or plate, the width does not appreciably change. A sheet of aluminum is rolled from 0.050 in. to 0.025 in. thickness. Assume the von Mises criterion. A. What is the effective strain, ε, caused by the rolling? B. What strain in a tension test (if it were possible) would cause the same amount of strain hardening?11. A piece of ontarium (which has a tensile yield strength of Y = 700 MPa) was loaded in such a way that the principal stresses, σ x , σ y , and σ z , were in the ratio 1 : 0 : −0.25. The stresses were increased until plastic deformation occurred. A. Predict the ratio of the principal strains, ρ = ε y /ε x , resulting from yielding according to von Mises. B. Predict the value of ρ = ε y /ε x resulting from yielding according to Tresca. C. Predict the value of σ x when yielding occurred according to von Mises. D. Predict the value of σ x when yielding occurred according to Tresca.12. A new yield criterion has been proposed for isotropic materials. It states that yielding will occur when the diameter of Mohr’s largest circle plus half of the diameter of Mohr’s second largest circle equals a critical value. This criterion can be expressed mathematically, following the convention that σ 1 ≥ σ 2 ≥ σ 3 , as (σ 1 − σ 3 ) + 1/2(σ 1 − σ 2 ) = C if (σ 1 − σ 2 ) ≥ (σ 2 − σ 3 ) and (σ 1 − σ 3 ) + 1/2(σ 2 − σ 3 ) = C if (σ 2 − σ 3 ) ≥ (σ 1 − σ 2 ). A. Evaluate C in terms of the tensile (or compressive) yield strength, Y. B. Let x, y, and z be directions of principal stress, and let σ z = 0. Plot the σ y versus σ x yield locus. (That is, plot the values of σ y /Y and σ x /Y that will lead toyielding according to this criterion.) [Hint: consider different loading paths (ratios of σ y /σ x ), and for each decide which stress (σ 1 , σ 2 , or σ 3 ) corresponds to (σ x , σ y , or σ z = 0); then determine
- 116. 98 MECHANICAL BEHAVIOR OF MATERIALS whether (σ 1 − σ 2 ) ≥ (σ 2 − σ 3 ), substitute σ x , σ y , and 0 into the appropriate expression, solve, and ﬁnally plot.]13. The tensile yield strength of an aluminum alloy is 14,500 psi. A sheet of this alloy is loaded under plane-stress conditions (σ 3 = 0) until it yields. On unloading it is observed that ε1 = 2ε2 and both ε1 and ε2 are positive. A. Assuming the von Mises yield criterion, determine the values of σ 1 and σ 2 at yielding. B. Sketch the yield locus and show where the stress state is located on the locus.14. Consider a capped thin-walled cylindrical pressure vessel made from a material with planar isotropy and loaded to yielding under internal pressure. Predict the ratio of axial to hoop strains, ρ = ε a /ε h , as a function of R, using A. The Hill criterion and its ﬂow rules (Equations (6.33) and (6.34)). B. The high-exponent criterion and its ﬂow rules (Equations (6.40) and (6.41)).15. In a tension test of an anisotropic sheet, the ratio of the width strain to the thickness strain, εw /εt , is R. A. Express the ratio ε2 /ε 1 of the strains in the plane of the sheet in terms of R. Take the 1-direction as the rolling direction, the 2-direction as the width direction in the tension test, and the 3-direction as the thickness direction. B. There is a direction, x, in the plane of the sheet along which e x = 0. Find the angle, θ, between x and the tensile axis. C. How accurately would this angle have to be measured to distinguish between two materials having R-values of 1.6 and 1.4?16. Redo Problem 6, assuming the Tresca criterion instead of the Von Mises criterion.17. The total volume of a foamed material decreases when it plastically deforms in tension. A. What does this imply about the effect of σ H = (σ 1 + σ 2 + σ 3 )/3 on the shape of the yield surface in σ 1 , σ 2 , σ 3 space? B. Would the absolute magnitude of the yield stress in compression be greater, smaller, or the same as the yield strength in tension? C. When it yields in compression, will the volume increase, decrease, or remain constant?
- 117. 7 Strain-Rate and Temperature Dependenceof Flow StressIntroductionFor most materials, an increase of strain rate raises ﬂow stress. The amount of the effectdepends on the material and the temperature. In most metallic materials the effect nearroom temperature is small and can often be neglected. A factor of 10 increase of strainrate may raise the level of the stress–strain curve by only 1 or 2%. On the other hand, atelevated temperatures, the effect of strain rate on ﬂow stress is much greater. Increasingthe strain rate by a factor of 10 may raise the stress–strain curve by 50% or more. Strain localization occurs very slowly in materials that have a high strain-rate depen-dence because less strained regions continue to deform. Under certain conditions, the ratedependence is high enough for materials to behave superplastically. Tensile elongationsof 1000% are possible. There is a close coupling of the effects of temperature and strain rate on the ﬂow stress.Increased temperatures have the same effects as decreased strain rate. This coupling canbe understood in terms of the Arrhenius rate equation.Strain-rate dependence of ﬂow stressThe average strain rate during most tensile tests is in the range of 10−3 to 10−2 /s. If ittakes 5 min during a tensile test to reach a strain of 0.3, the average strain rate is ε = ˙0.3/(5 × 60) = 10−3 /s. At a strain rate of ε = 10−2 /s a strain of 0.3 will occur in 30 s. ˙For many materials the effect of the strain rate on the ﬂow stress, σ , at a ﬁxed strain andtemperature can be described by a power-law expression, σ = C˙ m. ε (7.1)The exponent, m, is called the strain-rate sensitivity. The relative levels of stress at twostrain rates (measured at the same total strain) are given by σ2 /σ1 = (˙ 2 /˙ 1 )m , ε ε (7.2)or ln(σ 2 /σ 1 ) = m ln(˙ 2 /˙ 1 ). If σ2 is not much greater than σ1 , ε ε ln(σ2 /σ1 ) ≈ σ/σ. (7.3) 99
- 118. 100 MECHANICAL BEHAVIOR OF MATERIALS Table 7.1. Typical values of the strain-rate exponent, m, at room temperature Material m low-carbon steels 0.010 to 0.015 HSLA steels 0.005 to 0.010 austenitic stainless steels −0.005 to +0.005 ferritic stainless steels 0.010 to 0.015 copper 0.005 70/30 brass −0.005 to 0 aluminum alloys −0.005 to +0.005 α-titanium alloys 0.01 to 0.02 zinc alloys 0.05 to 0.08 Source: From various sources. Equation (7.2) can be simpliﬁed to σ/σ ≈ m ln(˙ 2 /˙ 1 ) = 2.3m log(˙ 2 /˙ 1 ). ε ε ε ε (7.4) At room temperature, the values of m for most engineering metals are between −0.005 and +0.015, as shown in Table 7.1. ε ε Consider the effect of a 10-fold increase in strain rate (˙ 2 /˙ 1 = 10) with m = 0.01. Equation ( 7.4) predicts that the level of the stress increases by only σ/σ = 2.3(0.01) (1) = 2.3%. This increase is typical of room-temperature tensile testing. It is so small that the effect of strain rate is often ignored. A plot of Equation (7.2) in Figure 7.1 shows how the relative ﬂow stress depends on the strain rate for several levels of m. The increase of ﬂow stress, σ/σ , is small unless either m or (˙ 2 /˙ 1 ) is high. ε ε 1.5 .5 .3 .2 .15 .10 1.4 .08 Figure 7.1. The dependence of ﬂow stress on strain rate for several values of 1.3 the strain-rate sensitivity, m, according toσ2/σ1 .06 Equation (7.2). From W. F. Hosford and R. M. Caddell, Metal Forming: Mechan- 1.2 ics and Metallurgy, Second ed., Prentice– .04 Hall, 1983. Reprinted by permission of Pearson Education, Inc., Upper Saddle River, NJ. 1.1 .02 .01 .005 1.0 1 2 5 10 20 50 100 1000 10000 ε2/ε1
- 119. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 101 Example problem 7.1: The strain-rate dependence of a zinc alloy can be represented by Equation (7.1) with m = 0.07. What is the ratio of the ﬂow stress at ε = 0.10 for a strain rate of 103 /s to that at ε = 0.10 for a strain rate of 10−3 /s? Repeat for a low carbon steel with m = 0.01. SOLUTION: For zinc (m = 0.07), σ2 /σ1 = (C εm2 )/(C εm1 ) = (˙ 2 /˙ 1 )m = ˙ ˙ ε ε −3 0.07 (10 /10 ) 3 = (10 ) 6 0.07 = 2.63. For steel (m = 0.01), σ2 /σ1 = (10 ) 6 0.01 = 1.15. Example problem 7.2: The tensile stress in one region of an HSLA steel sheet (m = 0.005) is 1% greater than that in another region. What is the ratio of the strain-rates in the two regions? Neglect strain-hardening. What would be the ratio of the strain rates in the two regions for a titanium alloy (m = 0.02)? SOLUTION: Using Equation (7.2), ε2 /˙ 1 = (σ2 /σ1 )1/m = (1.01)1/0.005 = 7.3. If m = ˙ ε 0.02, ε2 /˙ 1 = 1.64. The difference between the strain rates in differently stressed ˙ ε locations decreases with increasing values of m. Figure 7.2 illustrates two ways of determining the value of m. One method is to runtwo continuous tensile tests at different strain rates and compare the levels of stress at thesame ﬁxed strain. The other way is to change the strain rate suddenly during a test andcompare the levels of stress immediately before and after the change. The latter methodis easier and therefore more common. The two methods may give somewhat differentvalues for m. In both cases m is found from m = ln(σ2 /σ1 )/ln(˙ 2 /˙ 1 ). ε ε (7.5) For most metals, the value of the rate sensitivity, m, is low near room temperaturebut increases with temperature. The increase of m with temperature is quite rapid abovehalf of the melting point (T > T m /2) on an absolute temperature scale. In some cases,m may be 0.5 or higher. Figure 7.3 shows the temperature dependence of m for severalmetals. For some alloys there is a minimum between 0.2 T m and 0.3 T m . For aluminumalloy 2024, the rate sensitivity is slightly negative in this temperature range (see Fig-ure 7.4). . .Figure 7.2. Two methods of determining σ2 ε2 ε2 . .the strain-rate sensitivity. Either continu- ε1 σ2 ε1ous stress–strain curves at different strain σ1rates can be compared at the same strain . σ1 stress stress(left) or sudden changes of strain rate can ε1be made and the stress levels just beforeand just after the change can be compared(right). In both cases, Equation (7.5) canbe used to ﬁnd m. In rate-change tests, strain strain(ε2 /ε1 ) is typically 10 or 100. ˙ ˙
- 120. 102 MECHANICAL BEHAVIOR OF MATERIALS Copper Steel Aluminium 0.2 304 Stainless Strain-rate exponent, m Titanium Rene 41 Mo–T2C Figure 7.3. Variation of the strain-rate sensitivity, m, with temperature for several metals. Above about half of the melting point, m rises rapidly with tem- 0.1 perature. From W. F. Hosford and R. M. Caddell, ibid. 0 0 0.2 0.4 0.6 0.8 1.0 T/TmSuperplasticityIf the rate sensitivity, m, of a material is 0.5 or higher, the material will behave super-plastically, exhibiting very high tensile elongations. The high elongations occur becausethe necks are extremely gradual (like those that one observes when chewing gum is 0.16Strain-rate exponent, m 0.12 Figure 7.4. Temperature dependence of 2024-0 m for pure aluminum and aluminum alloy 0.08 2024. Note that at room temperature m is negative for 2024. From D. S. Fields Aluminum and W. A. Backofen, Trans. ASM, Vol. 51 (1959). 0.04 0 −200 0 200 400 T°C
- 121. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 103Figure 7.5. A titanium-alloy aircraft panel made by diffusion bonding and superplastic deformation. Threesheets were diffusion-bonded at a few locations and then internal pressurization of the unbonded channelscaused the middle sheet to stretch. Superplastic behavior is required because of the very high uniformextension required in the middle sheet. From W. F. Hosford and R. M. Caddell, ibid.stretched). Superplasticity permits forming of parts that require very high strains. Theconditions for superplasticity are1. Temperatures equal to or above half of the absolute melting point (T ≥ 0.5 T m ).2. Slow strain rates* (usually 10−3 /s or slower).3. Very ﬁne grain size (grain diameters of a few micrometers or less).Long times are needed to form useful shapes at low strain rates. With long times andhigh temperatures, grain growth may occur, negating an initially ﬁne grain size. For thisreason, most superplastic alloys either have two-phase structures or have a very ﬁnedispersion of insoluble particles. Both minimize grain growth. Under superplastic conditions, ﬂow stresses are very low and extremely high elon-gations (1000% or more) are observed in tension tests. Both low ﬂow stresses and highelongations can be useful in metal forming. The very low ﬂow stresses permit slow forg-ing of large, intricate parts with ﬁne detail. The very high tensile elongation makes itpossible to form very deep parts with simple tooling. Examples are shown in Figures7.5 and 7.6. The reason that very high tensile elongations are possible can be understood in termsof the behavior of a tensile bar having a region with a slightly reduced cross-sectionalarea (Figure 7.7). The following treatment is similar to the treatment in Chapter 5 of strainlocalization at defects. Assume now, however, that work-hardening can be neglected athigh temperatures and that Equation (7.1) describes the strain-rate dependence. Let Aa* Note that m is somewhat rate-dependent, so Equation (7.1) is not a complete description of the rate dependence. Nevertheless, m, deﬁned by m = ∂ln σ/∂ln ε, is a useful index for describing the rate sensitivity ˙ of a material and analyzing rate effects.
- 122. 104 MECHANICAL BEHAVIOR OF MATERIALSFigure 7.6. Complex part made from a sheet of a Zn–22%Al alloy. The very high strains in the walls requiresuperplasticity. From W. F. Hosford and R. M. Caddell, ibid.and Ab be the cross-sectional areas of the thicker and thinner regions. The force carriedby both sections is the same, so Fb = σb Ab = Fa = σa Aa . (7.6)Substituting σa = C εa , σb = C εb , Aa = Aao exp(−εa ), and Ab = Abo exp(−εb ), Equa- ˙m ˙mtion (7.6) becomes Abo exp(−εb )C εb = Aao exp(−εa )C εa . ˙m ˙m (7.7)Designating the ratio of the initial cross-sectional areas by Abo /Aao = f, fexp(−εb )˙ b = exp(−εa )˙ a . Now raising to the (1/m) power and recognizing that ε = εm εm ˙dε/dt, f 1/m exp(−ε b /m)dε b = exp(−ε a /m)dεa . Integration from zero to their currentvalues, ε b and ε a , results in exp(−εa /m) − 1 = f 1/m [exp(−εb /m) − 1]. (7.8) Under superplastic conditions the reduction in area is often quite large. The deforma-tion in the unnecked region can be approximated by letting εb → ∞ in Equation (7.8).In this case, the limiting strain in the unnecked region, εa is εa = −m ln(1 − f 1/m ). (7.9)Figure 7.8 shows how εa varies with m and f . Also shown are measured tensile elonga-tions, plotted assuming that εa = ln(%El/100 + 1). This plot suggests that values of fin the range from 0.99 to 0.995 are not unreasonable. The high values of m are a result of the contribution of diffusional processes to thedeformation. Two possible mechanisms are illustrated in Figure 7.9. One is a net diffu-sional ﬂux under stress of atoms from grain boundaries parallel to the tensile axis to grain Figure 7.7. Schematic of a tensile bar with one region (b) slightly smaller in a b a cross section than the other (a). Both must carry the same tensile force.
- 123. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 105 3 2000 1500 Ti-5 Al-2.5 Sn Zircaloy-4 Ti-6 Al-4V 1000 Pb-Sn Eutectic 2 Elongation, % 600 0.9 98 0.9 400εa * 0. 95 f= 0. 99 98 95 200 1 0. 90 0. 100 50 0 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 Strain-rate exponent, mFigure 7.8. Limiting strain, εa , in the unnecked portion of a tensile specimen as a function of f and m. Reportedvalues of total elongations are also shown as a function of m. These are plotted with the elongation convertedto true strain. From W. F. Hosford and R. M. Caddell, ibid.boundaries normal to the tensile axis, causing a tensile elongation. This amounts to anet diffusion of vacancies from grain boundaries normal to the tensile axis to boundariesparallel to it. The other possible mechanism is grain boundary sliding. With grain bound-ary sliding, compatibility where three grains meet must be accommodated by anothermechanism. Such accommodation could occur either by slip or by diffusion, but in bothcases the overall m would be below 1. Both diffusional creep and grain boundary slidingneed a very ﬁne grain size, high temperatures, and low strain rates. These mechanismsare discussed in more detail in Chapter 16.diffusional grain boundarycreep sliding diffusion regions of accomodationFigure 7.9. Sketches showing two possible mechanisms for superplastic deformation.
- 124. 106 MECHANICAL BEHAVIOR OF MATERIALS Example problem 7.3: A tensile bar is machined so that the diameter at one location is 1% smaller than that for the rest of the bar. The bar is tested at high temperature, so strain-hardening is negligible, but the strain-rate exponent is 0.25. When the strain in the reduced region is 0.20, what is the strain in the larger region? SOLUTION: f = (π D1 /4)/(π D2 /4) = (D1 /D2 )2 = (0.99/1)2 = 0.98. Substituting 2 2 εb = 0.20 and f = 0.98 into Equation (7.8), exp(−εa /m) −1 = f 1/m [exp(−ε a / m) − 1], exp(−εa /0.25) = (0.98)1/.25 [exp(−0.2/0.25) − 1] + 1 = 0.492. ε a = −0.25 ln(0.492) = 0.177. Figure 7.10 shows that for high values of m, the strain, ε a , in the region outside ofthe neck continues to grow even when the neck strain, ε b , is large. With low values of m,deformation outside of the neck ceases early.Combined strain and strain-rate effectsRate sensitivity may have appreciable effects at low temperatures, even when m is rela-tively small. If both strain and strain-rate hardening are considered, the true stress maybe approximated by σ = C ε n ε m. ˙ (7.10) Reconsider the tension test on an inhomogeneous tensile bar, with initial cross sectionsof Aao and Abo = fAoa . Substituting Aa = Aao exp(−εa ), Ab = Abo exp(−ε b ), σ a = C εa εa εm , n ˙and σ b = C εb εb ε into a force balance (Equation (7.6)) Fa = Aa σ a = Fb = Ab σ b , n ˙ m Aao exp(−εa )C εa εa m = Abo exp(−εb )C εb εb m. n ˙ n ˙ (7.11) 1 m = 0.60 m = 0.5 m = 0.40 0.8 f = 0.99 m = 0.30 0.6 m = 0.20εa Figure 7.10. Relative strains in unnecked 0.4 and necked regions for several values of rate sensitivity, m. 0.2 m = 0.10 0 0 0.2 0.4 0.6 0.8 1 εb
- 125. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 107Following the procedure leading to Equation (7.8), εa εb n/m exp(−εa /m)εa dεa = f 1/m n/m exp(−εb /m)εb dεb . (7.12) o oThis equation must be integrated numerically. The results are shown in Figure 7.11 forn = 0.2, f = 0.98, and several levels of m. Example problem 7.4: Reconsider the tension test in example problem 5.3. Let n = 0.226 and m = 0.012 (typical values for low carbon steel) and let f = 0.98 as in the previous problem. Calculate the strain, ε a , in the region with the larger diameter if the bar necks to a 25% reduction of area (ε b = ln(4/3) = 0.288.) SOLUTION: Substituting into Equation (7.12), εa εb n/m exp(−εa /m)εa dεa = f 1/m n/m exp(−εb /m)εb dεb o oor εa εb exp(−83.33εa )εa dεa = 0.1587 18.83 exp(−83.33εb )εb dεb . 18.83 o o Numerical integration of the right-hand side gives 0.02185. The left-hand side has the same value when εa = 0.2625. The loss of elongation in the thicker section is much less than that in Example Problem 5.3, where it was found that ε a = 0.195 with n = 0.226 and m = 0.Strain-rate sensitivity of bcc metalsFor bcc metals, including steels, a better description of the strain-rate dependence of ﬂowstress is given by σ = C + m ln ε , ˙ (7.13) m = 0.1 0.3 f = 0.98 0.05 n = 0.20Figure 7.11. Comparison of the strains 0.025 0.2in the reduced and unreduced sections εa 0.01of a tensile bar for a material that strain-hardens and is strain-rate sensitive. From 0.0W. F. Hosford and R. M. Caddell, ibid. 0.1 0 0.1 0.2 0.3 0.4 εb
- 126. 108 MECHANICAL BEHAVIOR OF MATERIALS 1 1 ε2 > ε1 ε2 > ε1 ε1 ε1 StressStress 0.5 0.5 0 0 0 0.1 0.2 0.3 0.4 0 0.1 0.2 0.3 0.4 Strain Strain A B Figure 7.12. Two possible effects of strain rate on stress–strain curves. The stain rates for the two stress– strain curves in each ﬁgure differ by a factor of 100. (A) Equation (7.3) predicts that the difference in ﬂow stress, σ , is proportional to the ﬂow stress, σ . (B) Equation (7.14) predicts that the difference in ﬂow stress, σ , is independent of the ﬂow stress, σ . where C is the ﬂow stress at a reference strain rate and m is the rate sensitivity. This expression indicates that a change of strain rate from ε1 to ε2 raises the ﬂow stress by an amount σ = m ln(˙ 2 /˙ 1 ). ε ε (7.14) which is independent of the stress level. This is in contrast to Equation (7.3), which predicts σ ≈ σ m ln(˙ 2 /˙ 1 ). The difference between the predictions of Equations (7.3) ε ε and (7.14) is illustrated in Figures 7.12a and 7.12b. This difference is also apparent in comparing Figures 7.13 and 7.14. For copper (fcc) at 25◦ C the difference between the stress–strain curves at different rates, σ , is proportional to the stress level. In contrast, the difference between the stress–strain curves at different rates, σ , for pure iron (bcc) at 25◦ C is independent of the stress level. 600 500 400 Figure 7.13. Stress–strain curves for Stress, MPa copper (fcc) at 25◦ C room temperature. Note that the difference, σ , between the 300 ε (s−t) stress–strain curves at different rates is 0.00014 0.015 proportional to the stress level. From P. S. 200 .82 Follansbee and U. F. Kocks, Acta Met., 81 Vol. 36 (1988): pp. 81–93. 1800 100 5000 8500 0 0.0 0.2 0.4 0.6 0.8 1.0 True strain
- 127. Figure 7.14. Stress–strain curves for iron (bcc) at 25◦ C. Note that the difference, σ , between the stress–strain curves at different rates is independent of the stress level. From G. T. Gray, in ASM Metals Handbook,Vol. 8, 2000. Example problem 7.5: Figure 7.15 is a plot of measured strain-rate exponents, m, for a large number of steels as a function of the ﬂow stress at which they were measured. Find the value of m in Equation (7.14) that best ﬁts the data in Figure 7.15. Figure 7.15. Correlation between the strain-rate exponent, m, and the static ﬂow stresses of steels. Each point represents a different steel. From W. F. Hosford and R. M. Caddell, ibid. Data from A. Saxena and D. A. Chatﬁeld, SAE Paper 760209, 1976. SOLUTION: Comparing Equations (7.3) and (7.14), σ = σ m ln(˙ 2 /˙ 1 ) = m ln(˙ 2 /˙ 1 ) ε ε ε ε indicates that m = mσ . Drawing a smooth curve through the data in Figure 7.15 and picking several values, m = 0.05 × 200 MPa = 10 MPa, m = 0.025 × 400 MPa = 10 MPa, m = 0.0125 × 800 MPa = 10 MPa. It is apparent that m = 10 MPa describes the data well. 109
- 128. 110 MECHANICAL BEHAVIOR OF MATERIALS 500 strain rate 10 400 1.0 0.1 0.01Stress, MPa 300 Figure 7.16. True stress–strain curves calculated 200 with σ = 520ε0.22 + 10 ln ε for several strain rates. ˙ 100 0 0 0.05 0.1 0.15 0.2 0.25 Strain For steels, the strain-hardening exponent, n, decreases with increasing strain rate. Thisis a result of the additive nature of the rate dependence. For power-law strain hardening,the constant, C, in Equation (7.16) is K ε n , so Equation (7.13) becomes σ = K εn + m ln ε. ˙ (7.15)Figure 7.16 is a plot of Equation (7.15) for K = 520 MPa, n = 0.22, and m = 10 MPafor several strain rates. In a plot of the same stress–strain curves on logarithmic scales(Figure 7.17), the average slope decreases as the strain rate increases. Because the con-ventional strain-hardening exponent, n, is taken as the average slope, n decreases withstrain rate (Figure 7.18).Temperature dependenceAs temperature increases, the whole level of the stress–strain curve generally drops.Figure 7.19 shows the decrease of tensile strengths of copper and aluminum. Usually therate of work hardening also decreases at high temperatures, as shown for aluminum inFigure 7.20. 500 strain rate 10Stress, MPa 1.0 0.1 0.01 Figure 7.17. The same stress–strain curves as in Fig- 200 ure 7.16, plotted on logarithmic scales. Note that the slope decreases with increasing strain rate. 100 0.01 0.02 0.05 0.10 0.20 Strain
- 129. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 111 0.25 Strain-hardening exponent, n 0.2Figure 7.18. The decrease of n withstrain rate calculated from Figure 7.17. 0.15 0.01 0.1 1 10 strain rate, 1/sCombined temperature and strain-rate effectsThe effects of temperature and strain rate are interrelated. Decreasing temperature hasthe same effect as increasing strain rate, as shown schematically in Figure 7.21. Thiseffect occurs even in temperature regimes where the rate sensitivity is negative. The simplest treatment of temperature dependence of strain rate is that of Zener *and Hollomon , who treated plastic straining as a thermally activated rate process. Theyassumed that strain rate follows an Arrhenius rate law, rate ∝ exp(−Q/RT ), that is widelyused in analyzing many temperature-dependent rate processes. They proposed ε = A exp(−Q/RT ), ˙ (7.16)where Q is the activation energy, T is the absolute temperature, and R is the gas constant.At a ﬁxed strain, A is a function only of stress, A = A(σ ), so Equation (7.19) can be Figure 7.20. Decrease of the strain-hardening expo-Figure 7.19. Tensile strengths decrease with in- nent of aluminum with increasing temperature. Fromcreasing temperature. Data from R. P. Carrecker and Hosford and Caddell, using data from R. P. CarreckerW. R. Hibbard Jr., Trans. TMS-AIME, Vol. 209 (1957). and W. R. Hibbard Jr., ibid.* C. Zener and H. Hollomon, J. Appl. Phys. Vol. 15 (1944): pp. 22–32.
- 130. 112 MECHANICAL BEHAVIOR OF MATERIALS Figure 7.21. Schematic plot showing the tempera- ture dependence of ﬂow stress at two different strain rates. Note that an increased strain rate has the same effects as a decreased temperature. From W. F. Hosford and R. M. Caddell, ibid.written A(σ ) = ε exp(+Q/RT ) ˙ (7.17)or A(σ ) = Z , (7.18)where Z = ε exp(+Q/RT ) is called the Zener–Hollomon parameter. ˙ Equation (7.20) predicts that a plot of strain at constant stress on a logarithmic scaleversus 1/T should be linear. Figure 7.22 shows that such a plot for aluminum alloy 2024is linear for a wide range of strain rates although the relation fails at high strain rates, Example problem 7.6: For an aluminum alloy under constant load, the creep rate increased by a factor of 2 when the temperature was increased from 71 to 77◦ C. Find the activation energy. Figure 7.22. Combinations of strain rate and temperature for several stresses in aluminum alloy 2024. The data are taken at an effective strain of 1.0. Data from D. S. Fields and W. A. Backofen, ibid.
- 131. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 113 SOLUTION: Since ε = A exp (−Q/RT ), the ratio of the creep rates at two temperatures ˙ is ε2 /˙ 1 = exp[(−Q/R)(1/T2 − 1/T1 )], so Q = R ln(˙ 2 /˙ 1 )/(1/T1 − 1/T2 ). Substitut- ˙ ε ε ε ing T1 = 273 + 71 = 344 K, T2 = 273 + 77 = 350 K, R = 8.314 J/mole · K, and ε2 /˙ 1 = 2 and solving, Q = 116 kJ/mole. Compare this with Figure 7.23. ˙ ε The Zener–Hollomon development is useful if the temperature and strain-rate rangesare not too large. Dorn and co-workers measured the activation energy, Q, for purealuminum over a very large temperature range. They did this by observing the changeof creep rate under Q ﬁxed load when the temperature was suddenly changed. Since thestress is constant, ε2 /˙ 1 = exp[(−Q/R)(1/T2 − 1/T1 )] ˙ ε (7.19)or Q = R ln(˙ 2 /˙ 1 )/(1/T1 − 1/T2 ). ε ε (7.20) Their results (Figure 7.23) indicated that Q was independent of temperature above500 K, but very temperature-dependent at lower temperatures. This observation waslater explained by Z. S. Basinski and others. The basic argument is that the stress helpsthermal ﬂuctuations overcome activation barriers. This is illustrated in Figure 7.24. Ifthere is no stress, the activation barrier has a height of Q, with random ﬂuctuations.The rate of overcoming the barrier is proportional to exp(−Q/RT ). An applied stressskews the barrier so that the effective height of the barrier is reduced to Q − σ v, wherev is a parameter with the units of volume. Now the rate of overcoming the barrier isproportional to exp[−(Q − σ v)/RT ]. The ﬁnding of lower activation energies at lowertemperatures was explained by the fact that in the experiments, greater stresses wereapplied at lower temperatures to achieve measurable creep rates. In Figure 7.24, the rate of the overcoming of the barrier from left to right isproportional to exp[−(Q − σ v)/RT ], whereas the rate from right to left is propor-tional to exp[−(Q + σ v)/RT ]. Thus the net reaction rate is C{exp[−(Q − σ v)/RT ] −exp[−(Q + σ v)/RT ]} = C exp(−Q/RT ){exp[(σ v)/RT ] − exp[−(σ v)/RT ]}. This sim-pliﬁes to ε = 2C exp(−Q/RT ) sinh[(σ v)/RT ]. ˙ (7.21) 160 148Figure 7.23. Measured activation ener-gies for creep of aluminum as a func- 120 117 Q, kJ/moletion of temperature. The change of Qwith temperature indicates that Equation 80(7.20) will lead to errors if it is applied overa temperature range in which Q changes. 40Data from O. D. Sherby, J. L. Lytton, andJ. E. Dorn, AIME Trans., Vol. 212 (1958). 0 0 200 400 600 800 1000 Temperature, K
- 132. 114 MECHANICAL BEHAVIOR OF MATERIALSFigure 7.24. Schematic illustration of the skewing of an activation barrier by an applied stress. From W. F.Hosford and R. M. Caddell, ibid.This expression has been modiﬁed, based on some theoretical arguments, to provide abetter ﬁt with the experimental data, ε = A exp(−Q/RT )[sinh(ασ )]1/m , ˙ (7.22)where α is an empirical constant and the exponent 1/m is consistent with Equation (7.1).Figure 7.25 shows that Equation (7.22) can be used to correlate the combined effects oftemperature, stress, and strain – rate over an extremely large range of strain rates. If ασ 1, sinh(ασ ) ≈ ασ , Equation ( 7.22) simpliﬁes to ε = A exp(+Q/RT )(ασ )1/m ˙ (7.23) σ = ε m A exp(−m Q/RT ) ˙ (7.24) σ = A Zm, (7.25)where A = (αAm )−1 . Equation (7.25) is consistent with the Zener–Hollomon de-velopment. At low temperatures and high stresses, (ασ ) 1, so sinh(ασ ) → exp(ασ )/2 10000000 creep (204 to 593°C) torsion (195 to 550°C) 10000 compression (250 to 550°C)Z/A1 = (ε/A1)exp[Q/RT)] 10 Figure 7.25. Plot of the Zener–Hollomon pa- rameter versus ﬂow-stress data for aluminum over a very wide range of strain-rates. Data are 0.01 from J. J. Jonas, Trans. Q. ASM, Vol. 62 (1969). slope = 4.7 α = 43 Pa−1 0.00001 Q = 157 kJ/mole0.00000001 0.01 0.1 1 10 100 sinh(ασ)
- 133. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 115and Equation (7.22) reduces to ε = C exp(α σ − Q/RT ). ˙ (7.26) Under these conditions both C and α depend on strain and temperature. For a constanttemperature and strain, σ = C + m ln ε. ˙ (7.27) Note that this equation is consistent with Equation (7.13) but not with the power-lawrate expression, Equation (7.1).Hot workingMetallurgists make a distinction between cold working and hot working. It is often saidthat hot working is done above the recrystallization temperature and the work materialrecrystallizes as it is deformed. This is an oversimpliﬁcation. The strain rates duringhot working are often so high that there is not enough time for recrystallization duringthe deformation. It is more meaningful to think of hot working as a process in whichrecrystallization occurs in the period between repeated operations, as in forging, rolling,etc., or at least before the work material cools from the working temperature to roomtemperature. Tool forces during hot working are lowered not only by the recrystallization itself,but also because of the inherently lower ﬂow stresses at high temperatures. A secondadvantage of hot working is that the resulting product is in an annealed state. There are,however, disadvantages of hot working. Among these are the following:1. The work metal tends to oxidize. In the case of steel and copper-base alloys this results in scale formation and a consequent loss of metal. Titanium alloys must be hot-worked under an inert atmosphere to avoid dissolving oxygen.2. Lubrication is much more difﬁcult and consequently friction much higher. This effect somewhat negates the effect of lower ﬂow stress.3. The scaling and high friction result in tool wear and shortened tool life.4. The resulting product surface is rough because of the scale, tool wear, and poor lubrication. There is also loss of precise gauge control.5. The lack of strain hardening in hot working is, in some cases, undesirable. Usually ingot breakdown and subsequent working are done hot until the section sizebecomes small enough so that high friction and the loss of material by oxidation becomeimportant. Hot rolling of steel sheets is continued to a thickness of 0.050 to 0.200 in.Then the product is pickled in acid to remove the scale and ﬁnished by cold working toobtain a good surface. Most cold-rolled sheet is sold in an annealed condition. With steels, the term cold-rolled refers to the surface quality rather than the state of work-hardening. The termwarm working is used to refer to working of metals above room temperature, but at a lowenough temperature so that recrystallization does not occur.
- 134. 116 MECHANICAL BEHAVIOR OF MATERIALSNOTESSvante August Arrhenius (1859–1927) was a Swedish physical chemist. He studied at Uppsala,where he obtained his doctorate in 1884. It is noteworthy that his thesis on electrolytes wasgiven a fourth (lowest) level pass because his committee was skeptical of its validity. From 1886to 1890 he worked with several noted scientists in Germany who did appreciate his work. In1887, he suggested that a very wide range of rate processes follow what is now known as theArrhenius equation. For years his work was recognized throughout the world, except in his nativeSweden. Count Rumford (Benjamin Thompson) was the ﬁrst person to measure the mechanical equiv-alent of heat. He was born in Woburn, Massachusetts in 1753, studied at Harvard, and taught inConcord, New Hampshire, where he married a wealthy woman. At the outbreak of the AmericanRevolution, having been denied a commission by Washington, he approached the British, whodid commission him. When the British evacuated Boston in 1776 he left for England, where hemade a number of experiments on heat. However, he was forced to depart quickly for Bavariaafter being suspected of selling British naval secrets to the French. In the Bavarian army he roserapidly to become Minister of War and eventually Prime Minister. While inspecting a cannon fac-tory, he observed a large increase in temperature during the machining of bronze cannons. Hemeasured the temperature rise and with the known heat capacity of the bronze, he calculatedthe heat generated by machining. By equating this to the mechanical work done in machining,he was able to deduce the mechanical equivalent of heat. His value was a little too low, in partdue to the fact that some of the plastic work done in machining is stored as dislocations in thechips. Thompson was knighted in 1791, choosing the title Count Rumford after the original name ofConcord. During his rapid rise to power in Bavaria he made many enemies, so when the windsof politics changed, he had to leave. He returned to Britain as an ambassador from Bavaria, butthe British refused to recognize him. During this period, he established the Royal Institute. At thistime, the United States was establishing the U.S. Military Academy at West Point, and Rumfordapplied and was selected to be its ﬁrst commandant. However, during the negotiations abouthis title, it was realized that he had deserted the American cause during the Revolution and theoffer was withdrawn. He ﬁnally moved to Paris where he married the widow of the famous Frenchchemist, Lavoisier, who had been beheaded during the French revolution.REFERENCESJohn H. Hollomon and Leonard Jaffe, Ferrous Metallurgical Design, Wiley, 1947.W. F. Hosford and R. M. Caddell, Metal Forming: Mechanics and Metallurgy, 2nd ed., Prentice–Hall, 1993.PROBLEMS 1. During a tension test the rate of straining was suddenly doubled. This caused the load (force) to rise by 1.2%. Assuming that the strain-rate dependence can be described by σ = C ε m , what is the value of m? ˙ 2. Two tension tests were made on the same alloy, but at different strain rates. Both curves were ﬁtted to a power-law strain-hardening expression of the form σ = K ε n . The results are summarized as follows:
- 135. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 117 Test A Test B −1 −3 strain rate (s ) 2 × 10 10−1 strain-hardening exponent, n 0.22 0.22 constant, K (MPa) 402 412 Assuming that the ﬂow stress at constant strain can be approximated by σ = C εm , ˙ determine the value of m. 3. To save weight in an automobile, replacement of a low-carbon steel with an HSLA steel is being considered. In laboratory tension tests at a strain rate of 10−3 /s, the yield strengths of the HSLA steel and the low carbon steel were measured to be 400 and 220 MPa, respectively. The strain-rate exponents are m = 0.005 for the HSLA steel and m = 0.015 for the low carbon steel. What percent weight saving could be achieved if the substitution was made so that the forces were the same at strain rates of 10+3 , typical of crash conditions? 4. The thickness of a cold-rolled sheet varies from 0.0322 to 0.0318 depending on where the measurement is made, so strip tensile specimens cut from the sheet show similar variations in cross section. A. For a material with n = 0.20 and m = 0, what will be the thickness of the thickest regions when the thinnest region necks? B. Find the strains in the thickest region if m = 0.50 and n = 0 when the strain in the thinnest region reaches i. 0.5, ii. ∞. 5. Estimate the total elongation of a superplastic material if A. n = 0, m = 0.5, and f = 0.98, B. n = 0, f = 0.75, and m = 0.8. 6. In superplastic forming, it is often necessary to control the strain rate. Consider the forming of a hemispherical dome by clamping a sheet over a circular hole and bulging it with gas pressure. A. Compare the gas pressure needed to form a 2.0-in. dome with that needed to form a 20-in. dome if both are formed from sheets of the same thickness and at the same strain rate. B. Describe (qualitatively) how the gas pressure should be varied during the form- ing to maintain a constant strain rate. 7. During a constant-load creep experiment on a polymer, the temperature was sud- denly increased from 100 to 105◦ C. It was found that this increase of temperature caused the strain rate to increase by a factor of 1.8. What is the apparent activation energy for creep of the plastic?
- 136. 118 MECHANICAL BEHAVIOR OF MATERIALS Stress, ksi 15 20 25 30 35 40 45 50 Steady-state creep rate (εss),s1 10−5 10−6 10−7 Figure 7.26. The effects of stress and tem- perature on the strain rate of nickel-base su- peralloy single crystals under stress. ASM, 10−8 From Metals Handbook, ninth ed., Vol. 8, 1000 °C (1830 °F) 925 °C (1700 °F) 1985, p. 306. 10−9 10−10 10−11 100 150 200 250 300 350 Stress, MPa 8. Figure 7.26 gives some data for the effect of stress and temperature on the strain rate of a nickel-base super alloy single crystal. The strain rate is independent of the strain in the region of this data. Determine as accurately as possible. A. The activation energy, Q, in the temperature range from 700 to 810◦ C. B. The exponent, m, for 780◦ C. 9. It has been suggested that ε = A exp[−(Q − σ v)/RT ] − A exp[−(Q + σ v)/ ˙ RT ] is a better representation of the dependence of strain rate on temperature Figure 7.27. Stress–strain curves for silver (fcc). Note that at 25◦ C the difference, σ , between the stress–strain curves at different rates is proportional to the stress level. From G. T. Gray in ASM Metals Handbook, Vol. 8, 2000.
- 137. STRAIN-RATE AND TEMPERATURE DEPENDENCE OF FLOW STRESS 119 and stress than the Holloman–Zener approach. Using this equation, derive an expression for the dependence of stress on strain rate if σ v Q.10. The stress–strain curve of a steel is represented by σ = (1600 MPa)ε0.1 . The steel is deformed to a strain of ε = 0.1 under adiabatic conditions. Estimate the temperature rise in the sample. For iron, ρ = 7.87 kg/m2 , C = 0.46.J/g · ◦ C, and E = 205 GPa.11. Evaluate m for copper at room temperature from Figure 7.13.12. The stress–strain curves for silver at several temperatures and strain rates are shown in Figure 7.27. Determine the strain-rate exponent m for silver at 25◦ C.
- 138. 8 SlipIntroductionPlastic deformation of crystalline materials usually occurs by slip, which is the slidingof planes of atoms over one another (Figure 8.1). The planes on which slip occursare called slip planes and the directions of the shear are the slip directions. These arecrystallographic planes and directions that are characteristic of the crystal structure. Themagnitude of the shear displacement is an integral number of interatomic distances, so thatthe lattice is left unaltered. If slip occurs on only part of a plane, there remains a boundarybetween the slipped and unslipped portions of the plane, which is called a dislocation.Slip occurs by movement of dislocations through the lattice. It is the accumulation ofthe dislocations left by slip that is responsible for work hardening. Dislocations and theirmovement are treated in Chapters 9 and 10. This chapter is concerned only with thegeometry of slip. Visual examination of the surface of a deformed crystal will reveal slip lines. Thefact that we can see these indicates that slip is inhomogeneous on an atomic scale.Displacements of thousands of atomic diameters must occur on discrete or closelyspaced planes to create steps on the surface that are large enough to be visible. Fur-thermore, the planes of active slip are widely separated on an atomic scale. Yet thescale of the slip displacements and distances between slip lines is small compared tomost grain sizes, so slip usually can be considered as homogeneous on a macroscopicscale.Slip systemsThe slip planes and directions for several common crystals are summarized in Table 8.1.Almost without exception the slip directions are the crystallographic directions withthe shortest distance between like atoms or ions and the slip planes are usually denselypacked planes.120
- 139. SLIP 121Table 8.1. Slip directions and planesStructure Slip direction Slip planesfcc <110> {111}bcc <111> {110}, {112}, {123}, pencil glideahcp <1120> (0001), {1100}, {1101} <1123>b {1101}dia. cub. <110> {111}NaCl <110> {110}CsCl <001> {100}Fluorite <110> {001}, {110} b , {111} ba With pencil glide, slip is possible on all planes containing the slip direction.b <1123>slip has been reported for many hcp crystals under special loading conditions or at high temperatures. slip directionFigure 8.1. Slip by shear between parallel planesof atoms. slip offset slip planeSchmid’s lawErich Schmid∗ discovered that if a crystal is stressed, slip begins when the shear stresson a slip system reaches a critical value, τc , often called the critical resolved shear stress.In most crystals, slip occurs with equal ease forward or backward,† so the conditionnecessary for slip can be written as τnd = ±τc . (8.1)The subscripts n and d refer to the slip plane normal and the direction of slip, respec-tively. This simple yield criterion for crystallographic slip is called Schmid’s law. In auniaxial tension test along the x-direction, the shear stress can be found from the stresstransformation (Equation 1.6), τnd = l nx l dx σ x x . (8.2)Schmid’s law is usually written as τc = ±σ x cos λ cos ϕ, (8.3)∗ E. Schmid, Proc. Internat. Cong. Appl. Mech., Delft, 1924, p. 342.† Bcc crystals are exceptions. The stress required to cause slip in one direction is less than that for the opposite direction.
- 140. 122 MECHANICAL BEHAVIOR OF MATERIALS Figure 8.2. Slip elements in uniaxial tension.where λ is the angle between the slip direction and the tensile axis, and φ is the an-gle between the tensile axis and the slip-plane normal (Figure 8.2), so ldx = cos λ andl nx = cos φ. Equation (8.3) can be shortened to σ x = ±τc /m x , (8.4)where mx is the Schmid factor, m x = cos λ cos φ. The condition for yielding under a general stress state is ± τc = l nx l dx σ x x + l ny l dy σ yy + · · · + (l nx l dy + l ny l dx )σ x y . (8.5) Example problem 8.1: A tensile stress of σ = 5 kPa is applied parallel to the [432] direction of a cubic crystal. Find the shear stress, τ , on the (111) plane in the [011] direction. SOLUTION: First ﬁnd m = cos λ cos φ for (111)[011] slip. In cubic crystals, the normal to a plane has the same indices as the plane, so the normal to (111) is [111]. Also, in cubic crystals, the cosine of the angle between two directions is given by the dot product of unit vectors in those directions. Therefore 2 cos φ = (4·1 + 3·1 + 2·1)/[(42 + 32 + 22 )1/2 (12 + 12 + 1 )1/2 ] √ √ = 5/( 29 3), cos λ = (4·0 + 3·1 + 2·1)/[(42 + 32 + 22 )1/2 (02 + 12 + 12 )1/2 ] √ √ = 5/( 29 2), √ m = cos λ cos φ = 25/(29 6) = 0.352, τ = mσ = 0.352 × 5 kPa = 1.76 kPa.
- 141. SLIP 123 Example problem 8.2: A cubic crystal is subjected to a stress state, σ x = 15 kPa, σ y = 0, σ z = 7.5 kPa, τyz = τzx = τx y = 0, where x = [100], y = [010], and z = [001]. What is the shear stress on the (111)[101] slip system? See Figure 8.3. σz = 0.75 [101] (111) σy = 0 Figure 8.3. Cubic crystal in Example Problem 8.2. σx = 1.5 SOLUTION: τnd = l nx l dx σ x + l nz l dz σ z , where d = [101] and n = [111]. Taking dot products, √ 2 l nx = [111]·[100] = (1·1 + 1·0 + 1·0)/ [(12 + 12 + 1 )(12 + 02 + 02 )] √ = 1/ 3, √ l dx = [101]·[100] = (1·1 + 0·0 + 1·0)/ [(12 + 02 + 12 )(12 + 02 + 02 )] √ = 1/ 2, √ 2 l nz = [111]·[001] = (1·0 + 1·0 + 1·1)/ [(12 + 12 + 1 )(02 + 02 + 12 )] √ = −1/ 3, √ l dz = [101]·[001] = (1·0 + 0·0 + 1·1)/ [(12 + 02 + 12 )(02 + 02 + 12 )] √ = 1/ 2. Substituting, √ √ √ √ τnd = (1/ 3)(1/ 2)15 kPa + (−1/ 3)(1/ 2)7.5 kPa √ = 7.5/ 6 = 3.06 kPa.Strains produced by slipThe incremental strain transformation equations (Equation (1.24)) may be used to ﬁndthe shape change that results from slip when the strains are small (i.e., when the latticerotations are negligible). For inﬁnitesimal strains, dε x x = l xn 2 dεnn + l xd 2 dε dd + · · · l xnl xd dγ nd . (8.6)
- 142. 124 MECHANICAL BEHAVIOR OF MATERIALSWith slip on a single slip system in the d direction and on the n plane the only strain termon the right-hand side of Equation (8.6) is dγ nd , so we can write dε x x = l xnl xd dγ nd . (8.7)In Schmid’s notation this is dε x x = cos λ cos φ dγ = mdγ , (8.8)where dγ is the shear strain on the slip system. The other strain components, referred tothe x, y, and z axes, are similarly dε yy = l ynl yd dγ , dε zz = l znl zd dγ , dγ yz = (l ynl zd + l ydl zn )dγ , (8.9) dγ zx = (l znl xd + l zdl xn )dγ , dγ x y = (l xnl yd + l xdl yn )dγ . Example problem 8.3: If slip occurs on the (111)[101] slip system in Example Prob- lem 2, what will be the ratios of the resulting strains, dε y /dε x and dε z /dε x , where x = [100], y = [010], and z = [001]? √ SOLUTION: dε x = l nx l dx γ nd = 1/ 6dγ nd and dε y = l ny l dy dγ nd . Substituting l ny = √ [111]·[010] = 1/ 3 and l dy = [101]·[010] = 0, dε y = 0, dε z = l nz l dz γ nd = −1/ √ 6dγ nd .Therefore, dε y /dε x = 0 and dε z /dε x = −1. For a polycrystalline material to have appreciable ductility, each of its grains mustbe able to undergo the same shape change as the entire body. That is, each grain in apolycrystal must deform with the same external strains as the whole polycrystal. For anindividual grain this amounts to an imposed set of strains ε1 , ε2 , γ 23 , γ 31 , γ 12 along thecrystal axes. Five independent strains, ε1 , ε 2 , γ 23 , γ 31 , γ 12 , describe an arbitrary strainstate or shape change. The third normal strain, ε 3 , is not independent, because ε 3 = −ε1 − ε 2 . If a material has less than ﬁve independent slip systems, a polycrystal of thatmaterial will have very limited ductility unless another deformation mechanism suppliesthe added freedom necessary. The number of independent slip systems is the same as thenumber of strain components, ε1 , ε 2 , γ 23 , γ 31 , γ 12 , that can be independently satisﬁedby slip. Example problem 8.4: The number of independent slip systems is the same as the number of strain components, ε1 , ε2 , γ 23 , γ 31 , γ 12 , that can be accommodated by slip. Find the number of independent slip systems in crystals of the NaCl structure that deform by <110>{110} slip.
- 143. SLIP 125 SOLUTION: Let the [100], [010], and [001] directions be designated as 1, 2, and 3 respectively and let the slip systems be designated as follows: [011](011) and [011](011) as Aa, [101](101) and [101](101) as Bb, and [110](110) and [110](110) as Cc. The strains along the cubic axes can be written as e1 = l 1Al 1a γ Aa + l 1Bl 1b γ Bb + l 1Cl 1c γ Cc = 0 + (1/2)γ Bb + (1/2)γ Cc e2 = l 2Al 2a γ Aa + l 2Bl 2b γ Bb + l 2Cl 2c γ Cc = 0 + (1/2)γ Aa + (1/2)γ Cc γ 23 = (l 2Al 3a + l 2al 3A )γ Aa + (l 2Bl 3b + l 2bl 3B )γ Bb + (l 2Cl 3c + l 2cl 3C )γ Cc γ 31 = (l 3Al 1a + l 3al 1A )γ Aa + (l 3Bl 1b + l 3bl 1B )γ Bb + (l 3Cl 1c + l 3cl 1C )γ Cc γ 12 = (l 1Al 2a + l 1al 2A )γ Aa + (l 1Bl 2b + l 1bl 2B )γ Bb + (l 1Cl 2c + l 1cl 2C )γ Cc. Substituting gives √ √ l 1A = [100]·[110] = 1/ 2, l 1a = [100]·[110] = 1/ 2, l 1B = [100]·[101] √ = 1/ 2, √ l 1b = [100]·[101] = 1/ 2, l 1C = [100]·[011] = 0, l 1c = [100]·[011] = 0, √ √ l 2A = [010]·[110] = 1/ 2, l 2a = [010]·[110] = −/ 2, l 2B = [010]·[101] = 0, √ √ l 2b = [010]·[101] = 0, l 2C = [010]·[011] = 1/ 2, l 2c = [010]·[011] = 1/ 2, √ l 3A = [001]·[110] = 0, l 3a = [001]·[110] = 0, l 3B = [001]·[101] = 1/ 2, √ √ l 3b = [001]·[101] = −1/ 2, l 3C = [001]·[011] = 1/ 2, l 3c = [001]·[011] √ = −1/ 2. Substituting (l 2Al 3a + l 2al 3A ) = (l 2Bl 3b + l 2bl 3B ) = (l 2Cl 3c + l 2cl 3C ) = 0 etc., it can be concluded that γ 23 = γ 31 = γ 12 = 0, so the shear strains γ 23 , γ 31 , and γ 12 cannot be satisﬁed. Therefore there are only two independent strains, ε1 and ε 2 , and so there are only two slip systems that are independent.Strain-hardening of fcc single crystalsFigure 8.4 is a typical stress–strain curve for an fcc single crystal. Initially slip occurson a single plane and the rate of strain hardening is very low. This low strain-hardeningrate is similar to that in crystals of hcp metals and is called easy glide or stage I. Atsome point, slip is observed on other systems. The result is that dislocations on differentslip systems intersect, causing much more rapid strain hardening. The result is a highand nearly constant rate of strain-hardening in stage II. Lower temperatures increase theextent of stage II. At higher strains, in stage III, the rate of strain hardening decreases. The extent of easy glide in a crystal depends on its orientation, its perfection, and thetemperature. A high degree of crystal perfection and a low temperature promote moreeasy glide. Likewise, the extent of easy glide is greater in orientations for which theresolved shear stress on other potential systems is low. Easy glide does not occur in fcccrystals oriented so that slip occurs simultaneously on many slip systems. Instead the
- 144. 126 MECHANICAL BEHAVIOR OF MATERIALS 40 easy glide stage II stage III 30shear stress, MPa 20 10 0 0 0.1 0.2 0.3 0.4 0.5 shear strainFigure 8.4. Schematic shear stress–shear strain curve for a typical single crystal of a fcc metal, showing aninitial stage of easy glide, a second stage with rapid and almost constant hardening rate, and ﬁnally a thirdstage in which the rate of strain-hardening decreases.initial strain-hardening rate is rapid and comparable with that in polycrystals (Figure8.5). No easy glide is observed in bcc single crystals. Extensive easy glide is observedin tension tests of single crystals of those hcp metals, which slip primarily on the basal(0001) plane (e.g., Zn, Cd, Mg).Tensile deformation of fcc crystalsIt is customary to represent the tensile axis in the basic stereographic triangle with [100],[110], and [111] corners, as shown in Figure 8.6. (Details of the stereographic projectionare given in Appendix B.) For all orientations of fcc crystals within this triangle, theSchmid factor for slip in the [101] direction on the (111) plane is higher than that for anyother slip system. Slip in this primary slip system should be expected. If the tensile axisis represented as lying in any other stereographic triangle, the slip elements may be foundby examining the remote corners of the three adjacent triangles. The <111> direction inone of the adjacent triangles is the normal to the slip plane and the <110> direction inanother adjacent triangle is the slip direction. Figures 8.7 and 8.8 show the orientation dependence of the Schmid factor, m, withinthe basic triangle. The highest value, m = 0.5, occurs where the tensile axis lies on the Figure 8.5. Stress–strain curves for polycrystalline aluminum and aluminum single crystals. Note that both the polycrystal and the <111>-oriented crys- tal strain-harden rapidly. Strain-hardening in orien- tations with only a single slip system (shaded region) is much lower. From U. F. Kocks, Acta Met. Vol. 8, (1960).
- 145. SLIP 127 101 111Figure 8.6. Basic orientation triangle. If the ten-sile axis of an fcc crystal lies in this triangle, themost heavily stressed slip system is [101](111). FromW. F. Hosford, The Mechanics of Crystals and Tex-tured Polycrystals, Oxford University Press, 1993. 100 110 111 mmin = 0.272 [101] 111 211 221 λ = 45° mmax = 0.500 321 311 0.408 311 mmax = 0.500 0.490 100 310 210 110 ϕ = 45° [111]Figure 8.7. Orientation dependence of the Schmid factor for fcc crystals. From W. F. Hosford, ibid. .28 [111] .32 .36 30 .40 .44 20 0.44 φ 0.48 10 .44 0.5[100] [110] 0 15 30 45 θFigure 8.8. Full representation of contours of constant Schmid factor for fcc crystals. From W. F. Hosford,ibid.
- 146. 128 MECHANICAL BEHAVIOR OF MATERIALSgreat circle between the slip direction and the slip-plane normal with λ = 45◦ andϕ = 45◦ . If the tensile axis lies on a boundary of the basic triangle, two slip systems areequally favored. They are the ones most favored in the two triangles that form the bound-ary. For example, if the tensile axis is on the [100]–[111] boundary, the second systemis [110](111), which is called the conjugate system. Two other systems have names:[101](111) is the critical slip system, and the system that shares the slip direction withthe primary system, [101](111), is called the cross-slip system. At the corners there arefour, six, or eight equally favored slip systems.Slip in bcc crystalsThe slip direction in bcc metals is always the direction of close packing, <111>. Slip hasbeen reported on various planes, {110}, {123}, and {112}. All of these planes containat least one <111> direction. G. I. Taylor suggested that slip in bcc crystals could bedescribed as <111>-pencil glide. This term means that slip can occur on any planethat contains a <111> slip direction. Figure 8.9 shows the orientation dependence ofthe Schmid factors for uniaxial tension with <111>-pencil glide. Note that the basicorientation triangle is divided into two regions, with a different <111> slip direction ineach.Slip in hcp crystalsWith all the hcp metals, the most common slip direction is <1120>. This is the directionof close contact between atoms in the basal plane. Several slip planes have been reported, [111] 0.22 0.38 30 0.4 slip direction = [111] 0.42 0.44 0.46 20 slip direction = [111] 0.48 φ 0.48 0.49 0.495 0.49 10 0.5 0.5 0.495 0.49 0.48 0.49 0.48 [110][100] 0 10 20 30 40 θFigure 8.9. Plot of Schmid factors for <111>-pencil glide of bcc cr ystals. The basic triangle is divided intotwo regions with different slip directions. The Schmid factor is 0.417 at [100] and [110] and it is 0.314 at [111].From W. F. Hosford, ibid.
- 147. SLIP 129Figure 8.10. Stresses necessary to operate severalslip systems in beryllium. Compression parallel to thec-axis can be accommodated only by pyramidal slip,which requires a very high stress. From a talk by W.R. Blumenthal, C. N. Tome, C. R. Necker, G. T. Gray, ´and M. C. Mataya.as indicated in Table 8.1. Slip in the <1120> direction causes no strains parallel to thec-axis, regardless of the plane of slip. Pyramidal slip on <1123>{1101} has been reportedfor a few hcp metals at high temperatures or under special loading conditions. Figure8.10 shows the shear stresses required for several slip systems in beryllium. The stressesrequired for pyramidal slip are much higher than the stresses to cause basal and prismslip and are often high enough to cause fracture. Twinning, unlike slip, does producec-direction strains.Lattice rotation in tensionSlip normally causes a gradual lattice rotation or orientation change. Figure 8.11 showsthe elongation of a long single crystal by slip on a single slip system. As the crystalis extended, the orientation of the tensile axis changes relative to the crystallographicelements. In Figure 8.11 the slip plane and slip direction are represented as being ﬁxedin space with the tensile axis rotating relative to these, whereas in a real tension test, thetensile axis would remain vertical and the crystal elements would rotate. The deformationby slip is like shearing a deck of cards or a stack of poker chips on the top of a table. Thefollowing geometric treatment of the orientation change during tension is essentially thatof Schmid and co-workers. Slip causes translation of point P parallel to the slip direction to a new position, P .Points C and C are constructed by extending the slip direction through O and constructingperpendiculars from P and P to the extension of the slip direction. The normal distance between OCC and PP is not changed by slip, so PC = P C .Substituting PC = l o sin λo and P C = l sin λ, l o sin λo = l sin λ, sin λo / sin λ = l/l o = 1 + e, or sin λ = sin λo /(1 + e), (8.10)where e = (l − l o )/l o = l/l o is the engineering strain.
- 148. 130 MECHANICAL BEHAVIOR OF MATERIALSFigure 8.11. Extension of a long thin crystal. Slip causes point P to move to P . (A). Points C and C areconstructed by extending the slip direction through point O and dropping normals from P and P . (B). PointsB and B’ are constructed by dropping normals from P and P to the slip plane through O. Similarly, slip does not change the distance between two parallel slip planes. By ananalogous construction it can be shown that cos φ = cos φ o /(1 + e). (8.11)The shear strain, γ , associated with the slip is γ = P P /PB = OC /PB − OC/PB. (8.12)Substituting OC = l cos λ, OC = l o cos λo , and PB = l o cos φ o = l cos φ, Equation(8.12) becomes γ = l cos λ/l cos φ − l o cos λo /l o cos φ o , or γ = cos λ/ cos φ − cos λo / cos φ o . (8.13) It is clear from Figure 8.11 and Equations (8.11) and (8.11) that φ increases and λdecreases during tensile extension. The orientation change in tension is a simple rotationof the slip direction toward the tensile axis. For an fcc crystal oriented in the basic triangle,the tensile axis will rotate toward [101] until it reaches the [100]–[111] boundary (Figure8.12a). At this point slip starts on [110](111), which is the system most favored in theconjugate triangle. With equal slip on the two systems, the net rotation of the tensile axisis toward [211] (Figure 8.12b). The rotation along the [100]–[111] boundary becomesslow as the tensile axis approaches [211], which would be the stable end orientation ifthe crystal could be extended inﬁnitely. The tensile axis of a bcc crystal deforming by pencil glide rotates toward the active<111> slip direction. For orientations near [110] and [111] (region A), the tensile axiswill rotate toward [111], as indicated in Figure 8.13. For crystal orientations in the basictriangle near [100] (region B), the rotation will be toward [111]. Once the tensile axis
- 149. SLIP 131Figure 8.12. (a) Primary slip in the [101] direction causes the tensile axis to rotate toward [101]. (b) Once thetensile axis reaches the [100]−[111] symmetry line, simultaneous slip in the [101] and [110] directions causesa rotation toward [211]. From W. F. Hosford, ibid.enters region A, the rotation will be toward [111]. When the [100]–[110] boundary isreached, combined slip in the [111] and [111] directions will cause rotation toward [110],which is the stable end orientation.Lattice rotation in compressionFor the compression of thin ﬂat single crystals, the compression axis rotates toward theslip-plane normal as sketched in Figure 8.14. For an fcc crystal, the compression axisrotates toward [111] until it reaches the [100]–[110] boundary, as shown in Figure 8.15.Then simultaneous slip on the (111) and (111) planes will cause a net rotation toward[110], which is the stable end orientation. compression axis slip-plane normal φo compression slip-plane axis normal φFigure 8.13. Rotation of the tensile axis for a in a bcccrystal deforming by <111>-pencil glide. If the tensileaxis is in region B, rotation toward [111] will carry itinto region A. In region A, slip in the [111] direction will Figure 8.14. Compression causes a rotation of therotate the tensile axis to the [100]−[110] symmetry slip-plane normal toward the compression axis,line, where duplex slip will cause a net rotation toward which is equivalent to a rotation of the compression[110]. From W. F. Hosford, ibid. axis toward the slip-plane normal.
- 150. 132 MECHANICAL BEHAVIOR OF MATERIALS Figure 8.15. In an fcc crystal, the compression axis rotates toward [111] until it reaches the [100]–[110] symmetry line, where duplex slip causes a net rota- tion toward [110]. From W. F. Hosford, ibid. For pencil glide, rotation toward the compression axis is equivalent to rotation awayfrom the active slip direction. Figure 8.16 shows that for bcc crystals, orientations initiallyin region A will end up rotating to [111], whereas those initially in region A will rotatetoward [100].Texture formation in polycrystalsIn polycrystalline metals, the grains undergo similar rotations, and these lead to crys-tallographic textures or preferred orientations. Table 8.2 shows that the experimentallyobserved textures developed in tensile extension and compression of polycrystals are inmost cases the same as the end orientations predicted for single crystals. Clearly the preferred orientations (crystallographic textures) are the result of the lat-tice rotation that accompanies slip. Such preferred orientations cause anisotropy of both Figure 8.16. For a bcc crystal deforming by <1117>- pencil glide, compression causes a rotation of orien- tations in region B away from [111] toward [100]. Ori- entations in region A rotate away from [111]. When they reach the [100]−[111] symmetry line, simultane- ous slip on the [111] and [111] directions causes a net rotation toward [111].
- 151. SLIP 133Table 8.2. Comparison of theoretical end orientations with preferred orientations Single crystals: end orientations Polycrystals: preferred orientationCrystal structure andslip systems Tension Compression Tension Compressionfcc {111}<110> <112> <110> <100> & <111> <110>bcc <111>-pencil glide <110> <100> & <111> <110> <100> & <111>hcp (0001)<1120> <1120> [0001] <1120> [0001]hcp {1100)<1120> <1010> [0001] <1010> [0001] and {1101)<1120>elastic and plastic properties. A rigorous analysis of slip in polycrystals and texture for-mation is much more complicated. However, the agreement between the end orientationspredicted for single crystals and the textures observed in polycrystals suggests that slipon the most highly stressed slip system plays the dominant role in texture formation.Approximate calculation of R-valuesFor textured sheets, it is possible to predict R-values (ratios of width to thickness strains,ε w /ε t , in tension tests). To do this, attention is focused on the most highly stressed slipsystem. Once this system has been identiﬁed, the strains in the x, y, z coordinate systemcan be calculated in terms of the shear strain, γ , on the slip system. The ratio, ε w /ε t , isthe R-value. Example problem 8.5: Consider a copper sheet with a (011)[211] texture. Predict the R-values in a tension test parallel to the [211] prior rolling direction. SOLUTION: Let x = [211] and z = [011]. The transverse direction must be y = [211] × [011] = [111]. Copper is fcc. The most favored slip systems would be (111)[101] and (111)[110]. Consider tension applied along [211]. For slip on (111)[101], the resulting strains can be found as ε x = γ cos λx cos φ x cos λx = [211]·[101] = {(2·1 + 1·0 + 1·1)/[(22 + 12 + 12 )(12 + 02 + 12 )]1/2 } √ = 3/ (6·2) 2 cos φ x = [211]·[111] = {(2·1 + 1·1 + 1·1)/[(22 + 12 + 12 )(12 + 12 + 1 )]1/2 √ = 2/ (6·3) so √ ε x = γ (1/ 6), ε z = γ cos λz cos φ z ; 2 cos λz = [011]·[101] = {(0·1 + 1·0 + 1·1)/[(02 + 12 + 1 )(12 + 02 + 12 )]1/2 } √ = 1/ (2·2)
- 152. 134 MECHANICAL BEHAVIOR OF MATERIALS 2 2 cos φ z = [011]·[111] = {(0·1 + 1·1 + 1·1)/[(02 + 12 + 1 )(12 + 12 + 1 )]1/2 } √ = 2/ (2 · 3) so √ ε z = γ (−1/ 6), ε y = γ cos λ y cos φ y ; 2 cos λ y = [111]·[101] = {(1·1 + 1·0 + 1·1)/[(12 + 12 + 1 )(12 + 02 + 12 )]1/2 } √ = 0/ (3·2) 2 2 cos φ y = [111]·[111] = {(1·1 + 1·1 + 1·1)/[(12 + 12 + 1 )(12 + 12 + 1 )]1/2 } √ = 1/ (3·3) so ε y = 0. Dividing, R = ε y /ε z = 0. Analysis of slip on the (111)[110] system would have resulted in exactly the same conclusion.NOTESCrystallographic slip was reported as early as 1867 by Reusch, who observed it in NaCl crystals.The ﬁrst report of slip lines in metals was by Ewing and Rosenhain in 1899. Slip was extensivelystudied in the early part of the 20th century. Two classic books were written in 1935 and 1936. Onewas Kristallplastizitat mit besonderer Berucksichtigung der Metalle, Springer-Verlag, Berlin, 1935, ¨ ¨by Erich Schmid and W. Boas. This was written in German and under Hitler it was forbidden tohave a German book translated into another language. After World War II, the Allies took Germancopyrights and the book was translated and published by F. A. Hughes and Co. Ltd., 1950, underthe title Plasticity of Crystals with Special Reference to Metals. The second book was Distortionof Crystals, 1936, by Constance F. Elam, who later published under the name Mrs. G. H. Tipper.Later W. Boas published An Introduction to the Physics of Metals and Alloys, Melbourne UniversityPress, 1947. Erich Schmid (May 4, 1896–Oct. 22, 1983) was born in Bruck-on-the-Mur in Austria and stud-ied in Vienna. His studies were interrupted by service in the First World War. He obtained hisdoctorate in 1920 and remained at the Technische Hochschule in Vienna for two years. In 1922,he left Austria for 30 years to work in various places in Germany and Switzerland. In Berlin he didresearch on metal crystals and formulated what is known today as “Schmid’s law.” During this pe-riod he introduced physical concepts into the study of metals to supplement the earlier chemicalconcepts. His research with Dehlinger and Sachs forms the basis for much of the present under-standing of the mechanical behavior of metals. During the Second World War Schmid worked ondeveloping and improving substitute materials. In 1951, he returned to the University of Viennain Austria and remained there until 1967. He served as President of the Austrian Academy ofScience for 10 years and was responsible for the establishment of several research institutes. Hewas awarded honorary doctorates by several technical universities in Germany and in 1979 wasrecognized with Austria’s highest achievement award. Scientiﬁc organizations and institutes inGermany, Austria, and Japan have given him numerous honors. In the 1930s Boas emigrated from Germany to Australia to escape the Nazi persecution ofJews. He spent the remainder of his career at Melbourne University.
- 153. SLIP 135Figure 8.17. Taylor’s illustration of shearing a pack of pencils. The direction of shearing is ﬁxed (parallel tothe pencils) but shearing can occur on any plane. From G. I. Taylor, Proc. Roy. Soc. Vol. 112 (1926). Geoffrey Ingram Taylor (1886–1975) was born in London. He contributed a steady stream ofimportant papers, principally on ﬂuid mechanics and plasticity. His grandfather was George Boole,who is renowned for developing the foundations of what is now called Boolean algebra. Taylor didboth his undergraduate studies and his graduate research at Cambridge. Taylor never receiveda doctorate, simply because Cambridge did not grant them until many years later. During theFirst World War, he did research at Farnsborough on aircraft. After the war he was appointedlecturer at Cambridge and remained there until his death. Taylor must be regarded as one of themost outstanding scientists of the ﬁrst half of the 20th century. His work with turbulent ﬂow isfundamental. Taylor’s studies of plasticity ranged from testing continuum models, to experimentsand analysis of slip in single crystals, to pioneering work that bridged the gap between crystaland continuum mechanics. He is regarded as one of the founders of dislocation theory, alongwith Orowan and Polanyi. Taylor coined the term pencil glide to describe slip in bcc metals onany plane containing a <111> slip direction. He chose the term because slip in one directionon any plane is similar to the behavior of a pile of pencils. Figure 8.17 is a copy of his illustra-tion.REFERENCESW. A. Backofen, Deformation Processing, Addison–Wesley, 1972.C. S. Barrett, Structure of Metals, McGraw–Hill, 1943.B. D. Cullity, Elements of X-Ray Diffraction, Addison–Wesley, 1956.W. F. Hosford, The Mechanics of Crystals and Textured Polycrystals, Oxford University Press, 1993.E. Schmid and W. Boas, Kristallplastizit¨ t, Springer-Verlag, Berlin. aG. I. Taylor, Proc. Roy. Soc., Vol. A116 (1927), pp. 16–38.PROBLEMS 1. If a single crystal of aluminum were stressed in uniaxial tension applied along the [021] direction, which slip system (or systems) would be most highly stressed?
- 154. 136 MECHANICAL BEHAVIOR OF MATERIALS 2. A single crystal of copper is loaded under a stress state such that σ 2 = −σ 1 , σ 3 = τ 23 = τ 31 = τ 12 = 0. Here 1 = [100], 2 = [010], and 3 = [001]. A. When the stress σ 1 = 6 kPa, what is the shear stress, τ , on the i. (111)[101] slip system? ii. (111)[110] slip system? iii. (111)[011] slip system? B. On which of these systems would you expect slip to ﬁrst occur as the applied stresses increased? C. Assuming slip on that system, determine the ratios of the strains, ε2 /ε 1 and ε3 /ε 1 . 3. A single crystal of aluminum was grown in the shape of a tensile bar with the [321] direction aligned with the tensile axis. A. Sketch a standard cubic projection with [100] at the center and [001] at the North Pole and locate the [321] direction on this projection. B. Which of the {111}<110> slip system(s) would be most highly stressed when tension was applied along [321]? Show the slip-plane normal(s) and the slip direction(s) of the system(s) on your plot. C. What will be the ratio of the shear stress on the slip system to the tensile stress applied along [321]? 4. An aluminum single crystal is subjected to a tensile stress of σ x = 250 kPa parallel to x = [100] and a compressive stress of σ y = −50 kPa parallel to y = [010] with σ z = τ yx = τ zx = τ x y = 0. What is the shear stress on the (111) plane in the [110] direction? 5. Consider an aluminum single crystal that has been stretched in tension applied parallel to x = [100] (σ x = +250 kPa) and compressed parallel to y = [010] (σ y = −50 kPa), with σ z = 0, where z = [001]. Assume that slip occurred on the (111) in the [110] direction and only on that slip system. Also assume that the strains are small. A. Calculate the ratios of resulting strain, ε y /ε x and ε z /ε x . B. If the crystal were strained until ε x = 0.0100, what would the angle be between the tensile axis and [100]? 6. NaCl crystals slip on {110}<110> slip systems. There are six systems of this type. Consider a crystal subjected to uniaxial compression parallel to z = [110]. A. On which of the {110}<110> slip systems would the shear stress be the highest? that is, on which of the systems would slip be expected? B. Let the lateral directions be x = [110] and y = [001]. Determine the shape change that occurs as the crystal deforms on one of these systems by ﬁnding the ratios ε y /ε z and ε x /ε z . Describe the shape change in words. [Hint: Analyze one of the slip systems in your answer to (A). Be careful about signs.]
- 155. SLIP 137 7. Predict the R-value for a sheet of an hcp metal with (0001) parallel to the rolling plane and [1010] parallel to the rolling direction. 8. Determine the number of independent slip systems for crystals with each of the following combinations of slip systems. (The simplest way to do this is to de- termine how many of the strains ε 1 , ε 2 , γ 23 , γ 31 , and γ 12 can be independently imposed on the crystal.) A. Cubic crystal that deforms by {100}<011> slip. B. Cubic crystal that deforms by slip on {100}<011> and {100}<001> systems. C. Cubic crystal that deforms by {110}<110> slip. D. Hcp crystal that deforms by slip on (0001)<1120> and {1010}<1120> systems. 9. A tetragonal crystal slips on {011}<111> systems. How many of the strains, ε x , ε y , ε z , γ yz , γ zx , γ x y , can be accommodated? [Note that in a tetragonal crystal the {011} family does not include (110) or (110).] Figure 8.18. A tetragonal crystal with {011}<111> slip systems.10. A. Consider an fcc single crystal extended in uniaxial tension parallel to [321]. Will the Schmid factor m = cos λ cos φ for the most highly stressed slip system increase, decrease, or remain constant as the crystal is extended? B. Consider an hcp single crystal that slips easily only on (0001)<1120> slip systems. If an hcp crystal is extended in uniaxial tension in a direction oriented 45◦ from the c-axis and 45◦ from the most favored <1120> slip direction, will the Schmid factor m = cos λcos φ for the most highly stressed slip system increase, decrease, or remain constant?11. Consider a sheet of an fcc metal that has a {110}<001> texture. That is, a {110} plane is parallel to the plane of the sheet and a <001> direction is parallel to the prior rolling direction. A. Predict the value of Ro (the strain ratio measured in a rolling direction tension test). [Hint: Let x, y, and z be the rolling, transverse, and sheet-normal direc- tions. Assign speciﬁc indices [hkl ] to the rolling, transverse, and sheet-normal
- 156. 138 MECHANICAL BEHAVIOR OF MATERIALS directions. Find the speciﬁc indices of the transverse direction, y. Then sketch a standard cubic projection showing these directions. (It is convenient to choose x, y, and z so that they lie in the hemisphere of the projection.) For uniaxial tension along x, determine which slip systems will be active, and assume an equal shear strain, γ i , on each. For each system, calculate the resulting strains, ε x , ε y , and ε z in terms of γ i and sum these over all slip systems. Assume equal amounts of slip on all the equally favored slip systems. Now predict the strain ratio Ro .] B. Predict R90 .
- 157. 9 Dislocation Geometry and EnergyIntroductionIt was well known in the late 19th century that crystals deformed by slip. In the early20th century the stresses required to cause slip were measured by tension tests of singlecrystals. Dislocations were not considered until after it was realized that the measuredstresses were far lower than those calculated from a simple model of slip. In the mid-1930sG. I. Taylor∗ , M. Polanyi,† and E. Orowan‡ independently postulated that preexistingcrystal defects (dislocations) were responsible for the discrepancy between measured andcalculated strengths. It took another two decades and the development of the electronmicroscope for dislocations to be observed directly. Slip occurs by the motion of dislocations. Many aspects of the plastic behavior ofcrystalline materials can be explained by dislocations. Among these are how crystalscan undergo slip, why visible slip lines appear on the surfaces of deformed crystals, whycrystalline materials become harder after deformation, and how solute elements affectslip.Theoretical strength of crystalsOnce it was established that crystals deformed by slip on speciﬁc crystallographic sys-tems, physicists tried to calculate the strength of crystals. However, the agreement be-tween their calculated strengths and experimental measurements was very poor. Thepredicted strengths were orders of magnitude too high, as indicated in Table 9.1. The basis for the theoretical calculations is illustrated in Figure 9.1. Each plane ofatoms nestles in pockets formed by the plane below (Figure 9.1a). As a shear stress isapplied to a crystal, the atoms above the plane of shear must rise out of the stable pocketsin the plane below and slide over it until they reach the unstable position shown in Figure9.1b. From this point they will spontaneously continue to shear to the right until theyreach a new stable position (Figure 9.1c). ∗ G. I. Taylor, Proc. Roy. Soc. (London), Vol. A145 (1934): pp. 362–87. † M. Polanyi, Z. Phys. Vol. 89 (1934): pp. 660–4. ‡ E. Orowan, Z. Physik, Vol. 89 (1934): pp. 634–59. 139
- 158. 140 MECHANICAL BEHAVIOR OF MATERIALSTable 9.1. Critical shear stress for slip in several materials Critical shear stress (MPa)Metal Purity % Experiment Theorycopper >99.9 1.0 414silver 99.99 0.6 285cadmium 99.996 0.58 207iron 99.9 ∼7.0 740Note: There is considerable scatter caused by experimental variables, particularly purity. 1 2 3 τ τ τ 4 a. b. c.Figure 9.1. Model of slip occurring by sliding of planes 1 and 2 over planes 3 and 4. For the unstable condition(b) the planes are at attracted equally to the stable conﬁgurations in (a) and (c). For simplicity, consider a simple cubic crystal. An applied shear stress, τ , will displaceone plane relative to the next plane as shown in Figure 9.2. When the shear displacement,x, is 0, d, 2d, or nd (i.e., γ = 0, 1, 2, . . ., n), the lattice is restored, so τ should be zero. Theshear stress, τ , is also zero when the displacement is x = (1/2)d, (3/2)d, etc. (γ = 1/2,3/2, . . .). A sinusoidal variation of τ with γ as shown in Figure 9.3 seems reasonable, so τ = τmax sin(2π γ ). (9.1)Here τ max is the theoretical shear stress required for slip. If the stress is less than τ max ,the shear strain is elastic and will disappear when the stress is released. For very lowvalues of γ (Figure 9.4), Hooke’s law should apply: τ = Gγ . (9.2)This can be expressed as (dτ/dγ )γ →0 = G. (9.3)Differentiating Equation (9.1), (dτ /dγ )γ →0 = 2π τ max cos(2π γ )γ →0 = 2π τ max . Substi-tuting into Equation (9.3), τmax = G/2π. (9.4) τ x γ =x/d Figure 9.2. Model used to calculate the the- d oretical shear stress for slip. d
- 159. DISLOCATION GEOMETRY AND ENERGY 141 +Figure 9.3. Theoretical variation of shear τ maxstress with displacement. τ γ 1 − + GFigure 9.4. The shear modulus, G, is theinitial slope of the theoretical τ versus γ τmaxcurve. τ γ 1 −A somewhat more sophisticated analysis for real crystal structures predicts somethingclose to τmax = G/10. (9.5) In Table 9.1, the theoretical strength values predicted by Equation (9.5) are ordersof magnitude higher than experimental measurements. The poor agreement betweenexperimental and theoretical strengths indicated that there was something wrong withthe theory. The problem with the theoretical calculations is that it was assumed thatslip occurs by one entire plane of atoms sliding over another at the same time. Taylor,Orowan, and Polanyi realized that it is not necessary for a whole plane to slip at thesame time. They postulated that crystals have preexisting defects that are boundariesbetween regions that are already displaced relative to one another by a unit of slip. Theseboundaries are called dislocations. Movement of a dislocation allows slip to occur. Thecritical stress for slip is the stress required to move a dislocation. At any instant, slip needonly occur at the dislocation rather than over the entire slip plane.The nature of dislocationsOne special form of dislocation is an edge dislocation, sketched in Figure 9.5. Thegeometry of an edge dislocation can be visualized as having cut partway into a perfectcrystal and then inserted an extra half plane of atoms. The dislocation is the bottom edgeof this extra half plane. The screw dislocation (Figure 9.6) is another special form. It canbe visualized as a spiral-ramp parking structure. One circuit around the axis leads oneplane up or down. Planes are connected in a manner similar to the levels of a spiral-parkingramp. An alternate way of visualizing dislocations is illustrated in Figure 9.7. An edgedislocation is created by shearing the top half of the crystal by one atomic distanceperpendicular to the end of the cut (Figure 9.7b). This produces an extra half plane of
- 160. 142 MECHANICAL BEHAVIOR OF MATERIALS x aFigure 9.5. An edge dislocation is the edge of an Figure 9.6. A screw dislocation. Traveling on the lat-extra half-plane of atoms. From A. G. Guy, Elements tice around the screw dislocation is like following theof Physical Metallurgy, Addison–Wesley, 1951. thread of a screw.atoms, the edge of which is the center of the dislocation. The other extreme form ofdislocation is the screw dislocation. A screw dislocation is generated by cutting into aperfect crystal and then shearing half of it by one atomic distance in a direction parallelto the end of the cut (Figure 9.7c). The end of the cut is the dislocation. In both cases thedislocation is a boundary between regions that have and have not slipped. When an edgedislocation moves, the direction of slip is perpendicular to the dislocation. In contrast,movement of a screw dislocation causes slip in the direction parallel to itself. The edgeand screw are extreme cases. A dislocation may be neither parallel nor perpendicular tothe slip direction.Burgers vectorsDislocations are characterized by Burgers vectors. Consider an atom-to-atom circuit inFigure 9.8 that would close on itself if made in a perfect crystal. If this same circuit isconstructed so that it goes around a dislocation, it will not close. The closure failure isthe Burgers vector, denoted by b. The Burgers vector can be considered a slip vector a. b. c.Figure 9.7. Consider a cut made in a perfect crystal (a). If one half is sheared by one atom distance parallelto the direction of the cut, an edge dislocation results (b). If one half is sheared by one atom distanceperpendicular to the direction of the cut, a screw dislocation results (c).
- 161. DISLOCATION GEOMETRY AND ENERGY 143Figure 9.8. The Burgers vector of a disloca-tion can be determined by drawing a clock-wise circuit that would close if it were drawn bin a perfect crystal. If the circuit is drawnaround a dislocation, the closure failure is theBurgers vector.because its direction is the slip direction and its magnitude is the magnitude of the slipdisplacement caused by its movement of the dislocation. A dislocation may wander through a crystal with its orientation changing from placeto place, but its Burgers vector is the same everywhere. See Figure 9.9. If the dislocationbranches into two dislocations, the sum of the Burgers vectors of the branches equals itsBurgers vector. There is a simple notation system for describing the magnitude and direction of theBurgers vector of a dislocation. The direction is indicated by direction indices and themagnitude by a scalar preceding the direction. For example, b = (a/3)[211] in a cubiccrystal means that the Burgers vector has components of 2a/3, −a/3, and a/3 alongthe [100], [010], and [001] directions, respectively, where a is the lattice parameter. Its √magnitude is |b| = [(2a/3)2 + (−a/3)2 + (a/3)2 ]1/2 = a 6/3). A dislocation in an fcc crystal corresponding to a full slip displacement that re-stores the lattice would have a Burgers vector (a/2)<110>. In this case the magnitude is √a 2/2. Example problem 9.1: Using proper notation, write the Burgers vector for a disloca- tion corresponding to the shortest repeat distance in a bcc crystal. SOLUTION: The shortest repeat distance is half of the body diagonal of the unit cell: b = (a/2)<111>.Figure 9.9. A dislocation may wander through acrystal, but everywhere it has the same Burgers vec-tor. Where it is parallel to its Burgers vector, it is a bscrew (a). Where it is perpendicular to its Burgersvector, it is an edge (b). Elsewhere it has a mixedcharacter. a
- 162. 144 MECHANICAL BEHAVIOR OF MATERIALSEnergy of a screw dislocationThe energy associated with a screw dislocation is the energy required to distort the latticesurrounding the dislocation elastically. The distortion is severe near the dislocation butdecreases with distance from it. Consider an element of length L and thickness dr ata distance r from the center of a screw dislocation (Figure 9.10a). The volume of theelement is 2πrLdr. Imagine unwrapping this element, so that it lies ﬂat (Figure 9.10b).Unwrapping causes no strain because the element is differentially thin. The shear strain associated with this element is γ = b/(2πr ), (9.6)where b is the Burgers vector of the screw dislocation. The energy/volume associatedwith an elastic distortion is Uv = (1/2)τ γ , (9.7)where τ is the shear stress necessary to cause the shear strain γ . According to Hooke’slaw, τ = Gγ , (9.8)where G is the shear modulus. Combining Equations (9.6), (9.7), and (9.8), the en-ergy/volume is Uv = Gγ 2 /2 = (1/2)Gb2 /(2πr )2 . (9.9)The elastic energy, dU, associated with the element is its energy/volume times its volume, dU = [(1/2)Gb2 /(2πr )2 ](2πr Ldr ) = Gb2 L/4π)dr/r. (9.10) b b r dr L dr 2πr a. b.Figure 9.10. (a) Screw dislocation in a cylindrical crystal; (b) ﬂattened element.
- 163. DISLOCATION GEOMETRY AND ENERGY 145The total energy of the dislocation per length, L, is obtained by integrating Equation(9.10): r1 U/L = Gb /(4π) 2 dr/r = Gb2 /(4π) ln(r1 /r0 ). (9.11) r0 Example problem 9.2: Equation (9.9) gives the energy/volume as a function of r. Calculate the distance from the core of a screw dislocation at which the energy per volume equals to the heat of vaporization, Hv , and express this distance in terms of r/b. Evaluate this critical value of r/b for copper, for which ρ = 8.93 Mg/m3 , G = 77 GPa, b = 0.255 nm, and Hv = 4.73 MJ/kg. SOLUTION: Solving Equation (9.9) for r/b, (r/b)2 = G/(8π 2 Uv ) = (77 × 109 Pa)/ (8π 8.93 × 103 kg/m3 × 4.73 × 106 J/kg) = 0.023, so that r/b = 0.15. 2 For copper, r = 0.15 × 0.255 = 0.04 nm. Clearly Equation (9.9) is not valid for values of r < 0.04 nm because it predicts that the material within this radius would vaporize The problem, now, is to decide what are appropriate values for the lower limit, ro ,and the upper limit, r1 , of the integral in Equation (9.11). We might be tempted to let robe 0 and r1 be ∞, but both would cause the value of U in Equation (9.11) to be inﬁnite.First consider the lower limit, ro . Equation (9.6) predicts an inﬁnite strain at r = 0,which corresponds to an inﬁnite energy/volume at the core of the dislocation (ro = 0).This is clearly unreasonable. The energy/volume can’t possibly be higher than the heatof vaporization. This discrepancy is a result of the breakdown of Hooke’s law at the veryhigh strains that exist near the core of the dislocation. The stress, τ , is proportional to γonly for small strains. A lower limit, ro , can be chosen so that the neglected energy ofthe core in the region, 0 < r < ro , is equal to the overestimation of the integral for r > ro .See Figure 9.11. A value of ro = b/4 has been suggested as reasonable. The upper limit, r1 , can’t be any larger that the radius of the crystal. A reasonablevalue for r1 is half of the distance between dislocations. At greater distances, the stress to ∞ dU/dr = (1/r) times a constant dU/dr actual dU/drFigure 9.11. Energy density near the core of a screwdislocation. r 0 ro
- 164. 146 MECHANICAL BEHAVIOR OF MATERIALSﬁeld is probably neutralized by stress ﬁelds of other dislocations. The value of r1 is oftenapproximated by 105 b, which corresponds to a dislocation density of 1010 dislocationsper m2 . This is convenient because ln(105 b/0.25b) = ln(4 × 105 ) = 12.9 ≈ 4π. With thisapproximation, the energy per length, UL , from Equation (9.11) simpliﬁes to UL ≈ Gb2 . (9.12) The process of choosing the limits of integration so that the expression for the en-ergy/length simpliﬁes to Equation (9.12) may seem arbitrary. Yet the results, althoughapproximate, are reasonable. The derivation of the energy of an edge dislocation is morecomplicated because the stress ﬁeld around an edge dislocation is more complex. Foredge dislocations, UL ≈ Gb2 /(1 − υ), (9.13)where υ is Poisson’s ratio. Thus the energy of an edge dislocation is greater than that ofa screw by a factor of 1/(1 − υ) ≈ 1.5. There are two important features of Equations (9.12) and (9.13). One is that theenergy of a dislocation is proportional to its length. Energy per length is equivalent toline tension, or a contractile force. The units of energy/length are J/m, which is the sameas the units of force, N. The second important feature is that the energy of a dislocation is proportional to b2 .This controls the energetics of reactions between parallel dislocations.Reactions between parallel dislocations and Frank’s ruleTwo parallel dislocations may combine and form a third dislocation. If they do, theBurgers vector of the third dislocation will be the vector sum of the Burgers vectorsof the two reacting dislocations. That is, if b1 + b2 → b3 , then b1 + b2 = b3 . Thereaction is energetically favorable if it lowers the energy of the system. Frank’s rule statesthat the reaction is favorable if b1 2 + b2 2 > b3 2 because the energy of a dislocation isproportional to b2 . Similarly, a dislocation, b1 , may spontaneously dissociate into twoparallel dislocations, b2 and b3 , if b1 2 > b2 2 + b3 2 . It is energetically favorable fordislocations with large Burgers vectors to react with one another to form dislocationswith smaller Burgers vectors. As a consequence, dislocations in crystals tend to havesmall Burgers vectors. Example problem 9.3: Consider the reaction of two parallel dislocations of Burgers vectors b1 = (a/2)[110] and b2 = a[011]. What would be the Burgers vector of the product dislocation if they reacted with each other? Would the reaction be energetically favorable? SOLUTION: b3 = b1 + b2 = (a/2)[110] + a[011] = [a/2 + 0, a/2 − a, 0 + a] = (a/2) [112]b1 2 + b2 2 = (a/2)2 (12 + 12 + 02 ) + (a/2)2 [02 + (−1)2 + 12 ] = a 2 . b3 2 = (a/2)2 [12 + (−1)2 + 22 ] = 1.5a 2 · b1 2 + b2 2 < b3 2 , so the reaction would be energetically unfavorable.
- 165. DISLOCATION GEOMETRY AND ENERGY 147 z θ y r x zFigure 9.12. Coordinate system for describing a lo- Figure 9.13. Coordinates around an edge disloca-cation near a screw dislocation. The dislocation is tion.parallel to z and at a distance r = 0.Stress ﬁelds around dislocationsAround a dislocation, the atoms are displaced from their normal positions. These dis-placements are equivalent to the displacements caused by elastic strains arising fromexternal stresses. In fact, the lattice displacements or strains can be completely describedby these stresses and Hooke’s laws can be used to ﬁnd them. It should be noted that the equations given below are based on the assumption ofisotropic elasticity. The coordinate system is shown in Figure 9.12. For a screw dislocationwith a Burgers vector, b, parallel to the z axis, τzθ = −Gb/(2πr ) and τr θ = τr z = σr = σθ = σz = 0, (9.14)where G is the shear modulus and r is the radial distance from the dislocation. The minussign indicates that the repulsive force is inversely proportional to the distance betweenthe dislocations. Equation (9.14) indicates that a screw dislocation creates no hydrostatic tension orcompression because σ H = (σ r + σ θ + σ z )/3 = 0. Therefore, there should be nodilatation (volume strain) associated with a screw dislocation. (However, real crystalsare elastically anisotropic, so there may be a small dilatations associated with screwdislocations.) For an edge dislocation which lies parallel to z and which has its Burgers vectorparallel to x (Figure 9.13), τx y = Dx(x 2 − y 2 )/(x 2 + y 2 )2 , (9.15a) σx = −Dy(3x 2 + y 2 )/(x 2 + y 2 )2 , (9.15b) σ y = Dy(x 2 − y 2 )/(x 2 + y 2 )2 (9.15c) σz = υ(σx + σ y) = −2Dυy/(x 2 + y 2 ), τ yz = τ zx = 0, (9.15d)where D = Gb/[2π(1 − υ)]. One of the important features of these equations is that there is a hydrostatic stress,σ H = (σ x + σ y + σ z )/3, around an edge dislocation. Combining Equations (9.15b),
- 166. 148 MECHANICAL BEHAVIOR OF MATERIALS contours of hydrostatic stress hydrostatic compression hydrostatic tension dFigure 9.14. Contours of hydrostatic stress around Figure 9.15. A low-angle grain boundary formed byan edge dislocation. Note that the level of hydrostatic edge dislocations. The misorientation angle θ = b/d.stress increases near the dislocation.(9.15c), and (9.15d), σH = −(2/3)Dy(1 + υ)/(x 2 + y 2 ) or σH = −A(y)/(x 2 + y 2 ), (9.16)where A = Gb(1 + υ)/[3π(1 − υ)]. Figure 9.14 shows how the hydrostatic stress variesnear an edge dislocation. There is hydrostatic compression (negative σ H ) above the edgedislocation (positive y) and hydrostatic tension below it. The dilatation causes interactions between edge dislocations. Given sufﬁcient mobil-ity, edge dislocations of like signs (same Burgers vectors) tend to form walls with onedislocation directly over another, as shown in Figure 9.15. The hydrostatic tension causedby one dislocation is partially annihilated by the hydrostatic compression of its neighbor.This relatively low energy and therefore stable conﬁguration forms a low-angle grainboundary. In substitutional solutions, solute atoms that are larger than the solvent atoms areattracted to the region just below the edge dislocation, where their larger size helpsrelieve the hydrostatic tension. Similarly, substitutional solute atoms that are smallerthan the solvent atoms are attracted to the region just above the edge. In either case edgedislocation will attract solute atoms (Figure 9.16). In interstitial solid solutions, all soluteatoms are attracted to the region just below the edge dislocation, where they help relievethe tension. It is this attraction of edge dislocations in iron for carbon and nitrogen that isresponsible for the yield point effect and strain-aging phenomenon in low carbon steel.(See Chapter 12.) Figure 9.16. If small substitutional solute atoms mi- grate toward the extra half-plane they help relieve the largesmall solute crowding there. Large substitutional solute atoms willsolute atoms help relieve the tension below.atoms
- 167. DISLOCATION GEOMETRY AND ENERGY 149Figure 9.17. The force per length on a dislocation, fL= −τ · b.Forces on dislocationsA stress in crystals causes a force on dislocations. Consider a dislocation of length L andBurgers vector b on a plane, as shown in Figure 9.17. A shear stress τ acting on thatplane will cause a force on the dislocation per unit length fL of f L = −τ · b. (9.17)Note that a dot product is possible here because once the plane of the stress is ﬁxed, thestress can be treated as a vector (force). The stress, τ , may result from the stress ﬁeld ofanother dislocation. Thus two screw dislocations exert an attractive force on each otherof f L = −Gb1 · b2 /(2πr ), (9.18)where b is the Burgers vector of the dislocation of concern. The minus sign means thatthey repel one another if the dot product is positive. An equivalent statement is that twodislocations repel each other if Frank’s rule predicts that their combination would resultin an energy increase. If the angle between b1 and b2 is greater than 90◦ , |b1 + b2 | >|b1 | + |b2 |. The interaction of two parallel edge dislocations is somewhat more complex. Theshear stress ﬁeld for one edge dislocation that lies parallel to z with a Burgers vectorparallel to x is given by Equation (9.15a), τ x y = Dx(x2 − y2 )/(x2 + y2 )2 , where D =Gb/[2π (1 − υ)]. The mutual force on that plane is f L = −{Gb1 · b2 /[2π(1 − υ)]}x(x 2 − y 2 )/(x 2 + y 2 )2 . (9.19)For dislocations with like sign (b1 · b2 > 0) there is mutual repulsion in the region x > yand attraction in the region x < y. This is equivalent to saying that there is mutualrepulsion if Frank’s rule predicts that a reaction would cause an increase of energy andmutual attraction if it would cause a decrease of energy. Figure 9.18 shows the regionsof attraction and repulsion. The stress, τ x y , is zero at x = 0, x = y, and x = ∞. Between x = 0 and x = y, τ x y is negative, indicating that the stress ﬁeld wouldcause attraction of edge dislocations of the same sign to each other. Therefore edgedislocations of the same sign tend to line up one above the other as shown in Figure 9.15.For x greater than y, the stress, τ x y , is positive, indicating that the stress ﬁeld would tendto repel another edge dislocation of the same sign.
- 168. 150 MECHANICAL BEHAVIOR OF MATERIALS y attraction attraction y>0>x, y>|x| y>x>0 repulsion repulsion y>0>x, |x|>y x>y>0 Figure 9.18. Stresses around an edge dislocation ei- ther attract or repel another parallel dislocation hav- ing the same Burgers vector, depending on how the x two are positioned relative to one another. 0>y>x x>0>y, x>|y| repulsion repulsion 0>x>y x>0>y, |y|>x attraction attractionPartial dislocations in fcc crystalsIn fcc crystals, slip occurs on {111} planes and in <110> directions (Figure 9.19).Consider the speciﬁc case of (111)[110] slip. The Burgers vector corresponding to dis-placements of one atom diameter is (a/2)[110]. A dislocation with this Burgers vectorcan dissociate into two partial dislocations, (a/2)[110]g → (a/6)[211] + (a/6)[12 1]. (9.20)We can check that this reaction is vectorially correct by noting that b1 = (−a/2, a/2, 0)does equal b2 = (−a/3, a/6, a/6) + b3 = (−a/6, a/3, −a/6). Figure 9.20 is a geometricalrepresentation of these two partials. Example problem 9.4: When an (a/2)[110] dissociates into two partial dislocations, (a/6)[211] and (a/6)[12 1], on what {111} plane must the partial dislocations lie? SOLUTION: The normal to the plane must be at 90◦ to both Burgers vectors, so it can be found by taking their cross product, [211] × [12 1] = −3,−3,−3 or (111). An alternative way is to try all of the {111} possibilities and see which has a zero dot product with both [211] and [12 1]. [001] (111) [110] [010][100]Figure 9.19. Slip systems in an fcc cr ystal.
- 169. DISLOCATION GEOMETRY AND ENERGY 151Figure 9.20. Burgers vectors for partial slip disloca-tions in an fcc cr ystal. -- -- -- (a/6)[121] (a/6)[211] -- (a/2)[110] Example problem 9.5: Into what other pair of (a/6)<211> partials could the (a/2)[110] dislocation in Example Problem 9.4 dissociate? On what plane would they lie? SOLUTION: By inspection, (a/2)[110] → (a/6)[21 1] + (a/6)[121]. The (a/6)[21 1] and (a/6)[121] partials must lie in a (111). Note that [21 1] · [111] = 0 and [121]· [111] = 0.Stacking faultsIf a single (a/6)<112> partial dislocation passes through an fcc crystal, it leaves behinda region in which the sequence of stacking of the close-packed {111} planes does notcorrespond to the normal fcc lattice. The correct stacking order is not restored until thesecond partial dislocation passes. The normal stacking order in fcc and hcp lattices isshown in Figure 9.21. In hcp crystals, the third close-packed plane, A, lies directly overthe ﬁrst, A. In fcc crystals, the third close-packed plan, C, is over neither the ﬁrst (A) A A A A A A A A A B C B B B B C B B A A A A A A B C C B B B A A A C A A A A A A A A B HCP FCC Plan view of close-packed planesFigure 9.21. (a) The normal stacking of {111} planes in an fcc cr ystal can be described as ABCABC. (b)When an (a/6)<112> partial passes through the crystal, the stacking sequence is changed to ABABC.
- 170. 152 MECHANICAL BEHAVIOR OF MATERIALSFigure 9.22. Stacking of close-packed planes in fcc and hcp crystals. When an (a/6)<112> partial dislocationmoves plane C so that it is directly over plane A, it creates a region where the packing sequence is hcp ratherthan fcc.nor the second (B){111} plane. Figure 9.22 shows that an (a/6)<112> partial dislocationchanges the position of the third plane so that it is directly over the ﬁrst and thereforeproduces a local region of hcp packing. In Figure 9.23, the stacking order near a stacking fault in an fcc crystal is com-pared with the stacking in fcc and hcp lattices and near a twin boundary in an fcccrystal. The stacking sequence near a stacking fault in an fcc crystal is similar to the packingsequence in the hcp lattice. Since this is not the equilibrium structure of fcc, the stackingfault raises the energy and the increase of energy depends directly on the area of thefault. The stacking fault energy, γ SF , is the energy per area of fault and can be regardedas a surface tension pulling the partial dislocations together. A stacking fault has twiceas many incorrect second-nearest neighbors as a twin boundary. The similarity of thepacking sequences at a twin boundary and at a stacking fault is clear in Figure 9.23. Formost metals, the stacking fault energy is about twice the twin boundary energy, as shownin Figure 9.24. The frequency of annealing twins is much higher in fcc metals (Ag, brass,Al-bronze, γ -stainless) of low stacking fault energy (SFE) than in those with higher SFE(Cu, Au). Annealing twins in the microstructures of aluminum alloys are rare. Table 9.2lists the values of the stacking fault energy for a few fcc metals. The values of γ SF forbrass (Cu–Zn), aluminum bronze (Cu–Al), and austenitic stainless steel are still lowerthan the value for Ag. The stacking fault between two (a/6)<112> partial dislocations is illustrated in Figure9.25. The mutual repulsion of two partials tends to drive them away from each other.However, balancing this mutual repulsion is the attraction that results from the surfacetension of the stacking fault between them (Figure 9.26).Table 9.2. Stacking fault energies of several fcc metalsAg Al Au Cu Ni Pd Pt Rh Ir16 166 32 45 125 180 322 750 300 mJ/m2 .Source From listing in J. P. Hirth and J. Lothe, Theory of Dislocations,Wiley, (1982).
- 171. DISLOCATION GEOMETRY AND ENERGY 153 fcc with a fcc with a hcp fcc stacking fault twin A A= A C A B C B B C C B A A B A A A B= B C A B C C A B C C SF twin B B B A A A boundary A C= A C C C A A B B B B A A A A regions of local hcp stackingFigure 9.23. Stacking of close-packed planes. 200 Twin boundary energy, (mJ/m2) Pt 100 Al Ni Cu Au Ag 0 0 100 200 300 400 Stacking fault energy, mJ/m2Figure 9.24. The relationship of stacking fault energy and twin boundary energy. The line representsγ stacking fault = 2γ twin . partial partial dislocation dislocation stacking faultFigure 9.25. Two partial dislocationsseparated by a stacking fault.
- 172. 154 MECHANICAL BEHAVIOR OF MATERIALS mutual repulsion from stress fields Figure 9.26. The equilibrium spacing be- tween two partial dislocations corre- sponds to the separation at which the mu- tual repulsion and attraction balance. attraction caused by stacking faultNOTESPostulation of dislocations: Calculations of the strength of crystals by J. Frenkel, Z. Phys., Vol. 37,(1926): p. 572, showed the great discrepancy between theory and experimental observation. It wasnot until 1934 that, G. I. Taylor, E. Orowan, and M. Polanyi more or less independently proposededge dislocations to explain the difference between σ theor and σ exper . Screw dislocations werepostulated later by J. M. Burgers, Proc. Kon. Ned. Akad. Wetenschap., Vol. 42 (1939): p. 378.Orowan’s interest in why crystals are as weak as they are was stimulated by an accident duringresearch for his bachelor’s degree at the Technische Universitat Berlin. He dropped his only zinc ¨single crystal on the ﬂoor. Rather than quit, he straightened the crystal and then tested it in creep.He later commented that reﬂection on the nature of the results contributed to his postulation ofdislocations.Discovery of the strength of whiskers: During an investigation of the failure of some electricalcapacitors at the Bell Telephone Laboratories, whiskers of tin about 2 × 10–6 m diameter werefound growing from the condenser walls. What distinguished this investigation from earlier ﬁndingsof metal whiskers is that these whiskers were tested in bending (C. Herring and J. K. Galt, Phys.Rev., Vol. 85, (1952): 1060). The surprising ﬁnding was that these whiskers could be bent to astrain of 2 to 3% without plastic deformation. This meant that the yield strength was 2 to 3% of theYoung’s modulus. For tin, E = 16.8 × 106 psi, so Y > 330,000 psi. Thus, overnight, tin became thestrongest material known to humanity. Once the Herring–Galt observation was reported, manyothers began testing whiskers of other metals such as copper and iron with similar results andtin lost this distinction.REFERENCESA. H. Cottrell, Dislocations and Plastic Flow in Crystals, Oxford, 1953.J. P. Hirth and J. Loethe, Theory of Dislocations, Wiley, 1982.D. Hull and D. J. Bacon, Introduction to Dislocations, third ed., Butterworth Heinemann, 1997.W. T. Read, Dislocations in Crystals, McGraw–Hill, 1953.J. Weertman and J. R. Weertman, Elementary Dislocation Theory, Oxford, 1992. * Hirth and Loethe give a more exact relation for the force between two parallel dislocations, f L = [G/(2πr )][(b1 · ξ )(b2 · ξ ) + (b1 × ξ ) · (b2 × ξ )/(1 − υ)], (9.22) where ξ is a unit vector parallel to the two dislocations. The two terms inside the brackets are the ef- fects of the screw and edge components of the dislocations. Thus the equilibrium separation of two partial dislocations depends inversely on the stacking fault energy, which varies from one fcc metal to another.
- 173. DISLOCATION GEOMETRY AND ENERGY 155PROBLEMS 1. A crystal of aluminum contains 1012 m of dislocation per m3 . A. Calculate the total amount of energy per m3 associated with dislocations. Assume that half of the dislocations are edges and half are screws. B. What would be the temperature rise if all of this energy could be released as heat? Data for aluminum: atomic diameter = 0.286 nm, crystal structure = fcc, density = 2.70 Mg/m3 , atomic mass = 27 g/mole, C = 0.215 cal/g◦ C, G = 70 GPa, υ = 0.3. 2. Calculate the average spacing between dislocations in a 1/2◦ tilt boundary in aluminum. See Figure 9.15 and look up any required data. 3. On which {110} planes of bcc iron can a dislocation with a Burgers vector (a/2)[111] move? 4. A single crystal of aluminum was stretched in tension. Early in the test the speci- men was removed from the testing machine and examined at high magniﬁcation (Figure 9.27). The distance between slip lines was found to be 100 µm and the average offset at each slip line was approximately 500 nm. Assume for simplicity that both the slip direction and the slip plane normal are oriented at 45◦ to the tensile axis. A. How many dislocations, on the average, must have emerged from the crystal at each observable slip line? B. Find the shear strain on the slip system, calculated over the whole crystal. C. Find the tensile strain (measured along the tensile axis) that must have occurred (i.e., what was the % elongation when the test was stopped?). tensile axis slip- plane normal 45° slip direction 45° Figure 9.27. Proﬁle of a crystal surface showing offsets caused by slip. average offset 500 nm average distance between active slip planes = 100 µm
- 174. 156 MECHANICAL BEHAVIOR OF MATERIALS 5. Consider the following reactions between parallel dislocations. In each case write the Burgers vector of the product dislocation and determine whether the reaction is energetically favorable: A. (a/2)[110] + (a/2)[110] → B. (a/2)[101] + (a/2)[011] → C. (a/2)[110] + (a/2)[101] → 6. Consider the dislocation dissociation reaction (a/2)[110] → (a/6)[211] + (a/6)[121] in an fcc crystal. Assume that the energy/length of a dislocation is given by EL = Gb2 and neglect any dependence of the energy on the edge versus screw nature of the dislocation. Assume that this reaction occurs and the partial dislocations move very far apart. Neglect the energy associated with the stacking fault between the partial dislocations. A. Express the total decrease in energy/length of the original (a/2)[110] disloca- tion in terms of a and G. B. On which {111} must these dislocations lie? 7. A dislocation in an fcc crystal with a Burgers vector b = (a/2)[011], dissociates on the (111) plane into two partial dislocations of the (a/6)<211> type. A. Give the speciﬁc indices of the two (a/6)<211> partial dislocations. B. Onto what other plane of the {111} family could the b = (a/2)[011] dislocation have dissociated? C. Give the speciﬁc indices of the two (a/6)<211> partials that would be formed if the (a/2)[011] dislocation dissociated on the plane in B. 8. Consider a circular dislocation loop of diameter d in a crystal under a shear stress τ . The region inside the circle has slipped relative to the material outside the circle. The presence of this dislocation increases the energy of the crystal by the dislocation energy/length times the length of the dislocation. The slip that occurs because of the formation of the dislocation under the stress τ lowers the energy of the system by τ Ab. (τ A is the shear force and b is the distance the force works through.) If the diameter of the loop is small, the energy will be reduced if the loop shrinks. If the loop is large enough the loop will spontaneously expand. Find the diameter of critical size loop in terms of b, G, and τ . For simplicity take EL = Gb2 . 9. Referring to Figure 9.23, ﬁnd the ratio of the wrong second nearest neighbors across a stacking fault to the number across a twin boundary. If the surface ener- gies are proportional to the number of wrong second nearest neighbors, what is γ SF /γ TB ?10. Using the values of γ SF from Table 9.2 and Equation (21), make an approximate calculation of the equilibrium separation, r, of two partial dislocations resulting
- 175. DISLOCATION GEOMETRY AND ENERGY 157 from dissociation of screw dislocation in aluminum and in silver. Express the separation in terms of atom diameters. The shear modulus of aluminum is 70 GPa and that of silver is 75 GPa. The atom diameters of Al and Ag are 0.286 and 0.289 nm.11. Plot the variation of the force fL with x on an edge dislocation caused by another edge dislocation at a ﬁxed level of y according to Equation (9.19). Let the units of fL be arbitrary.
- 176. 10 Dislocation MechanicsIntroductionOnce the concept of dislocations was accepted, there were three important questions tobe answered.1. When a single crystal is deformed, slip occurs with shear offsets of thousands of atom distances on relatively widely spaced planes, rather than uniformly throughout the crystal. See Figure 10.1. Why doesn’t slip occur uniformly at an atomic scale?2. Cold working increases the dislocation content of crystals even though dislocations must run out of the crystals. See Figures 10.2 and 10.3. Where do the additional dislocations come from?3. The yield stress increases as the number of dislocations increases even though without any dislocations, the strength would be even higher. See Figure 10.4. Why does the yield stress increase with dislocation density?Frank–Read sourcesThe ﬁrst two of these questions can be answered in terms of the Frank–Read source,which generates dislocations. Suppose that there is a dislocation of ﬁnite length, AB, ina slip plane (Figure 10.5). The dislocation leaves the plane at A and B, but the end pointsare pinned at A and B. A shear stress, τ , acting on the plane will create a force that causesthe dislocation to bow. This bowing is resisted by the line tension of the dislocation. Asthe shear stress is increased the dislocation will bow out until it spirals back on itself.The sections that touch annihilate each other, leaving a dislocation loop that can expandunder the stress and a restored dislocation segment between the pinning points. Theprocess can repeat itself, producing many loops. Frank–Read sources explains how thenumber of dislocations increases with deformation. Their existence on some planes andnot others explains why slip occurs with large offsets (corresponding to the passing ofmany dislocations) on widely spaced planes. A quantitative treatment of the operation of a Frank–Read source can be made by con-sidering a balance of forces acting on the bowed segment of the dislocation (Figure 10.6.)The applied shear stress, τ , causes a force, τ · bd, where d is the distance between the158
- 177. DISLOCATION MECHANICS 159 slip band 100 atom diameters 1000 atom diameters slip lineFigure 10.1. Sketch showing slip on widely spaced planes. The offsets of slip are thousands of atomdiameters. 1 µm 1 mmFigure 10.2. Dislocation structure (a) in annealed aluminum (B. Nost, Phil. Mag., Vol. 11 (1965), p. 183) and(b) in aluminum after 10% reduction of area at 77 K (P. R. Swann in Thomas and Washburn (Eds.), ElectronMicroscopy and Strength of Crystals, Interscience, 1963). Note the very great difference in magniﬁcation. Thedislocation density in (a) is about 102 /cm2 , while in (b) it is on the order of 1010 .Figure 10.3. Increase of dislocation density with strain in iron. Data from A. Keh and Weissmann, in G. Thomasand J. Washburn (Eds.), Electron Microscopy and Strengths of Crystals, Wiley, 1963.
- 178. 160 MECHANICAL BEHAVIOR OF MATERIALS 1000Resolved shear stress. MPa 100 Figure 10.4. Dependence of the critical shear stress for slip in copper as a function of dis- location density. Data are for copper and in- 10 clude experiments on polycrystals as well as single crystals oriented for single and multiple slip. Data from H. Weidersich, J. Inst. Metals, 1 Vol.16 (1964). 0.1 1010 1011 1012 1013 1014 1015 Dislocation density, ρ (m-2) A B τ d b. d A B e. A d B c. a. A B A B d d d. f.Figure 10.5. Sketch illustrating the operation of a Frank–Read source (adapted from T. H. Courtney, Mechan-ical Behavior of Materials, second ed., McGraw–Hill, 2000). A segment of a dislocation of length d is pinnedat points A and B (a). The segment bows out under a shear stress, τ (b). The shear stress reaches a max-imum when the segment becomes a semicircle (c). As the dislocation segment continues to expand underdecreasing stress (d), it eventually recombines with itself (e), forming a dislocation loop. The loop continuesto expand and a new dislocation segment, AB, is formed. The process can repeat itself, sending out manyloops. d Figure 10.6. Force balance on a pinned dislocation that is bowed by a shear stress, τ . θ θ Gb2 Gb 2sinθ τbd Gb2sinθ Gb2
- 179. DISLOCATION MECHANICS 161pinned ends. The line tension of the dislocation (energy/length), UL ≈ Gb2 (Equation(9.12)), acts parallel to the dislocation line and tends to keep it from moving. Consid-ering both ends, the vertical component of this force is 2Gb2 sinθ. This force reaches amaximum, 2Gb2 , when the dislocation is bowed into a semicircle (θ = 90◦ ). Equatingthese two forces and assuming the shear stress is parallel to b, τ bd = 2Gb2 or τ = 2Gb/d. (10.1)Thus the stress necessary to operate a Frank–Read source is inversely proportional to thesize of the source, d. Example problem 10.1: Slip was found to ﬁrst occur in some aluminum crystals when the resolved shear stress reached 1.0 MPa. Assuming that this is the stress necessary to operate the largest Frank–Read sources, calculate the size, d, of these sources. SOLUTION: Substituting τ = 106 Pa, G = 25 × 109 Pa, and b = 0.286 × 10−9 m into Equation (10.1), d ≈ 2bG/τ ≈ 14 µm.Dislocation pile-upsWhen dislocations from a Frank–Read source come to an obstacle such as a grain bound-ary or hard particle, they tend to form a pile-up (Figure 10.7). Because they are of likesign they repel one another. The total repulsion of a dislocation by a pile-up is the sumof the repulsions of each dislocation in the pile-up. With n dislocations in the pile-up,the stress on the leading dislocation, τ n , will be τn = nτ. (10.2)It takes a relatively small number in a pile-up to effectively stop further dislocationmovement. A pile-up creates a back stress on the source so that the stress to continue tooperate the source must rise. This higher stress allows other sources of slightly smallerspacing, d, to operate.Cross-slipA dislocation cannot move on a plane unless the plane contains both the dislocation andits Burgers vector. This requirement uniquely determines the slip plane, except in thecase of screw dislocations. Screw dislocations are parallel to their Burgers vectors, so barrierFigure 10.7. Pile-up of dislocations at an obstacle.
- 180. 162 MECHANICAL BEHAVIOR OF MATERIALS (111) Figure 10.8. A screw dislocation on one (111) slip plane can move onto another plane containing the Burgers vector. This is (111) called cross-slip. [101] successive positions of dislocationthey can slip on any plane in which they lie. When a screw dislocation gliding on oneplane changes to another, it is said to undergo cross-slip. In principle, screw dislocationsshould be able to cross-slip with ease to avoid obstacles (Figure 10.8). If, however, a screw dislocations is separated into partials connected by a stackingfault, both partials cannot be screws. They must recombine to form a screw dislocationbefore they can dissociate on a second plane (Figure 10.9). Such recombination increases the total energy and this energy must be suppliedby the applied stresses, aided by thermal activation. How much energy is required de-pends on the degree of separation of the partials and therefore on the stacking faultenergy. If the stacking fault energy is high, the separation of partial dislocations is small,so the force required to cause recombination is low. In metals of high stacking faultenergy (e.g., aluminum) cross-slip occurs frequently. In crystals of low stacking faultenergy (e.g., brass) the separation of partials is large. A high force is required to bringthem together, so cross-slip is rare. This is in accord with observation of slip traces onpolished surfaces. Slip traces are very wavy in aluminum and very straight in brass(Figure 10.10). Double cross-slip has been proposed as a variant of the original Frank–Read source.In this case, a segment of dislocation, which has undergone double cross-slip, can act asa Frank–Read source on its new plane, as shown in Figure 10.11. (111) (111) (111) (111) Figure 10.9. Cross-slip of a dissociated a b screw dislocation(a). It must ﬁrst recom- bine (b) and then dissociate onto the cross-slip plane (c) before it ﬁnally can glide on the cross plane (d). (111) (111) (111) c d
- 181. DISLOCATION MECHANICS 163 As polished and deformed 250× As polished and deformed 250×Figure 10.10. Straight parallel slip lines in an alloy of low stacking fault energy (left). Wavy slip lines in aluminumresulting from frequent cross-slip (right). G. Y. Chin, Metals Handbook, Vol. 8, eighth ed.Dislocation intersectionsThe number of dislocations increases as deformation proceeds and the increased numbermakes their movement becomes more difﬁcult. This increased difﬁculty of movement iscaused by intersection of dislocations moving on different planes. During easy glide therate of work-hardening is low because slip occurs on parallel planes and there are fewintersections. As soon as slip occurs on more than one set of slip planes, dislocationson different planes will intersect and these intersections impede further motion, causingrapid work-hardening. The nature of dislocation intersections can be understood by considering severaltypes of intersections in simple cubic crystals, as illustrated in Figure 10.12. When twodislocations intersect, a jog is created in each dislocation. The direction of the jog isparallel to the Burgers vector of the intersecting dislocation and the length of the jogequals the magnitude of the Burgers vector of the intersecting dislocation. For dislocations a and b in Figure 10.12, the jogs create no problem. If the upper partof dislocation a and the right side of dislocation b move slightly faster, the jogs will disap-pear. The same is true for dislocation c if its left side moves faster. The jog in dislocationd simply represents a ledge in the extra half plane, and it can move with the rest of theFigure 10.11. Double cross-slip. The segment of dis-location on the top plane can act as a Frank–Readsource on that plane.
- 182. 164 MECHANICAL BEHAVIOR OF MATERIALS before intersection: d a f b c e after intersection: a d f c b eFigure 10.12. Intersection of dislocations. The arrows indicate the direction of motion.dislocation. However, the jogs in dislocations e and f cannot move conservatively. The jogshave an edge character and the direction of motion is not in their slip plane. Figure 10.13is an enlarged view of dislocations e and f in Figure 10.12. Figure 10.14a shows that con-tinued motion of these jogged dislocations would force atoms into interstitial positions.Figure 10.14b shows that with jogs of the opposite sense, vacancies would be produced.If the intersection had been in the opposite direction, movement of the jogs would createa row of vacancies. Figure 10.15 shows rows of vacancies being created by movingjogs. Example problem 10.2: Consider the energy expended when a dislocation with vacancy-producing jogs moves through a crystal. Assume that the distance between jogs is d, and the energy to produce a vacancy is UV . Find the drag force per length, fL , caused by the jogs. SOLUTION: Every time a segment of dislocation of length d moves a distance b, a jog must be produced. Making an energy balance, the work done by the dislocation, fL bd, must equal EV , so fL = UV /(bd). f e Figure 10.13. Jogs produced in disloca-before intersection tions e and f by their intersection. The ar- f rows indicate the shear caused by con- after intersection tinued movement of the dislocations. The e jogs are such that they must create inter- stitial defects as they move.
- 183. DISLOCATION MECHANICS 165 a f eFigure 10.14. (a) Continued motion of joggeddislocations e and f will create interstitial atoms.This is like trying to slide two blocks with ledgesover one another. It requires that the same vol-ume be occupied twice. (b) With jogs of the op-posite sign, motion of the dislocations create bvacancies. This is like opening holes by slidingblocks with ledges over one another. e A high energy is required to produce a row of interstitials. Therefore an interstitial-producing jog will likely be pinned rather than able to produce a row of interstitials.This causes a drag on any motion of the dislocation. Intersections causing interstitial-producing jogs are geometrically much more likely than intersections causing vacancy-producing jogs. The reason for this can be understood in terms of the slip systems likelyto be simultaneously activated. Figure 10.16 illustrates this for a crystal with two slipsystems oriented at 45◦ to the axis of tension or compression. Intersection of these slipsystems will create only interstitial-producing jogs. In real crystals it is possible to ﬁndstress states that can activate slip systems to create vacancy-producing jogs, but they arefewer than those that create interstitials. Direction of movement B A Burgers vector (a) Slip planeFigure 10.15. Rows of vacancies produced bymovement of jogged screw dislocations. From D.Hull, Introduction to Dislocations, Pergamon, 1965. (b) Rc Vacancies (c)
- 184. 166 MECHANICAL BEHAVIOR OF MATERIALSFigure 10.16. Schematic showing why interstitial-producing jogs are more likely than vacancy-producingjogs. With multiple intersections the number of pinning points increases and the stress tocontinue moving the dislocation increases. These intersections act as anchors, greatlydecreasing the mobility of the dislocations. As the number of dislocations increases, thefrequency of intersections also increases, making further slip more difﬁcult.ClimbThe movement of an edge dislocation out of its glide plane can occur only if there isa net diffusional ﬂux of atoms away from or toward the dislocation. Such motion iscalled climb. Removal of atoms from a dislocation causes upward climb and addition ofatoms to the dislocation causes downward climb (Figure 10.17). Because climb requiresdiffusion, it is important only at elevated temperatures during creep. Diffusion-controlledclimb allows dislocations to avoid obstacles that impede their glide and may become acontrolling mechanism during creep (Chapter 16).NotesThe Frank–Read source was postulated to explain why the number of dislocations in a crys-tal increased during deformation (rather than decreasing as dislocations leave the crystal). F. C.Frank of the University of Bristol and W. T. Read of the Bell Telephone Laboratories each con-ceived the idea independently as they traveled to the Symposium on Plastic Deformation ofCrystalline Solids at the Carnegie Institute of Technology in Pittsburgh. Each became aware ofthe other’s ideas during informal discussions before the formal conference. In a Pittsburgh pub Figure 10.17. Climb of an edge dislocation by diffu- sion of vacancies.
- 185. DISLOCATION MECHANICS 167they worked out the theory together and decided to make a joint presentation (F. C. Frank andW. T. Read, Symposium on Plastic Deformation of Crystalline Solids, Carnegie Inst. Technol.1950, Vol. 44, and F. C. Frank and W. T. Read, Phys. Rev., Vol. 79 (1950, p. 722.).REFERENCESA. H. Cottrell, Dislocations and Plastic Flow in Crystals, Oxford, 1953.J. P. Hirth and J. Lothe, Theory of Dislocations, second ed., Wiley, 1982.D. Hull and D. J. Bacon, Introduction to Dislocations, third ed., Butterworth Heinemann, 1997.F. McClintock and A. Argon, Mechanical Behavior of Materials, Addison–Wesley, 1966.W. T. Read, Dislocations in Crystals, McGraw–Hill, 1953.J. Weertman and J. R. Weertman, Elementary Dislocation Theory, Oxford, 1992.PROBLEMS1. Typical values for the dislocation density in annealed and heavily deformed copper are 107 and 1011 cm−2 . (For copper: lattice parameter a = 0.361 nm, E = 110 GPa, υ = 0.30, ρ = 8.96 Mg/m3 .) A. Calculate the average distance between dislocations for both cases. For sim- plicity, assume all of the dislocations are parallel and in a square pattern. B. Calculate with Equation (9.11) the energy/length of dislocation line for both cases assuming the dislocations are screws.2. For a typical annealed metal, the yield stress in shear is 10−4 G. Deduce the typical spacing of a Frank–Read source using a typical value for b.3. Several theoretical models predict that the dislocation density, ρ, should increase parabolically with strain, ρ = Cε1/2 . Assuming this and the dependence of τ on ρ shown in Figure 10.4, predict the exponent n in the power law approximation of the true stress–true strain curve, σ = Kε n .4. Orowan showed that the shear strain rate is given by γ = dγ /dt = ρbv, where ˙ ρ is the dislocation density and v is the average velocity of the dislocation. In a tension test, the tensile strain rate, ε, is half of the shear strain rate, γ (˙ = (1/2)γ . ˙ ˙ ε ˙ if the Schmid factor = 1/2; otherwise ε < (1/2)γ . In a typical tension test, the ˙ ˙ crosshead rate is 0.2 in./min and the gauge section is 2 in. in length. Estimate v in a typical tension test for a typical metal with an initial dislocation density of 1010 /cm2 .5. Consider the possible intersections of dislocations sketched in Fig. 10.18. In the sketches, dislocations B and D are moving to the right and A and C are moving to the left. A. Sketch the nature of the jogs or kinks in each dislocation after they intersect one another. B. Which, if any, would leave a trail of vacancies or interstitials?
- 186. 168 MECHANICAL BEHAVIOR OF MATERIALS B D Figure 10.18. Sketch for Prob- A lem 5. C6. The sketches in Figure 10.19 show pairs of dislocations that are about to intersect. The arrows show the directions of motion (Dislocations A, C, and E are moving into the paper, dislocations B and F are moving out of the paper, and dislocation D is moving to the left.) A. Which of these dislocations (A, B, C, D, E, or F), after intersection, would have jogs that would produce point defects if the dislocations continued to move in the direction shown? B. Indicate for each whether the point defects would be vacancies or interstitials.7. Consider how dislocation intersections affect the stress necessary to continue slip. Let the density of screw dislocations be ρ (meters of dislocations/m3 ) and for simplicity assume that these dislocations are equally divided into three sets of dislocations, each set being parallel to one of the three orthogonal axes. A. Assume each set of dislocations is arranged in a square pattern. Express the distance between the dislocations in a set in terms of ρ. B. Now, consider the jogs formed as a screw dislocation moves. What will be the distance between jogs? C. Assume the energy of forming a row of interstitials is so high that the jogs essentially pin the dislocation. Express the shear stress necessary to continue the motion in terms of G, b, and ρ. √ D. Now assume that the dislocation density is proportional to ε. What would this model predict as the value of n in σ = Kεn ?8. A. Derive an equation for estimating the shear stress, τ , necessary to move a dislocation with vacancy-producing jogs in terms of the Burgers vector, b, the distance between jogs, d, and the energy to create a vacancy, EV . Note that f a d b c e Figure 10.19. Sketch for Problem 6.
- 187. DISLOCATION MECHANICS 169 there must be a vacancy produced each time a segment of dislocation of length d advances a distance b. The work done by the shear stress would be bdfL, where the force per length of dislocation is fL = τ b. B. Evaluate τ for d = 1 µm, EV = 0.7 eV, and b = 0.3 nm.9. Assume that a resolved shear stress of 1.4 MPa is applied to a crystal and causes dislocations to pile up at a precipitate particle. Assume that the shear strength of the particle is 7.2 MPa. What is the largest number of dislocations that can pile up at the precipitate before it yields?
- 188. 11 Mechanical Twinning and Martensitic ShearIntroductionMost crystals can deform by twinning. Twinning is particularly important in hcp metalsbecause hcp metals do not have enough easily activated slip systems to produce anarbitrary shape change. Mechanical twinning, like slip, occurs by shear. A twin is a region of a crystal inwhich the orientation of the lattice is a mirror image of that in the rest of the crystal.Normally the boundary between the twin and the matrix lies in or near to the mirrorplane. Twins may form during recrystallization (annealing twins), but the concern hereis formation of twins by uniform shearing (mechanical twinning), as illustrated in Fig-ure 11.1. In this ﬁgure, plane 1 undergoes shear displacement relative to plane 0 (themirror plane). Then plane 2 undergoes the same shear relative to plane 1, and plane 3relative to plane 2, etc. The net effect of the shear between each successive pair of planesis to reproduce the lattice, but with the new (mirror image) orientation. Both slip and twinning are deformation mechanisms that involve shear displacementson speciﬁc crystallographic planes and in speciﬁc crystallographic directions. However,there are important differences.1. With slip, the magnitude of the shear displacement on a plane is variable, but it is always an integral number of interatomic repeat distances nb, where b is the Burgers vector. Slip occurs on only a few of the parallel planes separated by relatively large distances. With twinning, on the other hand, the shear displacement is a fraction of an interatomic repeat distance and every atomic plane shears relative to its neighboring plane.2. The twinning shear is always directional in the sense that shear in one direction is not equivalent to shear in the opposite direction. Twinning in fcc crystals occurs by shear on the (111) plane in the [112] direction but not by shear in the [112] direction. In fcc metals slip can occur on a (111) plane in either the [110] or the [110] direct- ion.3. With slip the lattice rotation is gradual. Twinning reorients the lattice abruptly.170
- 189. MECHANICAL TWINNING AND MARTENSITIC SHEAR 171 20 1 2 3 0(a) (c) 3 1 0 0(b) (d)Figure 11.1. Formation of twins by shearing between parallel planes of atoms. From W. F. Hosford, TheMechanics of Crystals and Textured Polycrystals. Used by permission of Oxford Univ. Press.Formal notationThere is a formal notation system that describes twinning. Figure 11.2 illustrates a sphereof material, the top half of which has undergone a twinning shear. There are two ma-terial planes that remain undistorted. The ﬁrst undistorted plane, K1 , is the twinningplane (i.e., the mirror plane). The second undistorted plane is denoted by K2 . The direc-tion of shear is the ﬁrst characteristic direction, η1 . The second characteristic direction,η2 , lies in K2 and is perpendicular to the intersection of K1 and K2 . The plane containingη1 , η2 , and the normals to K1 and K2 is the plane of shear. Table 11.1 gives the twinningelements reported for twins in several metals. η2 η2 K2Figure 11.2. Homogeneously sheared hemisphere.The two undistorted planes are K1 and K2 . The sheardirection is η1 . The second characteristic direction, K1η2 , is the direction in K2 that is perpendicular to theintersection of K1 and K2 . From W. F. Hosford, ibid. η1
- 190. 172 MECHANICAL BEHAVIOR OF MATERIALSTable 11.1. Twinning elements for simple twinsStructure K1 K2 η1 η2fcc & dia. cubic {111} {111} <112> <112>bcc {112} {112} <111> <111>hcp {1012} {1012} <1011> <1011>Twinning shearFor the twins listed in Table 11.1, K 2 and η2 have the same forms as K 1 and η1 . In thesecases, twinning can be regarded as a shear creating a mirror image in an orthorhombic cell,as shown in Figure 11.3. This simple form of twinning can be analyzed as follows: Let thetwinning plane, K 1 , be (011) and the twinning direction, η1 , be [011]. In Figure 11.3, theshears are projected onto the (100) plane. When the upper left hand portion of the crystalundergoes the twinning shear, point A moves to a new position, E. The shear strain, γ , isdeﬁned as AE/EF. The length, EF, can be related to w and to h by noting that the triangleEFB is similar to triangle DCB, so that EF/DC = EB/DB. Substituting w = DC, h = √ √EB = BC, and DB = w2 + h2 , EF = wh/ w2 + h2 . Since triangle EFB is similar to √triangle DCB,√ FB/EB = BC/DC, so the length FB = h2/ w2 + h2 . Therefore, AE = √ √DB − 2FB = w2 + h2 − 2h2/ w2 + h2 . Substituting, γ = AE/EF = [( w2 + h2 ) − √ √2(h2/ w2 + h2 }/[wh/ w2 + h2 ]. Simplifying, γ = w/h − h/w. (11.1) If the center of the cell (point H in Figure 11.4) is connected to points A and E asshown in Figure 11.4, it is clear that line HA in the parent is equivalent to line HE in thetwin. Therefore, K2 = (011) and η2 = [011]. The angle of reorientation, θ, of the [010]direction and (001) plane is given by tan(θ/2) = h/w. (11.2)Figure 11.3. Sketch of a simple orthorhombic cell undergoing twinning. The shear strain is AE/AG.
- 191. MECHANICAL TWINNING AND MARTENSITIC SHEAR 173 η′2 [010]′ E η2 = [011]Figure 11.4. Determination of the reorientation an- Agle, θ, of the [010] direction and the twinning ele- K′ 2ments, K1 and K2 . H h K2 = (011) θ w [010]Table 11.2 gives the values of h and w in Equations (11.1) and (11.2) for several crystalstructures.Twinning in fcc metalsTwinning in fcc metals occurs on K1 = {111} planes in η1 = <112> directions.The atomic movements are shown in Figures 11.5 and 11.6. It is clear that K2 ={111} and η2 = <112>. The shear strain can be calculated √ √ √ √ from Equation (11.1) bysubstituting w = a 2 and h = a, γ = a 2/a − a/(a 2) = 2/2 = 0.707. The angleof reorientation of the [001] direction is, from Equation (11.2), θ = 2 arctan(h/w) = √2 arctan(1/ 2) = 70.5◦ .Twinning in bcc metalsFigure 11.7 is a plan view of the (110) plane in a bcc metal. The upper right half has √undergone twinning shear on the (112)[111] system. The shear strain is γ = 2/2 andproduces a tensile elongation parallel to [001]. Thus the deformation is equal in magnitudeto that in fcc twinning, but of the opposite sign. There is another important difference,however. In fcc crystals, all the nearest neighbor distances near a twin boundary arecorrect, so that every atom near the boundary has 12 near neighbors at the same dis-tance. In bcc some near-neighbor distances between atoms near the boundary are notcorrect.Table 11.2. Values of h, w, andCrystal structure h w γ √ √fcc and dia. cubic a a√ 2 2/2 √bcc a a/ 2 √ 2/2 √ √hcp c a 3 c/( 3a) − 3a/c
- 192. 174 MECHANICAL BEHAVIOR OF MATERIALS Figure 11.5. Atomic displacement in {111} <112> twinning of fcc metals. Example problem 11.1: The distance AG in Figure 11.7C is a little smaller than the normal interatomic distance (for example AF) as shown in Figure 11.7C. By what percentage is this distance too small? SOLUTION: Consider the atom at A. The nearest neighbors at B and C (two each) √ and at D, E, and F (one each) are at the correct distance from A (i.e., a 3/2). However, the atom at G is not at exactly the correct distance. The distance AG can be found by realizing that AG = 2AH and that triangle AHQ is similar to triangle CAQ, so AH/AC = AQ/QC. Therefore AH = AC × AQ/QC = √ √ √ √ √ (a/2)(a/ 2)/[(a/2)2 + (a/ 2)2 ]1/2 = [a2 /(2 2)]/[a 1/4 + 1/2] = a/ 6. The dis- √ tance AG = 2AH = 2a/ 6 =√ 0.8165a. When this is compared with the correct “near-neighbor” distance of a 3/2 = 0.8662a, there is a difference of (0.8165 − 0.8662)/0.8662 = 0.0574 or 5.7%. [001] – [112] (111) – K1 =(111) K2 =(111), η2 =[112] [010] – η1 = [112] [100] – a (110) planes a / √2Figure 11.6. Plan view of {111} <112> twinning in fcc crystals. The atom positions are projected onto theshear plane, (110). From W. F. Hosford, ibid.
- 193. MECHANICAL TWINNING AND MARTENSITIC SHEAR 175 – [001] – [1 11] [1 11] – B.( 112) – (112)A. G F C [100] [010] A a D B E C. G F C √ 2a a/2 H A Q a/ √ 2Figure 11.7. (A) Plan view of the (110) plane in a bcc crystal showing twinning on the (112)[111] system in theupper right half of the ﬁgure. The atoms in several unit cells are indicated. Those in one (110) plane are shown assquares, where as those one plane forward and one plane back are indicated by circles. (B) Perspective sketchshowing the twinning elements. (C) Nearest neighbor distances. The distance between A and G is too small.(See Example Problem 11.1.) From W. F. Hosford, ibid.Twinning in hcp metalsTwinning in hcp metals is in contrast to the cubic metals (both fcc and bcc) in which slipcan produce any shape change. Therefore, twinning is much more important in the hcpmetals than in the cubic metals. The number of slip systems in the hcp metals is limited.All the easy slip <1120> directions are perpendicular to the c-axis and therefore slipdoes not produce any elongation or shortening parallel to the c-axis. The most common twinning system in hcp metals is {1012}<1011>. This is a simplemode of the form in Figure 11.3 and Equations (11.1) and (11.2). Figure 11.8 showsthat the direction of shear associated with this twinning system depends on the c/a ratio. c – (10 12) – [ 1011] c c ca1a3 a√ 3 a√ 3 a√ 3 a2 A B C √Figure 11.8. (A) Perspective sketch showing {1012} <1011> twinning in hcp crystals. (B) For c/a < 3,√ thedirection of shear is [1011] and twinning will occur under tension parallel to the c-axis. (C) For c/a > 3,the direction of shear is [1011] and twinning will occur under compression parallel to the c-axis. From W. F.Hosford, ibid.
- 194. 176 MECHANICAL BEHAVIOR OF MATERIALSTable 11.3. The c/a ratios of various hcp metalsMetal c (nm) a (nm) c/aBe 0.3584 0.2286 1.568Cd 0.5617 0.2979 1.886Hf 0.5042 0.3188 1.582Mg 0.5210 0.3209 1.624Ti 0.4683 0.2590 1.587Zn 0.4947 0.2665 1.856Zr 0.5148 0.3231 1.593 √spherical atoms 8/3 = 1.633These are given in Table 11.3 for a number of hcp metals. Only zinc and cadmium √have c/a ratios greater than 3. Therefore only these metals twin when compressionis applied parallel √ the c-axis (or tensile stresses perpendicular to it). For all the other tohcp metals c/a < 3, so twins are formed by tensile stresses parallel to the c-axis (orcompressive stresses perpendicular to it). It has been found that the frequency of twinsin Cd–Mg solid solution alloys decreases as the composition approaches that for which √c/a = 3. Example problem 11.2: Consider the anisotropic yield locus of a titanium sheet with a texture such that the c-axis is nearly but not completely aligned with the sheet normal. Will {1012} <1011> twinning occur in tension or in compression in the plane of the sheet? Considering your answer to A, sketch the shape of the yield locus, taking into account the possibility of yielding by slip on the prism and pyramidal planes as well as of twinning. sy X slip Figure 11.9. Sketch of the yield locus for a tex- √ -X X ¯ tured hcp metal with c/a < 3. From W. F. Hosford - sx sx and W. A. Backofen in Fundamentals of Deforma- tion Processing, Syracuse Univ. Press, 1964. twinning -X - sy √ SOLUTION: The c/a ratio for titanium is less than 3, so titanium will twin in compres- sion but not in tension perpendicular to the c-axis. Slip will cause little thinning of the sheet since the <1120> slip directions are nearly parallel to the plane of the sheet. If only slip occurred, the yield locus would be approximated by an ellipse, elongated into the ﬁrst and third quadrants. The {1012} <1011> twinning mode under compression will foreshorten the elongation into the third quadrant as shown in Figure 11.9.
- 195. MECHANICAL TWINNING AND MARTENSITIC SHEAR 177 c – –( 12 10)planes c a1 -a 3 a√ 3 a2Figure 11.10. A plan view of the (12 10) plane of showing the atom positions on two adjacent (12 10) planes.From W. F. Hosford, The Mechanics of Crystals and Textured Polycrystals, Oxford Univ. Press., 1993. The atomic motions in twinning of the hcp lattice are very complex because the atomsdo not all move in the direction of shear. Figure 11.10 shows the atom positions on adjacent √(12 10) planes of a hypothetical hcp metal with a c/a ratio of (11/12) 3 = 1.588. Theatom motions are shown in Figure 11.11. Different atoms move different distance andthere are components of motion toward and away from the mirror plane. These atomicmovements have been described as a shear plus a shufﬂe. There are other twinning modes for hcp metals that are not the simple type describedby Equations (11.1) and (11.2) and illustrated in Figure 11.3. Some of these are listed inTable 11.4. The twin planes are shown in Figure 11.12. The twinning shear strains forthe various modes depend on the c/a ratio as shown in Figure 11.13 but only change signfor {1012} <1011>.Figure 11.11. The atom movements on two adjacent (12 10) planes during (1012) twinning. Note that theshear is not homogeneous. Some atoms move toward the twinning plane and some away from it. From W. F.Hosford, ibid.
- 196. 178 MECHANICAL BEHAVIOR OF MATERIALSTable 11.4. Other twinning elements in hcp metals.Metal K1 K2 η1 η2 γMg {1011} {1013} <1012> <3032> √ √Mg {1013} {1011} <3032> <1012> c/( 3a) − (3/4) 3a/cZr, Ti {1121} (0001) <1126> <1120> a/cZr, Ti {1122} {1124} <1123> <224 3> (2/3)[c/a − 2a/c] = {1124} {1122} 0.224 Zr, for 0.218 for TiShapes of twinsDeformation twins are generally lenticular (lens-shaped), as shown in Figure 11.14A.This is in contrast to twins that are formed during recrystallization. Annealing twins arebounded by almost perfectly ﬂat planes parallel to K1 , as shown in Figure 11.14B. Becausedeformation twins are lenticular, the boundaries between the twinned and untwinnedregions do not coincide exactly with the twinning plane (K1 ). The central plane is,however, approximately parallel to K1 . In fcc and bcc metals, twins are very narrowand usually look like parallel lines. In contrast, {1012} <1011> twins in hcp metalsare relatively fat. The shape of the deformation twins is probably related to the overallenergy change as a twin forms. There are two main contributions to this overall energychange. One is from the introduction of new surface (the twin boundary), which has asurface energy. The other is the strain energy that results when one portion of material(the twinned region) undergoes a plastic shear while the surrounding material does not.There is a mismatch between the twins and the matrix that must be accommodated byelastic distortion of the parent and/or slip in the parent. This accommodation is minimizedwhen the twins are long and narrow. In other words, the accommodation energy is lowwhen the aspect ratio (ratio of length to thickness) of the twin is very large. On the otherhand, the surface energy is minimized for a given volume of twin when the aspect ratioapproaches unity (a spherical shape). For twins with a high shear strain the strain energyterm should predominate, so that high aspect ratio would be expected. In contrast, a highinterfacial energy promotes fat twins. – –– –– – (10 12) (2 1 11) (2 1 12) (10 11) Figu

Be the first to comment